This compact undergraduate textbook provides a concise yet thorough introduction to the fundamentals of solid-state phys

*1,046*
*218*
*7MB*

*English*
*Pages 254*
*Year 2019*

*Table of contents : Preface to the Third Edition......Page 6Preface to the Second Edition......Page 7Preface to the First Edition......Page 8Contents......Page 10Mathematical Symbols......Page 13Abstract......Page 16Abstract......Page 292.1 Diffraction Theory......Page 342.2 Reciprocal Lattice, Brillouin Zones......Page 372.3 Types of Bonding......Page 42Abstract......Page 483.1 Quantum Theory: Max Planck and Albert Einstein......Page 493.2 Specific Heat of the Crystal Lattice, Phonon Spectrum......Page 513.3 Thermal Conductivity of the Crystal Lattice......Page 573.4 Ballistic Phonons......Page 58Abstract......Page 614.1 Approximation with Bound Electrons (Felix Bloch)......Page 634.2 Nearly-Free Electron Approximation (Rudolf Peierls)......Page 675.1 Drude-Lorentz Model......Page 705.2 Quantum Statistics, Fermi Distribution......Page 735.3 Fermi Surface......Page 755.4 Bloch-Grüneisen Law......Page 775.5 Thermoelectricity......Page 79Abstract......Page 846.1 Intrinsic Semiconductors......Page 866.2 Doped Semiconductors......Page 906.3 Excitons and Electron-Hole Droplets......Page 926.4 Metal-Semiconductor Contact, P-N Junction......Page 936.5 Transistor......Page 976.6 Photovoltaics, LED, Semiconductor Laser......Page 1006.7 Miniaturization, Planar Technology......Page 1026.8 Thermoelectricity, Peltier Cooling......Page 104Abstract......Page 1087.1 Hall Effect......Page 1097.2 Magneto-Resistance......Page 1117.3 Landau Theory, Landau Cylinders, de Haas–van Alphen Effect......Page 1127.4 Integer Quantum Hall Effect......Page 1187.5 Fractional Quantum Hall Effect......Page 1237.6 Generation of High Magnetic Fields......Page 126Abstract......Page 1288.1 Meissner Effect, Magnetic Penetration Depth, London Theory......Page 1318.2 Type-II Superconductors......Page 1408.3 Magnetic Flux Quantum......Page 1428.4 BCS Theory, Energy Gap......Page 1468.5 Josephson Effect......Page 1488.6 Motion of the Magnetic Flux Quanta......Page 1528.7 Technical Applications......Page 1559.1 Cuprate Superconductors......Page 1619.2 Symmetry of the Wave Function......Page 1689.3 Grain Boundaries......Page 1709.4 Intrinsic Josephson Junction......Page 1739.5 More New Superconductors: MgB2, Iron Pnictides......Page 1749.6 Technical Applications......Page 176Abstract......Page 17810.1 Diamagnetism......Page 17910.2 Paramagnetism......Page 18010.3 Ferromagnetism......Page 18310.4 Spin Waves......Page 18810.5 Antiferromagnetism......Page 19010.6 Technical Applications, Giant Magneto-Resistance, Spintronics......Page 192Abstract......Page 19711.1 Superlattices, Bloch Oscillations......Page 19811.2 Mesoscopic Regime, Ballistic Electron Transport, Quantized Conductance Value......Page 20311.3 Bottom up, Fullerenes......Page 20811.4 Graphene......Page 21211.5 Quantum Dots......Page 21311.6 Topological Insulators, Metals, and Semimetals......Page 21511.7 Aharonov-Bohm Effect......Page 218Abstract......Page 22012.2 Vacancies in the Crystal Lattice......Page 22112.3 Materials Science of Radiation Damage......Page 22612.4 Mechanical Strength of Materials......Page 22712.5 Dislocations......Page 22912.6 Materials Testing......Page 23212.7 Magnetic Impurities, Kondo Effect......Page 233Nobel Prizes in Physics Closely Connected with the Physics of Solids......Page 236Nobel Prizes in Chemistry Closely Connected with the Physics of Solids......Page 240Semiconductors......Page 242Special Subjects......Page 243Author Index......Page 245Subject Index......Page 249*

Undergraduate Lecture Notes in Physics

Rudolf P. Huebener

Conductors, Semiconductors, Superconductors An Introduction to Solid-State Physics Third Edition

Undergraduate Lecture Notes in Physics

Undergraduate Lecture Notes in Physics (ULNP) publishes authoritative texts covering topics throughout pure and applied physics. Each title in the series is suitable as a basis for undergraduate instruction, typically containing practice problems, worked examples, chapter summaries, and suggestions for further reading. ULNP titles must provide at least one of the following: • An exceptionally clear and concise treatment of a standard undergraduate subject. • A solid undergraduate-level introduction to a graduate, advanced, or non-standard subject. • A novel perspective or an unusual approach to teaching a subject. ULNP especially encourages new, original, and idiosyncratic approaches to physics teaching at the undergraduate level. The purpose of ULNP is to provide intriguing, absorbing books that will continue to be the reader’s preferred reference throughout their academic career. Series Editors Neil Ashby University of Colorado, Boulder, CO, USA William Brantley Department of Physics, Furman University, Greenville, SC, USA Matthew Deady Physics Program, Bard College, Annandale-on-Hudson, NY, USA Michael Fowler Department of Physics, University of Virginia, Charlottesville, VA, USA Morten Hjorth-Jensen Department of Physics, University of Oslo, Oslo, Norway Michael Inglis Department of Physical Sciences, SUNY Suffolk County Community College, Selden, NY, USA

More information about this series at http://www.springer.com/series/8917

Rudolf P. Huebener

Conductors, Semiconductors, Superconductors An Introduction to Solid-State Physics Third Edition

123

Rudolf P. Huebener Physikalisches Institut University of Tübingen Tübingen, Germany

ISSN 2192-4791 ISSN 2192-4805 (electronic) Undergraduate Lecture Notes in Physics ISBN 978-3-030-31419-4 ISBN 978-3-030-31420-0 (eBook) https://doi.org/10.1007/978-3-030-31420-0 This book was originally published in German by Spektrum Verlag, 2013. Original title: “Leiter, Halbleiter, Supraleiter: Eine Einführung in die Festkörperphysik”. 1st & 2nd editions: © Springer International Publishing Switzerland 2015, 2016 3rd edition: © Springer Nature Switzerland AG 2019 This work is subject to copyright. All rights are reserved by the Publisher, whether the whole or part of the material is concerned, speciﬁcally the rights of translation, reprinting, reuse of illustrations, recitation, broadcasting, reproduction on microﬁlms or in any other physical way, and transmission or information storage and retrieval, electronic adaptation, computer software, or by similar or dissimilar methodology now known or hereafter developed. The use of general descriptive names, registered names, trademarks, service marks, etc. in this publication does not imply, even in the absence of a speciﬁc statement, that such names are exempt from the relevant protective laws and regulations and therefore free for general use. The publisher, the authors and the editors are safe to assume that the advice and information in this book are believed to be true and accurate at the date of publication. Neither the publisher nor the authors or the editors give a warranty, expressed or implied, with respect to the material contained herein or for any errors or omissions that may have been made. The publisher remains neutral with regard to jurisdictional claims in published maps and institutional afﬁliations. This Springer imprint is published by the registered company Springer Nature Switzerland AG The registered company address is: Gewerbestrasse 11, 6330 Cham, Switzerland

Preface to the Third Edition

The third edition is a reprint of the second edition with a series of minor extensions. Because of the strong recent experimental and theoretical research activities in the ﬁeld of topological materials, Sect. 11.6 has been extended considerably. The author is grateful to Zachary Evenson from the Springer editorial ofﬁce for his effective support. Tübingen, Germany

Rudolf P. Huebener

v

Preface to the Second Edition

The second edition is an extended reprint of the ﬁrst edition. In many chapters, a more detailed mathematical treatment of the various subjects is given. A section dealing with magnetic impurities and the Kondo effect has been added. The author is grateful to Silvia Haindl and to Vladimir Kresin for detailed suggestions about expanding the book. Tübingen

Rudolf P. Huebener

vii

Preface to the First Edition

Only a few scientiﬁc-technical developments from the last century have affected our lives in such a powerful way as the spectacular advances in our knowledge of the electronic properties of solids. Many of the present achievements are intimately connected with these advances. To name only a few: the transistor and its extreme miniaturization in microelectronics, the electronic processing of data and highly developed and powerful computers, the mobile telephone and satellite communication, television and entertainment electronics, as well as numerous instruments and systems of medical technology. In the ﬁnal analysis, the theater of all these events of dramatic progress is the world of electrons in crystals, where the (quantized) vibrations of the crystal lattice continuously demonstrate their influence. The revolutionary advances in knowledge are due to many individual people. Frequently a true paradigm change has been necessary in order to arrange and order the new perceptions properly. Hence, it is not surprising that, as a rule, the pioneers of these new ideas initially had to overcome great difﬁculties and rejection, before the new concepts slowly gained acceptance. Also, in certain cases, highly focused research in large industrial laboratories turned out to be the key to success. This is impressively illustrated in particular by the invention of the transistor in the American Bell Laboratories. This book represents an updated and strongly extended edition of the book published by the same author nearly 10 years ago with the title Electrons in Action. In particular, the physical contents were pointed out more clearly by mathematically formulating the fundamentals. The book is aiming at students of the natural sciences, and in particular of physics and materials science, as well as at engineers, as an introduction to solid-state physics. It may serve as a motivating pre-stage and companion of the established and very detailed textbooks.

ix

x

Preface to the First Edition

In addition to the physical contents, the book treats the important role played by many famous and often still very young scientists. The fundamental developments are supplemented by describing their scientiﬁc and historic environment. Marius Orlowski, Virginia Polytechnic Institute, provided important advice. Tübingen May 2014

Rudolf P. Huebener

Contents

1

1

Spectacular Advances . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

2

Well 2.1 2.2 2.3

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

15 20 23 28

3

Permanent Movement in the Crystal Lattice . . . . . . . . . . . 3.1 Quantum Theory: Max Planck and Albert Einstein . . . 3.2 Speciﬁc Heat of the Crystal Lattice, Phonon Spectrum 3.3 Thermal Conductivity of the Crystal Lattice . . . . . . . . 3.4 Ballistic Phonons . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . .

. . . . .

. . . . .

. . . . .

. . . . .

. . . . .

. . . . .

35 36 38 44 45

4

Electric Conductor or Insulator?—Energy Bands . . . . . . . . . . . . . . 4.1 Approximation with Bound Electrons (Felix Bloch) . . . . . . . . . 4.2 Nearly-Free Electron Approximation (Rudolf Peierls) . . . . . . . .

49 51 55

5

Metals Obey the Rules of Quantum Statistics 5.1 Drude-Lorentz Model . . . . . . . . . . . . . . 5.2 Quantum Statistics, Fermi Distribution . . 5.3 Fermi Surface . . . . . . . . . . . . . . . . . . . . 5.4 Bloch-Grüneisen Law . . . . . . . . . . . . . . 5.5 Thermoelectricity . . . . . . . . . . . . . . . . .

6

Less 6.1 6.2 6.3 6.4 6.5

Ordered Lattice Structures in Crystals . Diffraction Theory . . . . . . . . . . . . . . . . Reciprocal Lattice, Brillouin Zones . . . . Types of Bonding . . . . . . . . . . . . . . . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . . . .

. . . . . .

. . . . . .

. . . . . .

. . . . . .

. . . . . .

. . . . . .

. . . . . .

. . . . . .

. . . . . .

. . . . . .

. . . . . .

. . . . . .

. . . . . .

. . . . . .

59 59 62 64 66 68

Can Be More: Semiconductors . . . . . . . . . . Intrinsic Semiconductors . . . . . . . . . . . . . . . Doped Semiconductors . . . . . . . . . . . . . . . . Excitons and Electron-Hole Droplets . . . . . . Metal-Semiconductor Contact, P-N Junction . Transistor . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . .

. . . . . .

. . . . . .

. . . . . .

. . . . . .

. . . . . .

. . . . . .

. . . . . .

. . . . . .

. . . . . .

. . . . . .

. . . . . .

. . . . . .

. . . . . .

73 75 79 81 82 86

. . . . . .

. . . . . .

xi

xii

Contents

6.6 6.7 6.8 7

8

9

Photovoltaics, LED, Semiconductor Laser . . . . . . . . . . . . . . . . Miniaturization, Planar Technology . . . . . . . . . . . . . . . . . . . . . Thermoelectricity, Peltier Cooling . . . . . . . . . . . . . . . . . . . . . .

Circling Electrons in High Magnetic Fields . . . . . . . . 7.1 Hall Effect . . . . . . . . . . . . . . . . . . . . . . . . . . . . 7.2 Magneto-Resistance . . . . . . . . . . . . . . . . . . . . . 7.3 Landau Theory, Landau Cylinders, de Haas–van Alphen Effect . . . . . . . . . . . . . . . . . . . . . . . . . . 7.4 Integer Quantum Hall Effect . . . . . . . . . . . . . . . 7.5 Fractional Quantum Hall Effect . . . . . . . . . . . . . 7.6 Generation of High Magnetic Fields . . . . . . . . .

89 91 93

........... 97 ........... 98 . . . . . . . . . . . 100 . . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

101 107 112 115

. . . . . . . 117

The Winner: Superconductors . . . . . . . . . . . . . . . . . . . . . 8.1 Meissner Effect, Magnetic Penetration Depth, London Theory . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 8.2 Type-II Superconductors . . . . . . . . . . . . . . . . . . . . . . 8.3 Magnetic Flux Quantum . . . . . . . . . . . . . . . . . . . . . . 8.4 BCS Theory, Energy Gap . . . . . . . . . . . . . . . . . . . . . 8.5 Josephson Effect . . . . . . . . . . . . . . . . . . . . . . . . . . . . 8.6 Motion of the Magnetic Flux Quanta . . . . . . . . . . . . . 8.7 Technical Applications . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . .

. . . . . . .

. . . . . . .

. . . . . . .

. . . . . . .

. . . . . . .

. . . . . . .

120 129 131 135 137 141 144

The Big Surprise: High-Temperature Superconductivity 9.1 Cuprate Superconductors . . . . . . . . . . . . . . . . . . . . . 9.2 Symmetry of the Wave Function . . . . . . . . . . . . . . . 9.3 Grain Boundaries . . . . . . . . . . . . . . . . . . . . . . . . . . 9.4 Intrinsic Josephson Junction . . . . . . . . . . . . . . . . . . 9.5 More New Superconductors: MgB2, Iron Pnictides . . 9.6 Technical Applications . . . . . . . . . . . . . . . . . . . . . .

. . . . . . .

. . . . . . .

. . . . . . .

. . . . . . .

. . . . . . .

. . . . . . .

. . . . . . .

. . . . . . .

151 151 158 160 163 164 166

. . . . . .

. . . . . .

. . . . . .

. . . . . .

. . . . . .

. . . . . .

. . . . . .

. . . . . .

169 170 171 174 179 181

10 Magnetism: Order Among the Elementary Magnets . . . 10.1 Diamagnetism . . . . . . . . . . . . . . . . . . . . . . . . . . . . 10.2 Paramagnetism . . . . . . . . . . . . . . . . . . . . . . . . . . . 10.3 Ferromagnetism . . . . . . . . . . . . . . . . . . . . . . . . . . 10.4 Spin Waves . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 10.5 Antiferromagnetism . . . . . . . . . . . . . . . . . . . . . . . . 10.6 Technical Applications, Giant Magneto-Resistance, Spintronics . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . .

. . . . . . . . . 183

11 Nanostructures: Superlattices, Quantum Wires, and Quantum Dots . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 189 11.1 Superlattices, Bloch Oscillations . . . . . . . . . . . . . . . . . . . . . . . 190 11.2 Mesoscopic Regime, Ballistic Electron Transport, Quantized Conductance Value . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 195

Contents

11.3 11.4 11.5 11.6 11.7

xiii

Bottom up, Fullerenes . . . . . . . . . . . . . . . . . . . Graphene . . . . . . . . . . . . . . . . . . . . . . . . . . . . Quantum Dots . . . . . . . . . . . . . . . . . . . . . . . . Topological Insulators, Metals, and Semimetals Aharonov-Bohm Effect . . . . . . . . . . . . . . . . . .

. . . . .

. . . . .

. . . . .

. . . . .

. . . . .

. . . . .

. . . . .

. . . . .

. . . . .

. . . . .

. . . . .

. . . . .

200 204 205 207 210

12 Defects in the Crystal Lattice: Useful or Harmful? . 12.1 Disorder at Thermodynamic Equilibrium . . . . . 12.2 Vacancies in the Crystal Lattice . . . . . . . . . . . . 12.3 Materials Science of Radiation Damage . . . . . . 12.4 Mechanical Strength of Materials . . . . . . . . . . . 12.5 Dislocations . . . . . . . . . . . . . . . . . . . . . . . . . . 12.6 Materials Testing . . . . . . . . . . . . . . . . . . . . . . 12.7 Magnetic Impurities, Kondo Effect . . . . . . . . . .

. . . . . . . .

. . . . . . . .

. . . . . . . .

. . . . . . . .

. . . . . . . .

. . . . . . . .

. . . . . . . .

. . . . . . . .

. . . . . . . .

. . . . . . . .

. . . . . . . .

. . . . . . . .

213 214 214 219 220 222 225 226

Nobel Prizes in Physics Closely Connected with the Physics of Solids . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 229 Nobel Prizes in Chemistry Closely Connected with the Physics of Solids . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 233 Bibliography . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 235 Author Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 239 Subject Index. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 243

Mathematical Symbols

a e f fL h h ħ j js k k kZ kF kB ‘ m mh mc n ns p r r t vD vF z mA mg nm

Distance between the neighboring atoms or building blocks of the crystal lattice Electric elementary charge Spring constant Lorentz force Hour Planck’s constant h/2p Electrical current density Supercurrent density Wave number = 2p=k Wave vector = kX + kY + kZ Component of the wave vector in z-direction Fermi wave vector Boltzmann’s constant Mean free path me = Electron mass Mass of the holes Cyclotron mass of the electrons Electron concentration Density of the superconducting electrons Hole concentration Lattice vector Electron coordinate Time Drift velocity Fermi velocity Figure of merit Milliampère Milligram Nanometer = 10–9 Meter xv

xvi

µm eV A B CV D2 De E F E G G Go GeV GHz H HC HC HC1 HC2 I Ir Ig IC J K K L L M N R RH S S Sm T TC TD TCU THz U U V V

Mathematical Symbols

Micrometer = 10–6 Meter Electron volt (energy unit) Vector potential Magnetic flux density Speciﬁc heat at constant volume Density of states in the two-dimensional case Density of states per volume Energy Free energy Electric ﬁeld Vector in the reciprocal lattice Density of the Gibbs free energy Quantized unit of the electrical conductance Giga-electron volt = 109 eV Giga-Hertz = 109 per second Magnetic ﬁeld Critical magnetic ﬁeld of a superconductor Coercive ﬁeld Lower critical magnetic ﬁeld of a superconductor Upper critical magnetic ﬁeld of a superconductor Electrical current Recombination current Generation current Critical electrical current density of a superconductor Exchange integral Kelvin Wave vector of the phonons Lorenz number Orbital angular momentum Magnetization Number of the crystal atoms Electrical resistance Hall constant Seebeck coefﬁcient Spin angular momentum Mixing entropy Temperature Critical temperature of a superconductor Debye temperature = hmD =kB Curie temperature Tera-Hertz = 1012 per second Total vibrational energy of a crystal Inner energy Electrical voltage Volume

Mathematical Symbols

a a d j je jG h e eF k km µ µo µB η x xB xc xD xL m mc mD mE v vp s n q qf r u uo u0 w П

Polarizability Madelung constant Scattering angle Heat conductivity Heat conductivity of the electrons Heat conductivity of the crystal lattice Debye temperature Electron energy Fermi energy Wavelength Magnetic penetration depth of superconductors Magnetic moment Permeability of vacuum Bohr magneton Damping coefﬁcient of the motion of magnetic flux quanta Angular frequency Bloch frequency Cyclotron angular frequency Debye angular frequency Larmor frequency Frequency xc/2p = Cyclotron frequency xD/2p = Debye frequency Einstein frequency Magnetic susceptibility Paramagnetic susceptibility Mean collision time Coherence length of a superconductor Lattice vector Flux-flow resistivity Electrical conductivity Phase of a wave function Magnetic flux quantum Atomic wave function Wave function of the superconducting Cooper pairs Peltier coefﬁcient

xvii

Chapter 1

Spectacular Advances

Abstract During the second half of the last century solid state physics and materials science experienced a great advance and established itself as an important and independent new ﬁeld. In addition to X-ray diffraction, new analytical tools such as neutron diffraction, electron microscopy, different versions of mechanical scanning techniques, and scanning electron and laser microscopy became available. Material fatigue, radiation damage, and the preparation of single crystals developed into important subjects. The invention of the transistor represented perhaps the ultimate highlight.

During the second half of the last century the physics of solids has experienced a tremendous growth, for which many important basic steps had already been prepared during the ﬁrst half of the century. An early decisive impulse for these developments came from the discovery of X-rays in 1895 in Würzburg, Germany, by Wilhelm Conrad Röntgen. Soon afterwards, this discovery lead to the ﬁrst observation of X-ray diffraction in crystals by Max von Laue in 1912 in Munich. William Henry Bragg, Professor in Leeds, England, together with his son William Lawrence Bragg at the early age of only 22 years, then started the systematic analysis of crystal structures by means of X-ray diffraction. Today, research dealing with the physics of solids has an impressively wide scope, if for no other reason than the fact that solids are always needed to fabricate useful or nice things, in contrast to the totally different role of liquids and gases. The exact knowledge of the physical properties of the materials that we use today becomes more and more important the further we advance in the ﬁeld of high technology. The large effort of research and development within the area of solid state physics becomes obvious if one looks at the program books for the relevant annual meetings of, say, the German Physical Society (DPG) or the American Physical Society (APS) which recently contained up to more than 2000 pages. (Today, these programs of the meetings are distributed mostly electronically). Often, the technological applications provide the key motivation for strong basic research in solid state physics. We illustrate this by the following two examples. On January 10, 1954, an English passenger airplane of the Comet type broke apart at © Springer Nature Switzerland AG 2019 R. P. Huebener, Conductors, Semiconductors, Superconductors, Undergraduate Lecture Notes in Physics, https://doi.org/10.1007/978-3-030-31420-0_1

1

2

1 Spectacular Advances

8200 m altitude in the Mediterranean near the isle of Elba without any prior warning and crashed into the sea. With only 3681 flight hours, the plane was relatively new. The search for the cause of the accident turned out to be extremely difﬁcult, even though people worked feverishly to clarify the cause of the terrible crash. Since the cause of the accident continued to remain unknown, it was ﬁnally concluded that the crash must have been the result of an unfortunate combination of several bad effects. Hence, on March 23, 1954, the grounding order for all airplanes of the same type, immediately issued on the day of the accident, was lifted again. Prior to this, a total of 62 modiﬁcations had been introduced in all Comet airplanes in operation or under construction. In this way it was hoped to exclude any possible cause of the accident (Fig. 1.1). Then a completely unexpected dramatic event happened. On April 8, i.e., only 16 days following the resumption of the regular flight operation, another Comet airplane with only 2704 h of flight operation crashed into the Mediterranean near Naples. Again, at a high altitude of 10 000 m this time, the plane suddenly apparently broke apart. Now the situation became extremely serious. The causes had to be found at the highest level, and all available means had to be utilized. After analysis of the many different possibilities, problems related to what is now called material fatigue, in particular associated with the wings, came to the center of attention. As a consequence, the complete fuselage of an airplane was dumped into a huge tank ﬁlled with water in order to expose it to changing, and in particular to cyclical, mechanical loads. In this way, it was found that, after some time, fatigue effects appeared on the wings. However, the fatigue problems on the fuselage itself were much more severe. Finally, the evidence became clear that the mechanical load during testing caused cracks in the fuselage, and that all the cracks originated at the rectangular corners of the cabin windows. The causes of both plane crashes had been found. However, this event also put to an abrupt end the British leading role in air trafﬁc. (Today a large piece of a side of one

Fig. 1.1 Comet jet-aircraft beginning a test flight after the crash of a plane in the Mediterranean near the isle of Elba. (Photo ullstein bild)

1 Spectacular Advances

3

of the two crashed aircrafts, recovered from the Mediterranean, is on display in the Science Museum in London). Because of these dramatic developments, intensive research activities were begun at the same time at many places. Until then only little was known about the phenomenon of material fatigue, its effect on the mechanical properties of materials, and the mechanisms leading to the development of microcracks. In this context of the material fatigue experienced sixty years ago with the Comet passenger airplane, it is interesting to note that the recent development of the largest passenger airplane, which has ever been constructed, the Airbus A 380, included an extensive and careful mechanical material fatigue testing procedure by means of hydraulic systems, as a critical step. Starting in 2005 the complete A 380 airplane, consisting of the whole fuselage and the wings, has been exposed for 26 months to mechanical loads varying with time and simulating a total number of 47500 flight cycles (take-off and landing). This testing load program corresponds to the 25 year lifetime of the A 380 airplane. As a second example, we recall the possible difﬁculties expected more than 60 years ago during the operation of the inner components of the ﬁrst nuclear reactors. At that time hardly anything was known about the behavior of, say, graphite when it is utilized for slowing down the neutrons which are emitted during nuclear ﬁssion within the reactor. Would it be possible that during their irradiation with the highly energetic neutrons the carbon atoms of the graphite lattice could be ejected out of their regular lattice sites, eventually leading to an energetically highly excited material, releasing abruptly its stored excess energy in an explosion like dynamite? Such problems concerned the scientists involved in the early reactor experiments. The American scientist Eugene Paul Wigner, originally from Hungary (later a Nobel laureate and famous for his theoretical work on mathematical group theory and symmetry principles and their role in atomic, nuclear, and elementary particle physics) was one of the ﬁrst who theoretically analyzed the physical properties of lattice defects and radiation damage in crystals. At that time, a young co-worker of Wigner, Frederick Seitz, performed the ﬁrst theoretical calculations on this subject (Fig. 1.2). Both scientists introduced the concept of the “Wigner-Seitz cell” into solid state physics. Following these initial steps, the ﬁeld of structural lattice defects in crystals has developed into an important subﬁeld of solid state physics, being investigated today in many laboratories. In 1940 Frederick Seitz also published the ﬁrst general textbook on solid state physics: “The Modern Theory of Solids”. An enormously important development took place with respect to microelectronics. Here the physics of solids has resulted in a total paradigm change in electronic technology. It was Mervin Kelly, one of the top-level managers of the famous American Bell Laboratories in Murray Hill in the Federal State of New Jersey, who realized at the end of the Second World War that the old mechanical relays and the evacuated amplifying tube made from glass had to be replaced by something better. To Kelly a highly promising candidate appeared to be the crystal, if it had suitable electric conduction properties. Therefore, at the Bell Laboratories a special group of scientists was organized, which was supposed to explore the

4

1 Spectacular Advances

Fig. 1.2 Eugene P. Wigner (left photo: Deutsches Museum) and Frederick Seitz (right: private photo)

electric conduction properties of solids. At the center of everyone’s attention then stood the semiconductor crystals of germanium and silicon. Already, relatively soon afterwards, an extremely momentous event had been the invention of the transistor by John Bardeen, Walter Brattain, and William Shockley. On December 23, 1947, they demonstrated the transistor for the ﬁrst time to the directors of their company. Subsequently, as a new electronic device, the transistor underwent intensive further development and improvement. Without a doubt, this invention represented the start of the modern age of digital electronics. These big advances in the ﬁeld of solid state physics, of course, were accompanied by similar advances in instrumental techniques and methods. Here we must mention the exploration of the regime of very low temperatures. In 1908 the Dutch scientist Heike Kamerlingh Onnes in Leiden achieved for the ﬁrst time the liquefaction of the noble gas helium. With this success the low-temperature range down to 4 K (−269 °C) became accessible. In this context the most spectacular event was the subsequent discovery of superconductivity by Kamerlingh Onnes in 1911. Until the 1930s, the number of laboratories equipped to perform experiments with liquid helium worldwide could be counted on the ﬁngers of one hand. In contrast, today about 1000 helium liqueﬁers are operating worldwide (Fig. 1.3). Today the largest liquefaction facility is operated at the particle accelerator Large Hadron Collider (LHC) in Geneva. There exist eight liqueﬁers each having a liquefaction rate of 3600 L/h, i.e., with a total rate of 28 800 L/h. Worldwide this corresponds to about 40% of the inventory of large liquefaction facilities for helium. Eventually, the available experimental regime was extended to lower and lower temperatures. In particular, we mention a technique relying on the elementary

1 Spectacular Advances

5

Fig. 1.3 Modern plant for liquefying the noble gas helium. On the left we see the controls and the cold box of the liqueﬁer, on the right the storage vessel for liquid helium. (Photo Linde AG)

atomic magnets of a paramagnetic substance. This technique consists of the following sequence of steps. Initially, a paramagnetic salt pill is precooled to about 1 K, in order to reduce considerably its content of thermal energy. Subsequently, the elementary magnets in the salt pill are all oriented in one direction by a strong magnetic ﬁeld, and simultaneously the heat of magnetization is removed, being deposited in the environment. In the next step, the salt pill is thermally decoupled from its environment. Then the magnetic ﬁeld is turned off. Now the pill is thermally isolated, and the directional disorder of the elementary magnets gradually reappears. As a necessary consequence, the temperature of the salt pill drops at the same time. In this way low temperatures of only a few thousandth Kelvin can be reached. This method of “adiabatic demagnetization” was proposed in 1926 by the Dutch scientist Peter Debye and in 1927 by the American William Francis Giauque. In 1933 the method was demonstrated experimentally for the ﬁrst time. The extended application of this principle to the elementary magnets of the atomic nuclei had already been proposed in 1934 by the Dutch scientist Cornelis Jacobus Gorter and in 1935 by Nicholas Kurti and Franz Eugen Simon from Oxford. The cooling effect due to this nuclear demagnetization was experimentally realized for the ﬁrst time in 1956. Using this technique, extremely low temperatures down to one millionth Kelvin or lower could be reached. However, at such low temperatures it becomes more and more difﬁcult to establish thermal equilibrium between the different components of the solid, namely the electrons and their elementary magnets, the lattice vibrations, and the elementary magnets of the atomic nuclei.

6

1 Spectacular Advances Because of their Jewish origin, Nicholas Kurti and Franz Eugen Simon had to leave Germany in 1933 when Hitler took over the government. Earlier, both had worked ﬁrst in Berlin and then at the Technical University in Breslau (today Wroclaw), and the English scientist Frederick Alexander Lindemann (later Viscount Cherwell) had arranged for a position for both of them at the Clarendon Laboratory in Oxford, England. As director of the Clarendon Laboratory Lindemann has done exactly the same at the time also for the two brothers Fritz and Heinz London, and for Kurt Mendelssohn. After they had left Germany, during subsequent years, all these people distinguished themselves by outstanding contributions to physics at low temperatures, and Oxford gained a top position in this ﬁeld.

An apparatus often used today for reaching temperatures much below 1 K is the mixing cryostat (Fig. 1.4). In this cryostat the two isotopes of the noble gas helium, which differ only by the number of neutrons in their atomic nuclei (3He with a single neutron and 4He with two neutrons), are pumped through several stages of heat exchangers, such that within the mixing chamber located at the coldest end of the instrument an almost pure liquid 3He phase is collected directly above a liquid mixed phase of 3He and 4He. For this technique to operate, the starting temperature must already have been lowered to 1 K by precooling. During operation, 3He atoms from the upper concentrated phase are dissolved continuously in the lower, much more diluted phase. In many ways this scheme resembles a regular evaporation process, in which the upper phase corresponds to the liquid and the lower phase to the vapor. As the ﬁnal result, a continuous cooling of liquid helium is achieved.

Fig. 1.4 Mixing cryostat for cooling down to temperatures well below 1 K. The coldest end with the mixing chamber is located at the bottom. On the top one can see the flange for mounting into the cryogenic container, which can also be evacuated. (Photo Oxford)

1 Spectacular Advances

7

With this apparatus the attached sample to be studied can also be cooled continuously. The lowest temperatures which can be reached are a few thousandth Kelvin. The principle of the mixing cryostat was proposed for the ﬁrst time in 1951 by Heinz London. The ﬁrst prototype was operated in 1965. Together with his brother Fritz London, Heinz London also had proposed an early theory of superconductivity. In addition to the continuing improvements in experimental instruments and to the reﬁnements of measuring techniques, sample preparation and the development of materials also saw much progress. Here an important step was the production of single crystals with extremely high purity. It was such ultra-pure single crystals which allowed the exact determination of many physical properties of materials and the achievement of a theoretical understanding based on these data (Fig. 1.5). The growing of large single crystals starts by dipping a little seed crystal under an inert gas atmosphere into the melt of the same material and then pulling it out again at a slow and well regulated speed. In this way, during solidiﬁcation of the melt, the exact atomic order of the seed crystal will be reproduced. Record sizes of such cylindrical single crystals up to more than one meter in height and nearly half a

Fig. 1.5 Silicon single crystal. (Photo Wacker Chemie AG)

8

1 Spectacular Advances

meter in diameter have been achieved. The concentration of atomic impurities in such a crystal can be reduced further by means of the “zone melting process”. During this process the total cross-section of a short length of the crystal is heated up to the melting temperature by means of, say, eddy current heating, while this heating zone is slowly moved from one end of the crystal to the other. In the resulting temperature gradient the atomic impurities are carried along to one end of the crystal. If necessary, this process can be repeated several times. The impurity concentration of silicon single crystals, routinely achieved today in the semiconductor industry, amounts to only about a single impurity atom within one billion silicon atoms. The spectacular advances in our physical understanding of the microscopic properties of solids were closely coupled to the progress of the instruments and methods available for the analysis of materials. In addition to the investigation of the structure of crystals by means of X-ray diffraction already mentioned, starting in the 1950s the diffraction of neutrons was also utilized more and more for clarifying crystal structures. For this purpose, special nuclear reactors built only for research purposes served as neutron sources. As an example we mention the egg-shaped research reactor (“Atomei”) built in the 1960s at the Technical University of Munich in Garching, Germany (Fig. 1.6). In some sense as a training ground, this reactor then turned out to become the point of origin for the much larger research reactor of the German-French Laue-Langevin Institute in Grenoble. In 2004 the “Atomei” was replaced by the new Research Reactor FRM II (research neutron source Heinz Maier-Leibnitz) in Garching. Similar construction projects for research reactors existed also in other countries with a highly developed industry.

Fig. 1.6 Egg-shaped research reactor (“Atomei”) in Garching near Munich. In the building on the left the new research reactor FRM II, completed in 2004, is located. (Photo Albert Scharger/TU Munich)

1 Spectacular Advances

9

In the same way as often happens with new ideas, the invention of the electron microscope initially had to withstand great difﬁculties and rejection. It all began with two Ph.D. students, namely Ernst Ruska and Bodo von Borries, who had joined the group of Max Knoll at the Chair of High-Voltage Engineering and Electric Plants at the Technical University of Berlin during December 1928 and April 1929, respectively. Here, at ﬁrst both worked on the improvement of the cathode ray oscilloscope. Because of the experience gained, before long they developed the idea that beams of fast electrons can be used for generating a magniﬁed image in a new type of microscope. On March 17, 1932 Ernst Ruska and Bodo von Borries submitted their ﬁrst and basic patents on the future electron microscope. However, a few large hurdles still remained to be overcome. “Why do we need electron microscopes, since we have light microscopes?” was the question that people were asking. However, soon both young scientists had a breakthrough. The Company Siemens & Halske in Berlin agreed to pick up the idea and prepared employment contracts for Bodo von Borries and Ernst Ruska. On December 7, 1937 the ﬁrst electron microscope built by Siemens was demonstrated to the Company directors (Fig. 1.7).

Fig. 1.7 Siemens electron microscope, a precursor of the Siemens Elmiskop 1, marketed in the 1950s. (Photo TU Berlin)

10

1 Spectacular Advances

After only three years of development, in terms of its spatial resolution the electron microscope had outpaced the light microscope. Starting in 1939, an initial series of the Supermicroscope (“Übermikroskop”), as it was called at the time, was offered for sale by Siemens. Again, the underlying basic concept of this microscope is the quantum-mechanical wave character of elementary particles, which had been proposed for the ﬁrst time by the French Louis de Broglie in his dissertation in 1924. The direct experimental proof of the wave nature of electrons was provided subsequently in 1927 by the two Americans Clinton Joseph Davisson and Lester Germer of the Bell Telephone Laboratories who showed that electrons are diffracted by the atomic lattice of crystals. During imaging based on the diffraction of waves, the spatial resolution is always limited by the wavelength. The shorter the wavelength, the correspondingly smaller are the structures that can be spatially resolved. The wavelength of the beam electrons is inversely proportional to the square-root of the accelerating voltage. At an electric voltage of 10 000 volts we have a wave length of k = 1.2 10−2 nm (nm = nanometer = 10−9 m). On the other hand, the wave length of visible light is much larger, k = 400–800 nm, and the achieved spatial resolution is correspondingly much weaker. Already in the 1950s, electron microscopy had celebrated a big success, along with many other successes, by imaging the structural defects in the crystal lattice, as discussed above, and by clarifying the phenomenon of material fatigue. In the latter case the “crystal dislocations” play a central role. They were observed directly for the ﬁrst time in 1956 at the Battelle Institute in Geneva in stainless steel and at the Cavendish Laboratory in Cambridge in aluminum. Eventually, electron microscopes were built for ever increasing accelerating voltages. Today we have instruments with an accelerating voltage of one million volts (Fig. 1.8). For the analysis of materials, beams of fast electrons have also been utilized in another important instrument: the scanning electron microscope. For this, pioneering research was done again in the 1930s by Max Knoll at the Technical University in Berlin, mentioned before, and by Manfred von Ardenne in his Laboratory in Berlin-Lichterfelde. An electron beam collimated down to an extremely small diameter of only 1–10 nm is scanned over the surface of the object to be investigated. Simultaneously, a suitable signal induced by the electron beam in the sample is recorded as a function of the spatial beam coordinates on the sample surface within the scanning window. Correct electronic signal processing then yields a two-dimensional image of the object. To generate the response signal one can use several effects. For example, the emission of secondary electrons due to the beam irradiation is quite often used. However, the beam-induced local change of a sample property such as the electric resistivity can also provide the signal for the image. Today, the signal based on the change in electric resistivity is often utilized for imaging structures in thin layers of semiconductors or superconductors. In the case of superconductors, spatially resolved images relating to their superconductivity can be obtained if the sample is cooled to sufﬁciently low temperatures during scanning with the electron beam.

1 Spectacular Advances

11

Fig. 1.8 Modern electron microscope with an accelerating voltage of one million volts. (Photo A. Tonomura)

Recently, the scanning principle for imaging was extended also to light beams. However, a necessary prerequisite for this was the availability of laser beams with their extremely narrow collimation. Today, laser scanning microscopes are widely used in many ﬁelds. An important milestone during the advances of the methods for the analysis of materials has been the construction of the ﬁrst scanning tunneling microscope by Gerd Binnig and Heinrich Rohrer of the IBM Research Laboratory in Rüschlikon near Zürich, Swizerland. Their ﬁrst patent application dealing with the scanning tunneling microscope was submitted in January 1979. In their instrument the surface to be investigated is mechanically scanned with a tiny metal tip. Using piezoelectric actuators, the metal tip can be moved in three dimensions with

12

1 Spectacular Advances

extremely high sensitivity. During the scanning process the sample surface is approached by the tip as close as about 1 nm. Simultaneously, the quantum-mechanical electric tunneling current is measured running between the tip and the sample surface, if an electric voltage is applied, even though a metallic contact between both does not exist. (The explanation of the effect of quantum mechanical tunneling had been one of the early major successes of the new theory of quantum mechanics). Because of the strong exponential dependence of the tunneling current on the distance between the tip and the sample surface, one can achieve that the tunneling current is limited only by a few or even the last single atom sticking out of the tip. In this way, today one routinely obtains atomic resolution in the lateral direction with this technique (Fig. 1.9). Very recently, even subatomic structures of silicon atoms due to the different electron orbitals, have been observed in the images (Fig. 1.10).

Fig. 1.9 Scanning tunneling microscope. The instrument is mounted on a flange for operation in ultra-high vacuum. (Photo OMICRON Nano Technology)

Fig. 1.10 Image of the individual atoms of a section of 5 nm 5 nm area on the surface of a silicon crystal, generated by means of atomic force microscopy. On the silicon atoms we can see a subatomic structure resulting from the electron orbitals. (Photo F. J. Giessibl)

1 Spectacular Advances

13

Fig. 1.11 The picture shows a ring of iron atoms placed on a copper surface. In this way an artiﬁcial coral reef consisting of 48 iron atoms has been created on an atomic scale. The circular lines appearing within the ring are due the density of the electrons existing within the ring. (Photo Almaden Research Center, 2000)

Soon after the invention of the scanning tunneling microscope, the mechanical scanning principle was extended to several other types of interaction between the probing tip and the sample surface. In particular, we mention the atomic force and the magnetic force microscopes. In the ﬁrst case, the mechanical force between the probing tip and the sample surface is utilized. The second case is based on a magnetic tip probing the magnetic sample properties. In recent years special research effort has been concentrated on the extension of the techniques we have discussed to very low temperatures and to the presence of high magnetic ﬁelds. Today, ease of operation is emphasized by the construction of the instruments. Finally, we point out that most of the techniques for material analysis discussed above are restricted to the sample surface and its immediate neighborhood (Fig. 1.11). In many cases the developments we have outlined were accompanied by the award of the Nobel Prize for Physics and in some cases for Chemistry to the people involved. In order to illustrate this, in the Appendix we have listed all Nobel Laureates who have a close relationship with the physics of solids.

Chapter 2

Well Ordered Lattice Structures in Crystals

Abstract The lattice structure of crystals is characterized by speciﬁc symmetry properties. Translation symmetry yields the 14 Bravais lattices. Rotation, reflection at a mirror plane, and inversion at a point result in the 32 crystallographic point groups. The diffraction of X-rays by a crystal, initiated in 1912 by Max von Laue, represented the ﬁrst experimental proof of the regular lattice structure of a crystal. The elements of diffraction theory, including the reciprocal lattice and Brillouin zones, are explained. The chapter ends with a discussion of quasi-crystals and the different types of bonding.

Crystals have always generated a particular fascination, because of the rich variety of their colors and shapes. While the systematic exploration of nature became increasingly important ever since the 17th century, at the same time the science of rocks and minerals developed into an independent branch and a collecting point for the many different individual observations. The amateur rock collectors and the mineralogists hiking with their tools through the mountains and hills in the early days must be looked upon as important forerunners of the modern scientiﬁc exploration into the properties of solids. The basic geometric crystallographic concepts for describing the large variety of observations also originated within this ﬁeld of mineralogy. In terms of physics, the most important property of crystals is their perfect lattice structure with the regular periodic repetition of exactly the same elementary building blocks in all three spatial dimensions. The elementary building blocks can be atoms or molecules, the latter consisting either of only a few or very many individual atoms. For example, the elementary building blocks of protein crystals contain up to 100 000 atoms. Because of their highly regular periodic lattice structure, crystals always possess a number of prominent symmetry properties. Of particular importance is the “translation symmetry” resulting from the regular periodic lattice conﬁguration of the building blocks in all three spatial dimensions. In a crystal the location of the building blocks of the lattice is described mathematically by the lattice vectors.

© Springer Nature Switzerland AG 2019 R. P. Huebener, Conductors, Semiconductors, Superconductors, Undergraduate Lecture Notes in Physics, https://doi.org/10.1007/978-3-030-31420-0_2

15

16

2 Well Ordered Lattice Structures in Crystals

r ¼ n1 a þ n2 b þ n3 c

ð2:1Þ

Here, n1, n2, and n3 are integers. a, b, and c are the three fundamental translation vectors. Here and in the following we denote vectors by bold symbols. The integer numbers n1, n2, n3 yield the lattice points of the crystal. (In (2.1) we assume, that the origin is located at a lattice point). The translation vectors a, b, c generate the elementary cell (Fig. 2.1), which in turn builds up the crystal lattice by its spatially periodic repetition. Because of this condition of translation symmetry, the possible conﬁgurations of all three-dimensional crystal lattices are highly restricted. As was shown already in 1850 by the Frenchman Auguste Bravais, there are only a total of 14 fundamental types of crystal lattices, which are now referred to as “Bravais lattices” (Fig. 2.2). By selecting the lengths of the three vectors a, b, c of the elementary cell (lattice constants) and the three angles between them, at ﬁrst one obtains seven fundamental types of crystal lattices. If additional lattice points exist at special locations within the elementary cell (in the center of the elementary cell or in the middle of the external surfaces), one obtains a total of 14 translation lattices. In general, the crystal structure is more complex than that of one of the 14 Bravais lattices. However, the crystal lattice is exactly replicated by means of a speciﬁc symmetry operation. In addition to translation, the following fundamental symmetry operations are important: rotation, reflection at a mirror plane, and inversion at a point. In the case of rotation one distinguishes how often the crystal lattice is exactly reproduced during a complete rotation by 2p. Hence, there exist single-, two-, three-, four-, and sixfold rotational axes, corresponding to a rotation by 2p, 2p/2, 2p/3, 2p/4, and 2p/6, respectively. The combination of rotation, reflection at a mirror plane, and inversion speciﬁes one of the 32 crystallographic point groups. By addition of the translation, one of the 230 space groups is obtained, characterizing the crystal structure. Here, mathematical group theory has provided an important input. Johannes Kepler, who was born in 1571 in the Swabian Free City Weil der Stadt near Stuttgart in Württemberg and who later studied at the University of Tübingen, is generally known because of his three famous Kepler’s laws of astronomy. However, among many things he also was concerned with the question, how can space be regularly and completely

Fig. 2.1 Elementary cell deﬁned by the translation vectors a, b, and c

2 Well Ordered Lattice Structures in Crystals

17

cubic

tetragonal

orthorhombic

monoclinic

triclinic

Fig. 2.2 The fourteen Bravais lattices representing all possibilities for the construction of a three-dimensional crystal lattice ﬁlled with the same objects as building elements. So in the early 17th century, i.e., more than 200 years before the considerations of Auguste Bravais, he speculated on the question of why snowflakes always have six corners, but never ﬁve or seven. He showed how the close packing of spheres generates a six-corner pattern. This work of Kepler clearly represents an early signiﬁcant contribution to geometrical crystallography.

Within the crystal lattice, there always exist speciﬁc planes along certain directions, which are closely and perfect periodically packed with atoms or with the

18

2 Well Ordered Lattice Structures in Crystals

elementary building blocks. On the outside of the crystal these planes then represent the extremely smooth and flat surface planes. This fact, together with the existing symmetry properties, is utilized extensively by the jewelry industry during the polishing of precious stones. In snow crystals the large variety of shapes is particularly impressive. Thomas Mann has well described this magniﬁcent appearance of the snowflakes in his novel “The Magic Mountain” (“Der Zauberberg”, here in an English translation): Brilliant clips, medals of decoration, jewelry stars, such as the most accurate jeweler cannot produce in a richer way and with more minute precision…., and among the myriads of magic little stars in their hardly visible, secret little splendor, not meant for the human eye, not a single one was equal to another.

The ﬁrst rigorous experimental proof of the regular lattice structure of crystals was given in 1912 at the University of Munich. Soon after his great discovery of X-rays in Würzburg, Röntgen (Fig. 2.3) had left this location, since he had accepted an offer from the University of Munich. In Munich his group, together with the theoretical physicists at the Chair of Arnold Sommerfeld, concentrated on the problem of clarifying the nature of X-rays. The major question was whether X-rays are just electromagnetic waves such as visible light, but with a much shorter wavelength, or whether they are a new kind of particle radiation. Max von Laue (Fig. 2.4), a young member at the Chair of Sommerfeld, was thinking about diffraction experiments with X-rays. During the time when he was theoretically analyzing the diffraction of X-rays on lattices of points or of bars, he learned from a discussion with Paul Peter Ewald, a Ph.D. student of Sommerfeld, that crystals are Fig. 2.3 Wilhelm Conrad Röntgen (Photo Deutsches Museum)

2 Well Ordered Lattice Structures in Crystals

19

Fig. 2.4 Left: Max von Laue. Right: Set-up of the Laue experiment. On the left we note the X-ray tube and on the right the stage for mounting the crystal. (Photos Deutsches Museum)

likely to consist of a regular lattice arrangement of atoms. Von Laue noted immediately that crystals would be well suited for the diffraction of X-rays, as long as the distance between the atoms in the crystal and the wavelength of the X-rays had a similar magnitude. An initial estimate was encouraging. For the ﬁrst experiments von Laue enlisted the help of Walter Friedrich, who had just been employed by Sommerfeld, and of Paul Knipping, a Ph.D. student of Röntgen, and success did not elude them. On June 8 and July 6, 1912 Sommerfeld was able to present the ﬁrst X-ray diffraction images of a crystal to the Bavarian Academy of Science. This pioneering discovery meant the recognition of two important facts: X-rays are electromagnetic waves, and crystals consist of a three-dimensional regular lattice of atoms (or molecules). For his discovery of X-rays, in 1901 Röntgen had received the ﬁrst Nobel Prize in Physics. His letter to the Royal Bavarian State Ministry for Church and School Matters, in which Röntgen had asked for leave of absence in order to attend the award ceremony in Stockholm, is a highly interesting contemporary document, which we wish to quote at this point. On December 6, 1901 Röntgen wrote (here in English translation): According to a conﬁdential information of the R. Swedish Academy of Science the most respectful and devoted undersigned has been awarded the ﬁrst Nobel Prize for the year 1901. The R. Swedish Academy is particularly keen that the Laureates personally receive the prize in Stockholm on the day of the award (Dec. 10). Since these prizes are of an exceptionally high value and are also highly honourable, the most respectful and devoted undersigned feels that he must follow, though not lightheartedly, the desire of the R. Swedish Academy and, therefore, he is asking for leave of absence for the coming week. Dr. W. C. Röntgen

20

2.1

2 Well Ordered Lattice Structures in Crystals

Diffraction Theory

According to the theory of the diffraction of waves at a point lattice, during wave irradiation, from each lattice point there originates a wave which spherically propagates in all spatial directions (Fig. 2.5). We all know the similar wave propagation which takes place on the surface of water after we have thrown a stone into it. The spherical waves originating from the different lattice points of the crystal superimpose and become enhanced or extinguished. This is referred to as interference. We consider the (elastic) reflection of a wave at a series of parallel lattice planes (Fig. 2.6). We denote the distance between two neighboring lattice planes by a, and the angle between the planes and the direction of the incoming or the outgoing wave by h. The difference of the distance covered by the wave upon the reflection at the two neighboring planes amounts to 2 a sinh. In the case of

Fig. 2.5 a Propagation of a spherical wave originating from a point. The dark rings illustrate the peaks of the wave which follow each other within the spatial distance of one wavelength. The picture corresponds to a snapshot and shows the wave propagation within a plane as, for example, on a water surface. b Interference between two waves such as shown in a, originating from two different centers. From b to d the distance between the two centers increases. In speciﬁc directions the peaks and the valleys of the waves coincide, such that both waves annihilate each other. The positions at which the annihilation takes place, appear closer and closer as the distance between the two centers increases

2.1 Diffraction Theory

21

constructive interference, at which the amplitudes of both waves exactly add to each other, this difference of the distance must be an integer multiple of the wavelength k. Hence, we obtain the famous Bragg reflection law 2 a sin h ¼ n k

ð2:2Þ

where n is an integer. So far, we have restricted our discussion to a series of parallel lattice planes, which all have the same normal vector. However, in the case of a three-dimensional crystal we have to deal with two additional orientations of the lattice planes with the corresponding two directions of the normal vectors. For this, it is convenient, to start with a straight periodic arrangement of points forming a chain (Fig. 2.7). The spherical waves originating from all points are ampliﬁed, reaching a maximum intensity, if the propagation distance starting from two neighboring points differs exactly by one wavelength or by a multiple of one wavelength. On the other hand, if the difference amounts to half a wavelength or an uneven multiple of half a wavelength, complete extinction occurs. In this way we ﬁnd that propagation directions for maximum or minimum intensity exist, and these are conically arranged around the straight line of points. The smaller the distance between the points, the larger is the opening angle of these cones. On the surface of an imagined sphere, having its center at the common tip of this family of cones, the propagation directions with maximum or minimum intensity form a series of circles. Next we extend our one-dimensional arrangements of points to a two-dimensional planar lattice. Now we must add a second family of cones which is arranged around the second newly-added straight line of points. On the surface of the imagined sphere, the propagation directions with maximum or minimum intensity yield a second series of circles. As a result, in this case the directions with maximum intensity are expected only for intersections between the corresponding circles originating from the two families of cones. However, such intersections always occur. Finally,

Fig. 2.6 Reflection of a wave at two neighboring lattice planes placed at the distance a. The difference of the distance covered by the wave upon the reflection at the two planes amounts to 2 a sinh. h is the angle between the lattice planes and the incoming and the outgoing wave, respectively

22

2 Well Ordered Lattice Structures in Crystals

Fig. 2.7 Generation of the Laue diagram as the interference pattern due to the diffraction of X-rays at a three-dimensional point lattice. a For a one-dimensional chain of points, the directions of maximum or minimum intensity lie on cones arranged around the one-dimensional chain. On the surface of an imagined sphere, having its center at the common tip of this family of cones, the directions of maximum or minimum intensity yield a series of circles. b For a two-dimensional planar lattice of points we must add a second family of cones which is arranged around the direction of the second, newly-added straight line of points. Now a second series of circles appears on the surface of the imagined sphere. The points of intersection of these circles then yield the directions of maximum or minimum intensity. c Finally, for a three-dimensional point lattice we deal correspondingly with three families of cones. However, in general the resulting three series of circles on the surface of the imagined sphere no longer have common points of intersection, which mark the directions of maximum or minimum intensity. Now such common points of intersection only exist for special values of the wavelength or frequency of the X-rays

extending our discussion to a three-dimensional lattice of points, we have to deal with three families of cones. Again, it is the intersections between all three families of cones on the surface of the imagined sphere, which determine the propagation directions with maximum diffraction intensity. However, now the three series of circles on the imagined sphere do not in general have any common intersections (Fig. 2.7). In this case common intersections, marking the directions of high intensity of the diffracted waves, only exist as exceptions, i.e., only for specially selected values of the wavelength or frequency of the X-rays. For these selected wavelengths we have special distinct diffraction directions with high intensity, generating a characteristic pattern of points on the photographic ﬁlm used for X-ray detection. This characteristic pattern is referred to as the “Laue diagram” (Fig. 2.8). However, this procedure only works if a whole frequency band of X-rays is available, from which the appropriate frequencies for the directions with high intensity are then automatically selected by the diffraction process. The Bragg diffraction law expressed in (2.2) is named after the two English scientists William Henry Bragg and his son William Lawrence Bragg, whom we have previously mentioned. Immediately following the publication of the ﬁrst Laue

2.1 Diffraction Theory

23

Fig. 2.8 Laue diagram of a cubic K2SnCl6 crystal obtained by X-ray diffraction (Photo J. Ihringer)

diagrams they have theoretically analyzed the underlying interference phenomena. The pattern of points on the Laue diagram is particularly useful for determining crystal symmetries.

2.2

Reciprocal Lattice, Brillouin Zones

Mathematically, the diffraction of a wave at a spatially periodic crystal lattice (periodic potential) can be treated conveniently by means of the concept of the reciprocal lattice. This concept is based on the abstract mathematical wave vector space or momentum space (Fourier space). It has been proposed by the American Josiah Willard Gibbs. A wave propagating along x-direction can be written as a complex function

24

2 Well Ordered Lattice Structures in Crystals

Fðx; tÞ ¼ Fo eiðkxxtÞ

ð2:3Þ

Here t denotes the time and x the angular frequency. The wave number k is connected with the wavelength k via the relation k = 2p/k. In the three-dimensional case the function (2.3) can be generalized, and we obtain Fðr; tÞ ¼ Fo eiðk rxtÞ

ð2:4Þ

where r = x + y + z and k = kx + ky + kz. Now the wave number k of the one-dimensional case is replaced by the wave vector k and its three components kx, ky, kz. The reciprocal lattice is deﬁned as follows: G ¼ h1 A þ h2 B þ h3 C

ð2:5Þ

where h1, h2, h3 are integers. The fundamental vectors A, B, C are connected with the translation vectors a, b, c of the elementary cell (Fig. 2.2) and are deﬁned as follows: A ¼ 2p

bc ; ab c

B ¼ 2p

ca ; ab c

C ¼ 2p

ab ab c

ð2:6Þ

We see that the vectors A, B, C of the reciprocal lattice are oriented perpendicularly to two fundamental axes of the crystal lattice, respectively. The convenience of the introduction of the reciprocal lattice becomes obvious, if one wants to express mathematically a function having exactly the periodicity of the crystal lattice (for example, the scattering potential of the electrons). Such a function is obtained in the form U(rÞ ¼

X

uG e i G r

ð2:7Þ

G

where the summation extends over all vectors G of the reciprocal lattice. This function satisﬁes the periodicity condition Uðr þ qÞ ¼ UðrÞ

ð2:8Þ

Here q is a lattice vector in the form of (2.1). We note that for the lattice vectors q the reciprocal-lattice vectors G satisfy the relation eiGq ¼ 1

ð2:9Þ

2.2 Reciprocal Lattice, Brillouin Zones

25

We see this by writing Gq ¼ ðh1 A þ h2 B þ h3 CÞðn1 a þ n2 b þ n3 cÞ ¼ 2pðh1 n1 þ h2 n2 þ h3 n3 Þ: This integer multiple of 2p directly yields the periodicity (2.8): X X Uðr þ qÞ uG ei Gðr þ qÞ ¼ uG ei G r ¼ UðrÞ G

G

We turn now to the diffraction problem, scattering a wave from the incoming wave vector k into the outgoing wave vector k´. The intensity of the scattered wave is proportional to Z X Z 0 0 intensity ds eirðkk Þ UðrÞ ¼ uG ds eirðkk Þ ei G r G

(ds = volume element). The last integral vanishes due to cancellation by interference, except for the case when the exponent itself vanishes, i.e., when k − k´ + G = 0. So we ﬁnd the important new form of the Bragg condition for the constructive interference between two waves which are scattered by the crystal from k to k´: k0 k ¼ G

ð2:10Þ

From the simple form of (2.7) and (2.10) we see again the advantage gained by the concept of the reciprocal lattice. The abstract momentum space (k-space) with the reciprocal lattice is divided into Brillouin zones. The boundaries of the Brillouin zones are found by erecting a plane in perpendicular direction at exactly the middle of a connecting straight line to a point of the reciprocal lattice. If one uses larger and larger reciprocal lattice vectors in this construction, one obtains the ﬁrst, second, third, etc. Brillouin zone. In Fig. 2.9 we show as an example the ﬁrst Brillouin zone in the two-dimensional

Fig. 2.9 Construction of the ﬁrst Brillouin-zone in the (two-dimensional) case of the two fundamental vectors A and B of the reciprocal lattice oriented perpendicular to each other

26

2 Well Ordered Lattice Structures in Crystals

case of the two fundamental vectors A and B oriented perpendicular to each other. As we will see in Chap. 4, in the case of the electronic band structure of materials the Brillouin zones play an important role. Following the initial success of X-ray diffraction experiments, the method was quickly developed further along different directions. In the “rotating-crystal technique“ a well-focused monochromatic X-ray beam is directed upon the crystal and, simultaneously, the crystal is rotated around a ﬁxed axis. The high intensity of the diffracted radiation is observed only for distinct angle orientations of the crystal relative to the incoming X-ray beam, for which the Bragg interference condition is satisﬁed. The two X-ray diffraction techniques that we have discussed so far require sufﬁciently large single crystals. As proposed for the ﬁrst time by Peter Debye and Paul Scherrer, even crystal powder can be used. The powder may be compressed into the form of a little cylinder. For this powder technique one again uses monochromatic X-rays. Among the many randomly arranged little crystals in the powder there always exist a sufﬁciently large number for which the Bragg diffraction condition is well satisﬁed by their orientation. Here the sample rotation of the rotating-crystal technique is done quasi-automatically. As an important result we note that all three methods serve well for exactly determining the atomic or molecular distances between nearest neighbors in the crystal lattice, if the wave length of the X-rays is known. During his experiments in Würzburg, Röntgen discovered the new radiation when he was investigating the physical behavior of gas discharges within an evacuated cathode ray tube. After only a few weeks of intensive experimentation he found that the new radiation always appeared if the fast electrons were abruptly decelerated by a solid obstacle in the glass tube. Here objects made from heavy elements such as tungsten or platinum were particularly effective. The principle of the generation of “bremsstrahlung”, as it was subsequently called, had been found, and it continues to be used today in the construction of X-ray sources. Röntgen had received one of his ﬁrst glass tubes, especially designed for the generation of X-rays with fused cathode and anode, from the glassworks of the Company “Greiner and Friedrichs” in the small town of Stützerbach near Ilmeau in Thuringia. Eventually, the large companies of the electronics industry took up the manufacture of X-ray equipment, and this ﬁeld developed into an important business sector. Right up until today, the degree of automatization and standard of operation of the equipment has continuously improved.

The generation of X-rays within large rings-shaped electron accelerators, referred to as electron synchrotrons, is the latest development. An impressive example is the large European Synchrotron Radiation Facility (ESRF) in Grenoble with its ring diameter of 270 m (Fig. 2.10). Along the circular structure there is room for about 60 different measuring stations (beam-ports). The accelerated electrons move along a circular trajectory at a high energy of 6 GeV. This trajectory results from the balance between a force directed towards the center of the ring and the centrifugal force directed outwards. Because of this constant acceleration of the electrons in order to keep their circular trajectory, “synchrotron radiation“ is emitted, the frequency of which depends upon the kinetic energy of the electrons. By means of special deflection elements inserted into the ring, the so-called

2.2 Reciprocal Lattice, Brillouin Zones

27

Fig. 2.10 Photograph of the large European synchrotron radiation source in Grenoble (bright ring in the foreground). The round tower-like container next to the ring is the external envelope of the German-French Research Reactor of the Laue-Langevin Institute. (Studio de la Révirée, Grenoble)

wigglers or undulators, individual beams with special properties can be supplied to the different beam-ports. Today, large intensive radiation sources similar to that in Grenoble are in operation worldwide at several locations. These radiation sources mainly serve to generate electromagnetic radiation of high intensity in the far ultraviolet and in the near X-ray spectral range. Today, X-ray diffraction represents one of the most important tools for the analysis of materials. As outstanding indications of the importance of X-rays in determining the structure of materials, in addition to the ﬁrst experimental proof of the lattice structure of crystals discussed before, we mention, for example, the X-ray analysis of Max Perutz of the hemoglobin in red blood cells which provides human oxygen transport, and the famous proposal for the structure of the DNA double helix by Francis Harry Compton Crick and James D. Watson, which during winter 1952/1953 was conﬁrmed for the ﬁrst time by Rosalind Franklin with her X-ray images. At this point we must also mention the work by Robert Huber, Johann Deisenhofer, and Hartmut Michel, clarifying the three-dimensional structure of the reaction center of photosynthesis by means of X-ray diffraction. The last three examples emphasize the great importance of X-rays in analyzing the structure of complex organic materials such as proteins and nucleic acids. Therefore, these concepts dating back to Max von Laue, W. H. Bragg, and W. L. Bragg, have been increasingly reﬁned. In this way it has become possible that, from the patterns of

28

2 Well Ordered Lattice Structures in Crystals

X-ray diffraction, both the periodic spatial lattice arrangement of the molecular crystal and the inner atomic structural detail of the protein molecules, can be reconstructed. However, in this case the relevant organic crystals must be prepared, which can often prove difﬁcult and can require special attention. In addition to the diffraction of X-rays, we again mention the (elastic) scattering of neutrons and its increasing importance for the analysis of the structure of crystals. In recent years in several research centers, the facilities for neutron diffraction have been strongly expanded. Finally, we wish to discuss a phenomenon, the discoverer of which at ﬁrst experienced rejection and mockery, until, after the gradual acceptance of his ideas, in 2011 he became honored by the award of the Nobel Prize in Chemistry: Daniel Shechtman and his discovery of quasi-crystals. On April 8. 1982 at the Johns Hopkins University in Baltimore, USA, with his electron microscope he obtained a diffraction image of an alloy of aluminum and manganese showing a tenfold symmetry. Hence, during a complete rotation an identical image was reproduced ten times, i.e., after each additional 36 degrees. The further research indicated, that the crystal itself exhibited a ﬁvefold symmetry, which should be impossible according to the state of knowledge at the time. In such a crystal showing ﬁvefold symmetry the atoms are arranged regularly, but not exactly periodically any more. How could Shechtman obtain the sharp diffraction pattern? For his results Shechtman was strongly criticized from all directions. Even he had to leave his research group in Baltimore, and went back to Israel. He could publish his results only two and a half years later. However, subsequently, support for Shechtman started gradually. Five weeks after his paper there appeared a publication discussing this new type of crystals, and the name “quasi-crystals” was proposed. Already in the middle 1970s the mathematician Roger Penrose had demonstrated, that, by using only two building blocks, a slender and a compressed, skewed rectangle, one can generate a pattern completely covering a plain surface, but never exactly repeating itself. In the meantime, quasi-crystals have been found in many materials systems and also in nature. In its communication regarding Shechtman, the Nobel Committee emphasized especially the “important lesson for science”: Apparently, the achievement by Dan Shechtman not only consists of the discovery of the quasi-crystals, but also of the fact, that he recognized the importance of this discovery and resolutely conveyed it to a skeptical scientiﬁc community.

2.3

Types of Bonding

In the last part of this chapter we want to discuss the types of bonding between the (atomic or molecular) constituents of a solid. In principle, in this case we always deal with some kind of an attractive (electrostatic) interaction between electrons and the positively charged atomic nuclei (gravity and nuclear forces do not play any role

2.3 Types of Bonding

29

in this discussion). There are special cases possible, resulting in the different types of bonding. In the form of a solid (or of condensed matter) the total energy of all constituents is always lower than in the case when it is completely disassembled into its atoms or molecules without any mutual interactions any more. The corresponding energy gain represents the binding energy. One distinguishes between the following main types of bonding: van-der-Waals bond, ionic bond, covalent bond, metallic bond, and hydrogen bond. Starting with the van-der-Waals bond, we consider atoms with completed electron shells (for example noble gases), which are difﬁcult to ionize. On time average, at each atom we ﬁnd a spherically symmetric charge distribution of the negative electron shells around the positive atomic nucleus. Whereas in the stationary state the electric ﬁeld in the external space vanishes, the motion of the outer electrons (fluctuations) results in a temporally varying dipole moment (the time-averaged value of which remains zero). Considering two atoms (1) and (2) at distance R, the instantaneous dipole moment p1 of (1) generates the electric ﬁeld jEj ¼ 2p1 =R3

ð2:11Þ

at the location of (2). The result is the induced dipole moment p2 ¼ ajEj ¼ 2a p1 =R3

ð2:12Þ

of (2). Here a denotes the polarizability. The attractive interaction between p1 and p2 can be seen from the two cases shown in Fig. 2.11. In case 1, because of the decrease of the electric ﬁeld E with increasing distance of p1, there results a force on p2 directed to the left. In case 2 we have an attraction again, since the distances between the opposite charges (attracting each other) are smaller than those between the same charges (repelling each other).

Fig. 2.11 Attractive interaction between the dipoles p1 and p2 of the two atoms (1) and (2) in the case of the van-der-Waals bond. Further details in the text

Case 1 :

Case 2 :

30

2 Well Ordered Lattice Structures in Crystals

As we know from electrostatics, the potential energy U(R) between two dipoles p1 and p2 at mutual distance R is UðRÞ ¼

p1 p2 3ðp1 RÞðp2 RÞ : R3 R5

ð2:13Þ

In case 1 of Fig. 2.11 one obtains UðRÞ ¼ 2p1 p2 =R3 ¼ 4a p21 =R6 :

ð2:14Þ

Here we note, that the temporal average p21 [ 0, even though p1 ¼ 0. The weak van-der-Waals bond is undirected. It is found in noble gases and in crystals of many organic molecules. The value of the bond energy is about U 1021 J 102 eV with R 0.4 nm. At this point we include a remark about energy units: We have: 1 eV (electron volt) = 1:6 1019 J (Joule) and - with Boltzmann’s J T. Hence, the value of U given constant kB - the thermal energy kB T 1023 K above is obtained in the case T = 100 K. Therefore, the melting temperature of these materials is about 100 K. From (2.13) and (2.14) one ﬁnds that the bond energy U(R) decreases rapidly with increasing distance R, proportional to R6 . However, because of the overlapping of the electron shells, at sufﬁciently small distance one ﬁnds repulsion. Assuming the empirical repulsion law proportional to R12 one obtains UðRÞ ¼ 4e

r 12 r6 : R R

ð2:15Þ

The model potential (2.15) ﬁxed by means of the two parameters e and r is referred to as the Lennard-Jones potential. It is shown in Fig. 2.12. This potential and other similar model potentials having two or more parameters adjusted to the experimental data serve for calculating physical quantities.

Fig. 2.12 Schematic of the Lennard-Jones potential U(R) according to (2.15)

U

σ

1.122 σ R

-ε

2.3 Types of Bonding

31

Turning now to a crystal consisting of N atoms, with (2.15) one ﬁnds the total energy Utot by summation over all pairs: 8 ! ! 9 is the probability, that a vibrational state with the angular frequency x and the quantized energie ħx is occupied. This probability is given by the Bose-Einstein distribution \nx [ ¼

1 ehx=kB T

1

ð3:2Þ

3.2 Speciﬁc Heat of the Crystal Lattice, Phonon Spectrum

39

to which we will return below again. The distribution (3.2) had been proposed by Planck for the ﬁrst time in his famous law of electromagnetic radiation. In his model of the quantized energy of the lattice vibrations, in (3.1) and (3.2) Einstein at ﬁrst had assumed only a single frequency x = xE. Only a few years later, this Einstein model has been extended by Peter Debye, who assumed a continuous frequency spectrum of the vibrations, ranging between zero and a characteristic maximum frequency, the Debye-frequency xD. Now the vibrational energy of the crystal is given as an integral over all phonon frequencies U¼

xZD

dx DðxÞ\nx [ hx

ð3:3Þ

0

spectral energy density

Here D(x) is the number of vibrations per frequency interval, also referred to as density of states. (In Chap. 6 we will return to the calculation of the density of states D(x)). As an example, in Fig. 3.4 we show the spectral energy density of the phonons of a germanium crystal. In this way Debye was able for the ﬁrst time to explain the temperature dependence of the total energy of the lattice vibrations in crystals and in particular the famous T3 behavior of the speciﬁc heat at low temperatures, in excellent agreement with experiment. Again, Planck’s energy quantization, now applied to

Fig. 3.4 Spectral energy density of the phonons in a germanium crystal at the temperature of 10 K according to the Planck radiation law, plotted versus the phonon frequency m

40

3 Permanent Movement in the Crystal Lattice

the lattice vibrations, has played a central role, and the classical law of Dulong and Petit has been eliminated. The measurements of the speciﬁc heat of crystals, together with the Debye model, had created a signiﬁcant advance of the general acceptance of quantum theory. For example, it was only after these measurements that the later Nobel Laureate Walther Nernst became convinced that Planck’s quantum theory was more than just an interpolation formula and that it represented new fundamental physics. The fact, that Planck had based his revolutionary new idea on the physics of heat radiation, had resulted from the relatively high level of experimental optics already reached at that time. In the years 1910–1916 in Berlin, in an extensive research program together with many collaborators, Walther Nernst systematically investigated the speciﬁc heat of many solid materials at low temperatures, conﬁrming the quantum theory. In the meantime, Nernst had recognized clearly the fundamental importance of quantum theory. Therefore, he also organized the ﬁrst large conference dealing with this subject, the famous First Solvay-Conference on “The Theory of radiation and the quanta” held in Brussels from October 30 until November 3, 1911. For this conference Nernst had been able to enlist the ﬁnancial support of the Belgian industrialist Ernest Solvay.

The important central idea during the development of quantum mechanics in the 1920s was the strict limitation of all statements about the atomic world to observable facts. The fact that the elementary particles such as electrons, protons, neutrons, etc., are exactly identical, must be centrally incorporated into the theory. If the same two elementary particles are exchanged, the result must remain unaffected. Hence, the theoretical qualities must have certain symmetry properties. This requirement has severe consequences for the probability distribution of the different states of the systems, and new concepts for quantum statistics are needed. The ﬁrst steps in this direction originated from the Indian physicist Satyendra Nath Bose. In 1924 he had derived Planck’s radiation law in a new way. Since he ran into difﬁculties during the publication of his results, he approached Einstein asking him for support. Einstein felt enthusiastic about Bose’s paper and arranged for its publication in the Zeitschrift für Physik. Subsequently, starting from Bose’s results, in some additional papers Einstein pointed out the formal similarity between radiation and an ideal gas. Today, the resulting concept of quantum statistics is referred to as Bose-Einstein statistics. Bose-Einstein statistics apply to exactly identical elementary particles with zero or integer angular momentum. Hence, these particles are also called bosons. A single quantum state can be occupied by an arbitrarily large number of bosons. Since phonons have zero angular momentum, they belong to this kind of particles. Light quanta or photons are bosons also, since their angular momentum is equal to one. However, electrons require a different kind of quantum statistics, as we will discuss in Chap. 5. The energy spectrum of phonons is described also by Planck’s radiation law, similar to the photon spectrum of a heat radiator (Fig. 3.4). However, compared with the spectrum of electromagnetic radiation, the phonon spectrum displays an important difference, since its frequencies are restricted to the range below a

3.2 Speciﬁc Heat of the Crystal Lattice, Phonon Spectrum

41

characteristic maximum frequency, the “Debye frequency” xD. This maximum frequency xD simply results from the discrete lattice structure of the crystals. Below the nearest-neighbor distance of the crystal lattice, length scales for the lattice vibrations are meaningless, resulting in the deﬁnition of a minimum value of the wavelength and a corresponding maximum value of the vibration frequency. The resulting maximum value ħ xD of the phonon energy is referred to as the Debye energy. Since, on the other hand, the electromagnetic waves propagate in a continuous medium without any lattice structure, in this case we are not confronted with corresponding minimum or maximum values of the wavelength and the frequency, respectively. One ﬁnds the density of states D(x) from the number of the elastic natural frequencies ﬁtting exactly into the volume of the crystal, say, into a cube with the edge length L. Furthermore, in K-space the increment of the volume due to the frequency increment dx must be considered. (Here and in the following, K denotes the phonon wave vector). In this way one ﬁnds D(x) * x2. By inserting < nx > from (3.2) into (3.3), ﬁnally we obtain the vibrational energy of the crystal. The speciﬁc heat (at constant volume) of the lattice vibrations derived from this energy is given by 3 @U T zZD z4 ez CV ¼ ð ÞV ¼ 9 N kB dz @T h 0 ðez 1Þ2

ð3:4Þ

Here, h = ħxD/kB denotes the Debye-temperature. In this context, introducing the quantity z = ħx/kBT is convenient (zD = ħxD/kBT = h/T). At low temperatures (T < < h) the expression in (3.4) yields CV * T3, in good agreement with the experimental data. On the other hand, at high temperatures (T > > h) from (3.4) one obtains the constant result CV = const, i.e., the classic law of Dulong and Petit. The dependence of the phonon frequency x on the wave vector K of the phonons is obtained from a theoretical model, in which the crystal lattice is approximated by point-like masses connected with each other by elastic spiral springs. In the simplest case of a linear chain with the lattice constant a and the same point-like masses m, connected with each other by means of the same spring constant f, one ﬁnds the dispersion relation 1=2 4f Ka x¼ sin m 2

ð3:5Þ

In the case of a discrete lattice with the distance a between neighbors, the wave vector K is conﬁned to the range of the ﬁrst Brillouin zone, i.e., in the case of the one-dimensional chain to the range −ap K ap. In the limit of small values of the wave vector, one obtains from (3.5):

42

3 Permanent Movement in the Crystal Lattice

x¼

a2 f m

1=2 K

ð3:6Þ

1=2 represents the sound velocity. Equation (3.6) indicates the m acoustic limit, and (3.5) characterizes an acoustic mode. In the simplest case we only have to deal with a single atom per elementary cell of the crystal lattice. The vibration of the atom can occur within all three spatial dimensions. Hence, the phonons propagating through the crystal are also characterized by different spatial directions of the lattice vibrations. In the case of “longitudinal phonons” the atoms of the crystal lattice vibrate parallel to the propagation direction of the wave. On the other hand, for the “transverse phonons” the vibration occurs along each of the two principal directions perpendicular to the propagation direction, respectively. In this way the three “acoustic phonon modes” must be distinguished: one longitudinal mode and two transverse modes. They are referred to as acoustic modes, since in the limit of large wavelengths the corresponding phonons propagate with the velocity of sound (Fig. 3.5). (Because of the cubic face-centered symmetry in the case of the example of copper, the boundary of the ﬁrst Brillouin zone is located at K = 2p/a, in contrast to K = p/a in the case of the linear chain or the simple cubic symmetry with the lattice constant a). If the crystal lattice contains more than a single atom per elementary cell, the “optical modes” must be added. In the case of the optical modes, the atoms within the elementary cell oscillate in opposite phase relative to each other. If the atoms carry opposite electric charge, as in the case of the ionic crystals, due to these oscillations electric dipole moments appear, which affect the optical properties. In the case of p atoms per elementary cell, there are a total of 3p different phonon modes: 3 acoustic modes and 3p – 3 optical modes. The factor

a2 f

Fig. 3.5 Phonon angular frequency x = 2pm plotted as a function of the wave number K of the phonons (“dispersion curves”) of a copper crystal. The wave vector is oriented along the direction of the cube edges of the cubic unit cell of the crystal. L denotes the longitudinal and T the transverse phonon branch. a = 0.361 nm is the distance between neighbors in the cubic crystal lattice of copper. (B. N. Brockhouse)

3.2 Speciﬁc Heat of the Crystal Lattice, Phonon Spectrum

43

Experimentally, the energy spectra of the phonons are determined mostly by means of inelastic neutron scattering in crystals. The pioneering experiments were performed by Bertram Neville Brockhouse from McMaster University in Canada. He carried out his ﬁrst measurements in 1955 with aluminum. One needs to measure the change in energy and momentum of the neutrons as they emit or absorb a phonon within the crystal. The impressive advances in the ﬁeld of neutron spectroscopy, which to a large extent were due to Heinz Maier-Leibnitz and his group ﬁrst at the Technical University of Munich in Garching and later at the Laue-Langevin Institute in Grenoble, have turned out to be extremely fruitful.

Max von Laue and his colleagues in Munich, prior to their famous X-ray diffraction experiment, were very concerned at the time by the following obvious question: Is it not likely that the perturbation of perfect order in the crystal lattice due to the permanent lattice vibrations really ruins the observation of X-ray diffraction? However, the clear and positive experimental result gave a decisive answer to this question. In 1913 Peter Debye wrote a series of papers theoretically treating the role of the thermally excited vibrations of the crystal lattice as it affects the diffraction of X-rays. During the 1920s this subject was taken up again by the Swedish theorist Ivar Waller. Both scientists have shown that the thermal lattice vibrations only effect a reduction of the maximum intensity of the diffracted beam, whereas the linewidth of the diffracted beam remains the same. The reason for this is simply that the thermal motion of the many atoms in the lattice is completely uncorrelated, leading effectively to a cancellation between the oscillations of the different atoms. This reduction of intensity of the diffracted beam is quantiﬁed in terms of the “Debye-Waller factor”. This factor indicates, furthermore, that the intensity of the diffracted beam strongly increases with decreasing temperature. The Debye-Waller factor played a key role later during the discovery of the Mössbauer effect. As a young Ph.D. student in Munich Rudolf L. Mössbauer has been asked by Heinz Maier-Leibnitz, his thesis advisor, to study the resonance absorption of c-radiation in atomic nuclei. Mössbauer was supposed to ﬁnd out if the c-radiation emitted by an atomic nucleus of the source is resonantly re-absorbed by another atomic nucleus of the same element in the absorber. For the observation of this effect it is necessary for there to be sufﬁcient overlap between the spectral energy widths of the c-radiation for the emission and the absorption processes. Here the main issue centered around the question of whether this required overlap disappears, perhaps completely, because of the recoil during the emission and absorption of the c-quantum, thereby eliminating the possibility of resonance absorption. It is interesting that initially in particular Heinz Maier-Leibnitz had the idea of enhancing this energetic overlap by increasing the temperature and thereby enlarging the thermal linewidth of the c-radiation. However, this idea was soon discarded, and Mössbauer instead cooled the source and the absorber with liquid oxygen. This then turned out to be crucial, and Mössbauer could observe for the ﬁrst time the recoil-free nuclear resonance fluorescence. He performed his ﬁrst experiments using the 129-keV-radiation of the iridium isotope 191Ir, with the iridium atoms implanted within a crystal. Again, it was the elimination of the influence of the phonons on the linewidth of the Mössbauer line, which had

44

3 Permanent Movement in the Crystal Lattice

produced the effect he was looking for, exactly as prescribed by the Debye-Waller factor. The question of the recoil now became irrelevant, since the iridium atoms were solidly implanted within the host crystal. The extremely narrow energy width of the Mössbauer line is ﬁnally limited only because of the “natural line width”, resulting from the ﬁnite lifetime of the quantum mechanical state due to the Heisenberg uncertainty relation. Because of this extremely narrow linewidth a large number of highly sensitive measurements has become possible in many areas. An early spectacular case is the detection of the energy change in the quanta of c-radiation after they have travelled upwards a certain distance in height in the gravitational ﬁeld of the Earth. In 1960 this was detected by the American physicists Robert V. Pound and Glen A. Rebka. In their experiment the distance in height travelled was 22.5 m.

3.3

Thermal Conductivity of the Crystal Lattice

In crystals phonons also contribute to the transport of heat energy. In electrical insulators they represent the only mechanism determining the heat conductivity. The phonon contribution jG to the heat conductivity of a crystal is closely connected with the lattice component C of the speciﬁc heat. This is indicated by the simple formula of the kinetic theory of jG: 1 jG ¼ v C ‘ 3

ð3:7Þ

Here v is the velocity and ‘ the mean free path of the phonons. As a model, we can think about phonons in terms of a gas experiencing many collisions between its particles. Because of the many collisions, in general the heat transport provided by the phonons is a diffusive process. With increasing temperature the number of thermally excited phonons, and hence the collision probability among the phonons, increases. As a result, with increasing temperature the heat conductivity decreases. However, at very low temperatures we have an exception. In this case, the number of phonons is very small, the collisions between them become unimportant, and it is only the number of phonons which matters. Now the mean free path ‘ is limited by the collisions with the surface of the crystal, and it becomes independent of the temperature. In this regime we have C * T3 and because of (3.7) jG * T3. At higher temperatures, an exact theoretical treatment shows, that a novel process must be taken into account, the “umklapp-process” (U-process). It effects, that the directed momentum of the phonons is transferred to the crystal and is lost for the heat transport. Denoting the wave vectors of the phonons participating in the umklapp-process by Ki, we obtain

3.3 Thermal Conductivity of the Crystal Lattice

K1 þ K2 ¼ K3 G:

45

ð3:8Þ

G is a vector in the reciprocal lattice. Processes with G = 0 are referred to as N-processes. The concept of the umklapp-processes has been proposed for the ﬁrst time in 1929 by Rudolf E. Peierls, who was born in Berlin and later emigrated to England. (In Chap. 2 in the case of (2.10) we have dealt already with a similar case, in which during a Bragg reflection the momentum of the photon is transferred to the crystal). The umklapp-processes yield an important contribution only if K1 þ K2 12 G. However, at low temperatures they are frozen out, since phonons satisfying this condition are not thermally excited. On the other hand, at high temperatures (T > h) the U-processes are dominant. Their number increases proportional to the number of phonons, which in turn is proportional to temperature. Hence, for the mean free path ‘ of the phonons one ﬁnds ‘ T1 . Because C = const in this case, from (3.7) we obtain: jG T1 . The overall result for the temperature dependence of the heat conductivity of the lattice is a curve with a distinct maximum (Fig. 3.6). For example, in sapphire (Al2O3) this maximum is located near 30 K. Diamond is a material with an extremely high heat conductivity. Therefore, a special effort has recently been concentrated on the development of thin diamond layers, which are highly interesting technologically for cooling purposes because of their large heat conductivity.

3.4

Ballistic Phonons

Fig. 3.6 Temperature dependence of the heat conductivity of an electrical insulator (schematically)

heat conductivity

As we have discussed before, the collision processes between phonons become more and more rare at sufﬁciently low temperatures. In this regime phonons can propagate freely over distances as large as, say, about mm to cm with sound velocity. In this case we are dealing with ballistic phonons. The propagation of ballistic phonons can be observed easily, if a heat pulse is applied locally to the front surface of a well-cooled crystal. The generated phonon pulse can be detected locally at the back of the crystal after the proper time of flight (Fig. 3.7). For

temperature

46

3 Permanent Movement in the Crystal Lattice

(a)

(b)

electron or laser beam

phonon pulse

crystal

crystal

detector

Fig. 3.7 Ballistic propagation of phonons at low temperatures. a Scheme of an experiment to measure the propagation time of the phonons. On the left hand side of the crystal the phonons are generated by means of a heat pulse applied to the source S, and subsequently they are detected on the right hand side of the crystal with the detector D. A thin metal layer deposited on the crystal surface can act as a source by means of the application of an electric current pulse. A deposited thin layer, the electric resistance of which responds sensitively to pulsed temperature changes, can also serve as detector. b A pulsed electron beam or laser beam, directed at the crystal surface at one side of the crystal, can also be used for the generation of a phonon pulse. If furthermore the beam is scanned over the crystal surface, while the detector remains locally ﬁxed on the opposite side of the crystal, the ballistic propagation of the phonons can be studied as a function of the propagation direction in the crystal

Fig. 3.8 Image of the intensity of the ballistic phonons in dependence on the propagation direction in a silicon single crystal at a temperature of 2.0 K (“phonon imaging”). While the crystal surface on one side is scanned with the electron beam, the intensity of the ballistic phonons is recorded on the opposite side of the crystal with a locally ﬁxed detector in dependence on the coordinate point of the scanned crystal surface. Bright regions correspond to high intensity. The spatially diagonal line of the cubic unit cell of the crystal is oriented perpendicular to the scanned surface of the crystal

3.4 Ballistic Phonons

47

generation of the heat pulse, a pulsed laser beam or electron beam directed on the crystal surface can be used. Due to the anisotropy of the elastic crystal properties, the ballistic propagation of the phonon energy displays distinct maxima along certain directions within the crystal. This effect is referred to as phonon focusing, and can be easily demonstrated using the method we have just discussed. The only requirement is that the beam is scanned laterally over the crystal surface, while the detector is ﬁxed locally at the back of the crystal. In Fig. 3.8 we show a typical example. If the crystal is cooled to lower and lower temperatures, eventually only the “zero-point motion” of the building blocks of the crystal remains. The zero-point motion follows from the quantum mechanical uncertainty relation, which requires that a spatially ﬁxed object always displays a ﬁnite uncertainty of its momentum. The resulting zero-point energy of an oscillator at frequency m amounts to ½ h m.

Chapter 4

Electric Conductor or Insulator?— Energy Bands

Abstract Application of quantum mechanics to the electrons in the periodic potential of the crystal lattice yields the energy bands separated from each other by forbidden energy gaps. The approximations with bound electrons (F. Bloch) and with nearly-free electrons (R. Peierls) are discussed. Depending on how the energy states within the bands are occupied by electrons, we deal with electrical conductors, semiconductors, or insulators.

After the principles of the new quantum mechanics had been established during 1925 and 1926 mainly by Werner Heisenberg from Germany, Erwin Schrödinger from Austria, and Paul Adrien Maurice Dirac from England, there developed a strong interest in applying the theory to as many different cases as possible. Only by applying the theory to a large number of examples could familiarity with the new concepts be achieved. After simple cases such as the hydrogen atom or the hydrogen molecule had been treated, more complex problems were tackled. At that time important developments began in Leipzig. In 1927, at the young age of only 26 years, Heisenberg had already accepted the offer of a Chair of Theoretical Physics at the University of Leipzig. Here he quickly attracted a group of extremely gifted and creative young scientists, who subsequently had a dominant impact on further developments in physics. At the beginning of 1928 Heisenberg had already recognized that quantum mechanics would play an important role for crystals. The Swiss scientist Felix Bloch, born in Zürich, had just joined Heisenberg’s group as a Ph.D. student (Fig. 4.1). For his thesis Heisenberg proposed two possible subjects: Bloch could take up the quantum mechanical theory of ferromagnetism or the electron theory of metals. Since Bloch knew that Heisenberg had already worked out the basic parts of the ﬁrst subject, he preferred the second one. Only in this way could he hope to come up with a signiﬁcant contribution of his own. Indeed, soon afterwards Heisenberg published his famous theoretical paper which became the starting point of the modern theory of ferromagnetism. The quantum mechanical theory of electrons in crystals requires the solution of the Schrödinger equation in the case of the spatially periodic crystal lattice. In this © Springer Nature Switzerland AG 2019 R. P. Huebener, Conductors, Semiconductors, Superconductors, Undergraduate Lecture Notes in Physics, https://doi.org/10.1007/978-3-030-31420-0_4

49

50

4 Electric Conductor or Insulator?—Energy Bands

Fig. 4.1 Werner Heisenberg (left), (Photo: Deutsches Museum) and Felix Bloch (right), (Photo: Nobel Museum)

case, the energy spectrum of the electrons is determined by the periodic potential U(r) of the crystal atoms. Then the Schrödinger equation is

h2 Dwðr) + U(rÞ wðrÞ ¼ e wðr). 2m

ð4:1Þ

Here m denotes the mass and w(r) the wave function of the electrons. D is the 2 2 2 Laplace operator Dw ¼ @@xw2 þ @@yw2 þ @@ zw2 and e the energy of the electrons. The potential energy U(r) must satisfy the periodicity condition (2.8). In the theoretical treatment we distinguish between two different important approximations: the bound-state approximation (after Felix Bloch) and the free-electron approximation (after Rudolf E. Peierls). In both cases we deal only with the electrons in the highest available energy range, and not with the lower levels of the strongly bound states at the individual atoms at the sites of the crystal lattice.

4.1 Approximation with Bound Electrons (Felix Bloch)

4.1

51

Approximation with Bound Electrons (Felix Bloch)

In his dissertation, the results of which he published in 1928, Felix Bloch formulated the quantum mechanical foundation of the theory of electrons in crystal lattices. Due to the periodic potential of the crystal lattice in all three dimensions, the de Broglie waves of the electrons are spatially modulated following the rhythm of the lattice structure. In the approximation with bound electrons one assumes, that the electrons with the highest energy remain located most of the time at a certain lattice site, and only occasionally move to a neighboring lattice site, because of the small interaction between both locations. Their binding energy at a certain lattice site is assumed to be much larger than their kinetic energy. In this case the solution of the Schrödinger equation found by Bloch is based on the wave function uO ðrÞ of the quantum mechanical states of the electrons of the isolated individual atom or molecule with their corresponding discrete energy levels. We denote the coordinate of the electron by r and the coordinate of the atom or molecule (i.e., of the lattice site) by q. The solution proposed by Bloch in form of the superposition of the atomic wave functions uO ðrqÞ is then given by: wk ðrÞ ¼

X q

eikq uO ðrqÞ:

ð4:2Þ

This ansatz leads directly to the extended periodicity condition wk ðr þ qÞ ¼ eikq wk ðrÞ

ð4:3Þ

with the phase factor eikq . The periodicity (4.3) can be seen by writing wk ðr þ qo Þ ¼

X

¼e

q

eikq uO ðr þ qo qÞ

ikqo

X q

eikðqq0 Þ uO ðr½q qo Þ ¼ eikqo wk ðrÞ

The function wk(r) in (4.2) represents the famous Bloch ansatz for the quantum mechanical wave function of the electrons, upon which all further theoretical developments for crystals have since been built. The fact, that according to (4.3) a phase factor eikq “…can always be separated from the eigenfunctions, and where the rest only displays the periodicity of the lattice, can be vividly expressed such, that we are dealing with planar de-Broglie waves, which are modulated by the rhythm of the lattice structure” (the words of Felix Bloch in his paper About the Quantum Mechanics of the Electrons in Crystal Lattices, published in 1928, here in English translation). With the wave function (4.2) one ﬁnds the electron energy ek in the following way. Applying the rules of quantum mechanics, we have

52

4 Electric Conductor or Insulator?—Energy Bands

Z ds

wk ðrÞek wk ðrÞ

Z ¼ ek

ds wk ðrÞwk ðrÞ

ð4:4Þ

and using (4.1) we ﬁnd 1 ek ¼ N

Z

ds wk ðrÞ½

h2 D þ Ua ðr qÞ þ U(rÞ Ua ðr qÞwk ðrÞ 2m

ð4:5Þ

Here ds denotes the volume element. In (4.5) under the integral we have added and subtracted again the atomic potential Ua(r) shown in Fig. 4.2, and we have used the normalization of the wave function Z

ds wk ðrÞwk ðrÞ ¼ N

ð4:6Þ

where N is the number of the crystal atoms. We start with the ﬁrst two terms under the integral in (4.5). We assume that the atomic functions uO(r) of neighboring atoms overlap only very little. For each h2 atomic function uO(r − q) in the Bloch sum the operator ½ 2m D þ Ua ðr qÞ yields the eigenvalue eo, and we obtain Z 1 ds eo wk ðrÞwk ðrÞ ¼ eo ð4:7Þ N The last two terms under the integral in (4.5) yield R 1 ðrÞeikq ½U(rÞ Ua ðrqÞuO ðrqÞ ¼ N ds w (k ) P P ikðqq0Þ R 1 0 ¼N e dsuo ðrq Þ½U(rÞ Ua ðr qÞuo ðrqÞ q q0 In the double sum over q0 and q the two indices are treated independently of each other, and we can use the following procedure. We keep one running index ﬁxed and replace the sum by the factor N. For this we use q = 0 (Since the summation index runs over all lattice points, an arbitrarily taken ﬁxed index yields the same Fig. 4.2 Comparison of the energy of an electron, Ua(r), in the case of an isolated individual atom (solid line), and the case of the presence of atoms at the neighboring lattice sites, U(r) (dashed curve)

4.1 Approximation with Bound Electrons (Felix Bloch)

53

contribution as any other neighboring lattice point because of the translation symmetry). The factor N is cancelled, and we obtain for the last two terms (noting that we took q = 0) Z X eikq0 ds uo ðrq0 Þ½U(rÞ Ua ðrÞuO ðrÞ ð4:8Þ q0

In the sum over q0 we start with q0 ¼ 0; and then we take the nearest neighbors of = 0, i.e., q0 ¼ a, then the next-nearest neighbors q0 ¼ 2a, etc., where a denotes the lattice constant. However, often the next-nearest neighbors (and all others further away) can be neglected because of the vanishing product qo ðrq0 Þ uO(r) indicating the overlap of the atomic functions. The contribution q0 ¼ 0 yields ek = eo − a, with Z ð4:9Þ a ¼ ds uo ðrÞ½UðrÞ Ua ðrÞuo ðrÞ Ua(r) is the potential energy in the unperturbed individual atom. As we see from Fig. (4.2), due to the presence of the atoms at the neighboring lattice sites, we have Ua (r) [ U(r), and therefore a > 0. Turning to the contribution q0 ¼ a, we assume simple cubic symmetry of the lattice and combine the contributions of the nearest neighbors at the distances ±a in x-, y-, and z-direction, respectively. In this way we ﬁnd ek ¼ eO a 2b cos kx a þ cos ky a þ cos kz a

ð4:10Þ

With Z b ¼

ds uo ðr aÞ½U(rÞ Ua ðrÞuO ðrÞ

ð4:11Þ

The factor b contains the interaction between the nearest neighbors. In general, we have again b > 0. Because of the interaction between each atom or molecule and its neighbors within the crystal lattice, the discrete energy levels split up and broaden into energy bands. From (4.10) we see, that the lowest energy value is e = eO − a − 6b. From the highest energy value e = eO − a + 6b we see, that the width Δe of the energy band amounts to Δe = 12 b. Since the overlap between uo ðr aÞ and uO (r) increases with decreasing lattice constant a, then also the quantity b and, hence, the bandwidth Δe increases. In Fig. 4.3 we show this behavior schematically in the case of a one-dimensional chain. So far we have considered only the interaction of an atom or molecule at a certain lattice site with its nearest neighbors. In order to achieve a higher accuracy

54

4 Electric Conductor or Insulator?—Energy Bands

Fig. 4.3 Electronic band structure of a one-dimensional straight chain of hydrogen atoms with a distance between neighbors of 0.3, 0.2, and 0.1 nm, respectively. The electron energy e is plotted as a function of the wave vector k. For a single isolated hydrogen atom the electron energy is −13.6 eV. The broadening of this energy level results in the energy bands. The energy width of these bands increases strongly with decreasing distance between neighboring atoms. (R. Hoffmann)

of the approximation, one can include also the interaction with the next-nearest neighbors (and perhaps beyond those). At the end of our discussion of the bound-state approximation we note, that the interaction with the atoms or molecules at the neighboring lattice sites results in a broadening of the discrete energy values, associated with an isolated atom at a lattice site, into energy bands, the bandwidth of which increases with decreasing distance between the nearest neighbors.

4.2 Nearly-Free Electron Approximation (Rudolf Peierls)

4.2

55

Nearly-Free Electron Approximation (Rudolf Peierls)

In the other important limiting case, the approximation with free electrons, discussed for the ﬁrst time by Rudolf E. Peierls also in Leipzig, nearly-free electrons are assumed, and the perturbation by the periodic potential of the crystal lattice is considered to be small. In this case the electrons can propagate freely through the crystal in the form of matter waves. However, this free propagation is interrupted if the matter waves undergo Bragg reflection at the crystal lattice. If we completely ignore the potential energy U(r) in the Schrödinger equation (4.1), we obtain as solution the wave function of free electrons: wðr) ¼ eikr :

ð4:12Þ

By inserting (4.12) into (4.1), in the case U = 0 one ﬁnds the electron energy e ¼ h2 k2 =2m:

ð4:13Þ

The wave function (4.12) represents a plane wave with the wave vector k. However, a small periodic potential U(r) in (4.1) causes a strong effect, if the wave vector k lies close to the boundary of a Brillouin zone. At the zone boundary, the wave vector k exactly satisﬁes the Bragg condition (2.10), such that the wave experiences Bragg reflection. As an example, schematically indicated in Fig. 4.4, we take the point G1 of the reciprocal lattice and the zone boundary at G1/2. Due to the Bragg reflection, the wave vector k = G1/2 changes from k to k′ = k − G1= −G1/2. In the presence of the periodic potential U(r), the solution of the Schrödinger equation can be written as superposition of plane waves: wðr) ¼

X

ck eikr :

ð4:14Þ

k

If we express the small periodic potential U(r) of the crystal lattice in the form of (2.7), then in the case k = G1/2 (after some calculations) one obtains the electron energy

Fig. 4.4 Bragg reflection from k = G1/2 to k′ = k − G1 = −G1/2

56

4 Electric Conductor or Insulator?—Energy Bands

e ¼ e k uG 1 :

ð4:15Þ

Between the energies ek þ uG1 and ek uG1 there appears a forbidden energy gap, in which the solution (4.14) of a propagating wave does not exist. The spectral energy curve e(k) always approaches the boundaries of the Brillouin zones with zero slope. The magnitude of the energy gap increases with increasing coefﬁcient uG1 in (2.7), i.e., with increasing potential energy U(r) of the crystal lattice. In Fig. 4.5 we show the appearance of the forbidden energy gaps due to the Bragg reflection at the periodic potential of the crystal and the comparison with the case of the perfectly free electrons. In 1931 Allan H. Wilson from England had joined Heisenberg’s group in Leipzig, and ﬁnally it was he who provided the deﬁnite answer to the question, of whether a crystal is an electrical conductor, a semiconductor, or an insulator (Fig. 4.6). According to his proposal, which then turned out to be correct, the energy bands of the electrons in a crystal are responsible for the differences in the electrical conductivity. Here the decisive argument is based on the fact, that the preferential motion of the electrons along a certain direction (of an applied electric ﬁeld) is only possible, if the electronic states of the energy spectrum relevant under the non-equilibrium exist and can be occupied. If a band is only partly ﬁlled with electrons we have metallic electrical conductivity. On the other hand, one obtains an electrical insulator, if all energy bands are completely ﬁlled with electrons, and if at the same time no empty band exists nearby along the energy axis. Any band which is completely ﬁlled cannot contribute to the electrical conductivity, since the distribution of the velocities of all electrons in the band cannot be changed. However, in order to conduct an electrical current, the velocities of the electrons

Fig. 4.5 Energy bands in crystals. In the crystal lattice the continuous energy spectrum of free electrons (a) is divided into different energy bands, which are separated from each other by forbidden energy gaps (b). E energy; k wave vector; a distance between neighbors in the crystal lattice

4.2 Nearly-Free Electron Approximation (Rudolf Peierls)

(a)

(b)

57

(c)

empty band

empty band

Fig. 4.6 Energy-band model of the electric conductivity of crystals. a A completely ﬁlled energy band having a large energy distance (“energy gap”) to the next higher, but still completely empty energy band, yields an electric insulator. b A completely ﬁlled energy band with only a small energy distance to the next higher, but still nearly empty energy band, results in a semiconductor. c A well, but not yet completely ﬁlled energy band yields the electric conductance of a metal

must be redistributed in favor of the flow of current, which is impossible for a completely ﬁlled band, since unoccupied energy values are not available. There then remains as an interesting situation, the case where an empty band exists energetically close on top of a ﬁlled band, such that electrons can be transferred from the lower to the upper band by means of their thermal excitation energy. Hence, the energy gap between both bands must be sufﬁciently small. In this case we deal with a semiconductor, a subject we will discuss in Chap. 6. Typical values of the energy gap are about 0.1–1 eV in the case of semiconductors and about 10 eV in the case of insulators. For the theoretical physicists in Leipzig it has taken only three years to solve the problem of the electrical conductivity of crystals in terms of the energy bands of the electrons.

Chapter 5

Metals Obey the Rules of Quantum Statistics

Abstract The classical Drude-Lorentz model could explain some aspects of the electronic properties of metals such as the Wiedemann-Franz law. However, quantum statistics and the Fermi distribution of the electron energies turned into the key for the electronic theory of metals, including the important concept of the Fermi surface in momentum space. Over a wide temperature range the electronic transport properties of metals are dominated by the interaction between electrons and phonons (Bloch-Grüneisen law). Thermoelectricity (Peltier and Seebeck effect) is discussed briefly.

5.1

Drude-Lorentz Model

Before the quantum mechanical foundations discussed in Chap. 4 were developed, there already existed classical models for describing the behavior of electrons in metals. Here the dominating model was due to Paul Drude and Hendrik Antoon Lorentz. The electrons in a metal were assumed to represent an ideal gas which can move freely within the crystal lattice. Further, only one kind of mobile carriers of negative electric charge was assumed to exist. In some way, the presence of the atoms of the crystal lattice was ignored. However, they should occasionally result in collisions with the mobile electrons. In this way one could arrive at a ﬁnite value of the “electron mean free path” and, hence, a ﬁnite electrical conductivity. In an electric ﬁeld E the electrons in a crystal experience the force F= ħ

–e E .

ð5:1Þ

Here k denotes the wave vector and e the charge of the electrons. The quantity ħk is the mechanical momentum of the electrons. According to (5.1), after the time Δt the wave vector increases by the amount Δk. In the absence of any scattering processes, the increment Δk will grow further and further. However, since electrons

© Springer Nature Switzerland AG 2019 R. P. Huebener, Conductors, Semiconductors, Superconductors, Undergraduate Lecture Notes in Physics, https://doi.org/10.1007/978-3-030-31420-0_5

59

60

5 Metals Obey the Rules of Quantum Statistics

always experience scattering processes (due to phonons or defects in the crystal lattice), Equation (5.1) is valid only during a limited time interval. This time interval is the average time s between two scattering events, and one ﬁnds ħ ∆k = F τ = m ∆v.

ð5:2Þ

Here m denotes the mass and Δv the drift velocity of the electrons. Together with (5.1) one obtains for the electric current density j: j ¼ nðeÞDv ¼ ne2

s E; m

ð5:3Þ

where n denotes the density of the electrons. With the electrical conductivity r from the relation j = r E one ﬁnds: r ¼ n e2 s=m:

ð5:4Þ

As the result we obtain Ohm’s law, based on the average “relaxation time” s, assumed to be independent of the electric ﬁeld E. Since electrons also carry heat energy in addition to their electric charge, they also contribute to the heat conductivity of metals. This contribution of the electrons represents a second important mechanism of heat conduction, which must be taken into account in metals, in addition to the heat transport by the phonons, which we have discussed in Chap. 3. Often the contributions from both mechanisms are of similar magnitude. Since the transport of heat energy and of electric charge is due to the same electrons, one expects that the electronic part of the heat conductivity and the electrical conductivity will be proportional to each other, in agreement with experiment. This can be demonstrated using the following argument. In a temperature gradient dT/dx an energy current of density w flows from the hot to the cold side, given by w ¼ ð1=2Þn v feðT½xvsÞ eðT½x þ vsÞg de dT w ¼ n v2 s dT dx

ð5:5aÞ ð5:5bÞ

Here, e denotes the particle energy. In Fig. (5.1) we illustrate the argument leading to (5.5a, 5.5b). The mean free path ‘ = v s of the electrons represents the relevant length scale, at which the average motion of the electrons is affected along the temperature gradient. Based on the average energy ½ kBT per degree of freedom of a free particle, in the case of three degrees of freedom the energy e is given by 1 3 e ¼ m v2 ¼ kB T 2 2

ð5:6Þ

5.1 Drude-Lorentz Model

61

Fig. 5.1 Illustration regarding the heat current density of (5.5a, 5.5b). The arrows near Thigh and Tlow indicate the average electron energy

and using de 3 ¼ CV ¼ kB dT 2

ð5:7Þ

we obtain the energy current density

3 w ¼ n kB 2

2

sT dT dT ¼ je : m dx dx

ð5:8Þ

In (5.8) we have introduced the heat conductivity je of the electrons. Together with (5.4) we ﬁnd L=

je 9 ¼ ðkB =eÞ2 : rT 4

ð5:9Þ

The ratio L is referred to as the Lorenz number, named after Ludwig Lorenz. (A more accurate averaging yields the prefactor p2/3 instead of 9/4). The result in (5.9) is the famous Wiedemann-Franz law. Often this law is very useful for estimating the heat conductivity of the electrons in a metal, if the electrical conductivity, which can be measured relatively easily, is known. The explanation of the experimentally observed Wiedemann-Franz law was one of the successes of the Drude-Lorentz model. However, the model failed to predict the electrical and the thermal conductivity of the electrons separately, i.e., not just the ratio between both conductivities. But further and much more fundamental

62

5 Metals Obey the Rules of Quantum Statistics

difﬁculties appeared with respect to the speciﬁc heat of the electrons. Their contribution to the speciﬁc heat was found to be much smaller than expected from classical concepts. Again, the solution of this problem was provided by the new quantum mechanics and in particular by the application of the “Pauli principle”.

5.2

Quantum Statistics, Fermi Distribution

Again, it is the exact identity of the electrons as elementary particles, which makes them indistinguishable and which requires a new form of quantum statistics in order to obtain the probability distribution of the states. We have noted this already for the quantized lattice vibrations in terms of bosons. The quantum statistics deviate strongly from the classical (Maxwell-Boltzmann-) statistics, as we have discussed in Chap. 3 in the case of the Bose-Einstein distribution (3.2) of particles having vanishing or integer angular momentum (phonons and photons). However, now we deal with the electrons as elementary particles, having a half-integer angular momentum. In 1925 Wolfgang Pauli had formulated his famous exclusion principle, which states that each quantum mechanical state of a system can at most be occupied by a single electron. Here the important point is that an electron carries a half-integer angular momentum. In this way Pauli was able to explain the closure of the electron shells of the atoms. In 1926 Enrico Fermi from Italy and Paul Adrien Maurice Dirac showed independently from each other, that the application of the Pauli principle also leads to a new form of quantum statistics which today are referred to as Fermi-Dirac statistics. In general, Fermi-Dirac statistics are valid for elementary particles with a half-integer angular momentum, as is the case for the electrons. Such particles are referred to as fermions. Their angular momentum is also called spin. Because of the quantization of the direction of the angular momentum, the half-integer spin of the electrons can be oriented along only two possible directions. According to the Pauli principle, each state can be occupied for each of the two spin directions at most only by a single electron. Therefore, the many electrons in a metal must distribute themselves over many states with different energies within an energy band. In this way the electrons in an energy band must occupy sequentially the different “seats” with increasing energy. The last electron then must take the highest energy level. This highest energy level of the occupied states is referred to as the Fermi energy and the corresponding energy distribution of the electrons as the Fermi distribution (or Fermi-Dirac distribution). In the following we denote the Fermi energy by eF. The Fermi-Dirac distribution function f(e) is given by fðeÞ ¼

1 eðeeF Þ=kB T

þ1

:

ð5:10Þ

e is the particle energy and eF the Fermi energy (or the chemical potential). The function f(e) is shown in Fig. 5.2.

5.2 Quantum Statistics, Fermi Distribution

63

Fig. 5.2 Fermi distribution function: Because of the Pauli exclusion principle each quantum mechanical state in a crystal can be occupied at most by only one electron. At the temperature of zero Kelvin, for all energies up to the Fermi energy eF the Fermi distribution function has the value of one, and at eF it drops abruptly from one to zero. At a ﬁnite temperature T, the drop of the Fermi distribution function from one to zero is smeared out along the energy axis, and it occurs at the Fermi energy within an energy width of about kBT

Mathematically the Fermi distribution f(e) is a simple function of the electron energy. Between zero energy and the Fermi energy this function has a value of one, since in this energy interval the states can be occupied only by a single electron. At the Fermi energy the function abruptly drops from one to zero, having approximately the shape of a rectangle. However, this rectangular shape is exactly valid only at zero temperature. At a temperature T, different from zero, the drop of the Fermi function from one to zero is smeared out along the energy axis and happens within an energy interval of about kBT at the Fermi energy (Fig. 5.2). This energy width kBT has already appeared in our discussion of the thermal energy associated with the individual degrees of freedom of the normal modes of the crystal lattice. Now we return again to the speciﬁc heat of the electrons. Since the electrons in a metal must obey a highly restrictive prescription in the form of the Fermi distribution, nearly all electrons in the relevant energy band are energetically ﬁxed and cannot change their energetic state. If we arbitrarily pick out an electron, we see that all energetically neighboring states are already occupied. Hence, this electron can reach an unoccupied state only by means of a very large jump in energy, effecting a physical change in this way. However, in general such a large energy jump is impossible. Only for the few electrons near the Fermi energy is this possible, since they are energetically sufﬁciently close to states which are still unoccupied and which they can reach by thermal excitation. The fraction of the electrons in this exceptional energy interval is approximately given by kBT/eF. It is also exactly this fraction, which contributes to the speciﬁc heat of the electrons. We see that the speciﬁc heat in a metal must be reduced by this factor kBT/eF compared with the value expected from the classical theory and that, furthermore, it becomes proportional to the absolute temperature. Both results agree well with experiment. In this way it was quantum statistics which again removed the difﬁculties of the classical theories with the speciﬁc heat, in this case for the electrons. Using the relevant numbers for the monovalent metals, one ﬁnds for room temperature

64

5 Metals Obey the Rules of Quantum Statistics

approximately the value kBT/eF = 0.01. Compared with the Fermi energy, the transition from the occupied to the unoccupied states happens within a relatively narrow energy interval. Hence, the rectangular shape of the Fermi function mentioned above is still reasonably well preserved. Exactly the same argument as we have used above for the speciﬁc heat of the electrons also applies to the paramagnetism of the electrons in metals. This was pointed out for the ﬁrst time by Wolfgang Pauli, who explained in this way the relatively small value of the “paramagnetic susceptibility” in metals and its independence of the temperature. We will return to this subject in Chap. 10.

5.3

Fermi Surface

At this stage we recall that the states of the electrons in a crystal represent planar waves, as formulated for the ﬁrst time by Felix Bloch and Rudolf E. Peierls in their quantum mechanical theory. The planar waves are characterized by their wavelength and their propagation direction. Both qualities are combined in the “wave vector” k. Its direction indicates the propagation direction of the wave. Its absolute value k, referred to as the wave number, is equal to the inverse of the wavelength k except for the factor 2p: k = 2p/k. The state of the electrons in the crystal is not unequivocally identiﬁed by the energy alone. For the same electron energy the wave vectors of the matter waves can still point in all different directions in the crystal, in this way deﬁning different states in view of the Pauli principle. Hence, the Fermi distribution of the electrons must apply to all directions of the wave vectors separately. With increasing energy of the electrons, the magnitude of their wave vectors also increases. Hence, the Fermi energy as the maximum energy of the occupied states also corresponds to a maximum value of the wave vector. This maximum value is referred to as the Fermi wave vector kF, and all states up to kF are occupied by electrons. All states above kF remain unoccupied. From this discussion we see that our treatment of the quantum mechanical electron states in a crystal must be extended to a three-dimensional space of the wave vectors, the so-called k-space. Since the wave vector is proportional to the particle momentum, this space is also referred to as the momentum space. In this momentum space the Fermi wave vectors kF with their magnitudes and their directions represent a surface, the “Fermi surface”, for the particular material. The Fermi surface is one of the most important concepts for the discussion of the electronic crystal properties (Fig. 5.3). The Fermi energy eF and the Fermi wave vector kF are connected by the relation ε F = ħ2 kF2 / 2 m

ð5:11Þ

This relation is shown in Fig. 5.4. In the simplest case, if the influence of the crystal lattice on the de Broglie waves associated with the electrons is negligible, the Fermi surface has a spherical shape. We deal with this case to a good approximation in the monovalent metals, as for

5.3 Fermi Surface

65

Fig. 5.3 Fermi surface of copper. – The Fermi surface exists in momentum space, and it indicates up to which value all wave vectors are used up in order to accommodate the available electrons. In the simplest case the Fermi surface is a sphere, the radius of which is given by the Fermi wave vector kF. The picture shows the Fermi surface of copper for which, historically, deviations from the spherical shape were detected for the ﬁrst time. The short “necks” visible in eight different directions are a characteristic feature of the Fermi surface of copper

Fig. 5.4 The energy spectrum e(k) of the electrons is occupied up to the Fermi energy eF and up to the Fermi wave vector kF. (It is assumed that kBT > h) all phonon states up to the Debye frequency xD are occupied, and the number of phonons per state is proportional to T (as we see from the distribution (3.2)). Therefore, in this temperature range we expect for the electrical resistivity q that q * T. On the other hand, at temperatures much smaller than the Debye temperature h (T 0. The magnetic ﬁeld H is assumed to be oriented perpendicular to the x-direction. Equations (8.8) and (8.12) are referred to as ﬁrst and second London equation, respectively. In addition to Maxwell’s equations, they are valid in the case of superconductors and characterize these in contrast to other materials. From (8.15)

126

8 The Winner: Superconductors

Fig. 8.8 Dependence of the density of the super conducting electrons, ns, and of the magnetic ﬁeld, H, upon the distance from the interface between a normal (N) and a superconducting (S) region

we see, that the magnetic ﬁeld is shielded exponentially from the interior of the superconductor, and that the shielding occurs within a surface layer of thickness km. At T ! TC we ﬁnd ns ! 0, and, hence, km ! ∞. For many superconductors the magnetic penetration depth covers the range km = 40–60 nm. It strongly increases upon approaching the critical temperature TC. The magnetic penetration depth represents an important length, which is speciﬁc for each material. It plays an important role in many properties of superconductors. For example, because of the ﬁnite magnetic penetration depth, an accumulation of small superconducting grains, with the diameter of each grain being similar to the magnetic penetration depth, altogether only displays a strongly reduced Meissner effect, since the magnetically shielded volume fraction remaining in each grain is correspondingly reduced to a relatively small value. A superconducting circular current, similar to that flowing as a shielding current and causing the Meissner effect, can also serve to ﬁnd out in a simple experiment, if the electrical resistance in a superconductor is exactly zero, or if a ﬁnite residual resistance still remains. For this purpose the usual resistance measurement, based on the electric voltage drop along a current-carrying conductor, is not sufﬁcient, since the electric voltage can be too small to be detected by this method. However, instead of this conventional resistance measurement, one can also start a circular electric current in a superconducting ring by magnetic induction. As in an electric coil, the circular current then generates a magnetic ﬁeld, that only remains to be detected. Now the task consists in observation of how long the magnetic ﬁeld of the circular current can be detected. The longer the running time of the current, during which no reduction of the magnetic ﬁeld is observed, the closer the electrical resistance of the superconducting ring must approach zero. In 1961 the two Americans D. J. Quinn and W. B. Ittner performed an advanced version of such an experiment. By means of two sequentially deposited layers of lead they produced a thin superconducting tube of lead, and they then investigated the temporal decay of the magnetic flux trapped within the tube over a time of seven hours. From their

8.1 Meissner Effect, Magnetic Penetration Depth, London Theory

127

measurements at a temperature of 4 K, as the upper limit of the electrical resistivity of superconducting lead, they obtained the value 3.6 10−23 X cm. This value is about 17 powers of ten smaller than the resistivity of one of our best metallic conductors, copper, at room temperature. In addition to the magnetic penetration depth, a second characteristic length plays a fundamental role in superconductors: the “coherence length” n. This length indicates the smallest possible spatial distance, within which the property of superconductivity can vary appreciably. In the year 1950, the Englishman Alfred Brian Pippard was the ﬁrst to point out this spatial rigidity of superconductivity. Also in 1950, the two Russians Vitaly Lazarevich Ginzburg and Lew Dawidowitsch Landau developed another theoretical approach dealing with the question of the spatial coherence of superconductivity. The “Ginzburg-Landau theory” starts from an ansatz for the thermodynamic energy, in combination with the general concept of Landau of “higher-order phase transitions”, which are classiﬁed according to a speciﬁc mathematical scheme. The superconducting property is expressed in terms of a wave function w. Initially, it was felt that between the two characteristic lengths km and n the coherence length n is always larger than the magnetic penetration depth km. This resulted from the following considerations. Because of the ﬁnite extension of the coherence length n, a superconducting region cannot exist exactly up to the interface, which separates it from a normal region. Instead, it loses its superconducting property—and, hence, also its superconducting condensation energy—already at the distance n from this interface. This results in the positive interface energy a1 = (HC2/8p) n. However, from this we have to subtract the amount (HC2/8p) km, since within the magnetic penetration depth km no gain and, hence, no loss of condensation energy appears. Therefore, the wall energy a of an interface between a normal and a superconducting region is given by a ¼ ðHC 2 =8pÞðn km Þ:

ð8:16Þ

This role of the two lengths n and km is shown in Fig. 8.8. In its simplest form the Meissner effect is observed only if, in the nearest environment of the superconductor, the magnetic ﬁeld practically remains unchanged during the ﬁeld expulsion. We have such a case, if the shape of the superconductor is thin and long, and if its longitudinal direction is oriented parallel to the magnetic ﬁeld. In the other case, if, for example, the superconductor is shaped in the form of a thin plate which is placed perpendicularly within the magnetic ﬁeld, near the outer border of the plate, the magnetic ﬁeld is strongly enhanced because of the ﬁeld expulsion, and it can quickly become larger than the critical magnetic ﬁeld HC(T). Now the complete expulsion of the magnetic ﬁeld cannot be maintained, and magnetic flux will penetrate into the superconductor. As Landau proposed for the ﬁrst time in 1937, as a consequence, a new state is formed in which both normal domains carrying the local

128

8 The Winner: Superconductors

Fig. 8.9 Intermediate state of a superconducting lead ﬁlm of 9.3 µm thickness at 4.2 K in increasing (d – f) and decreasing (j – l) perpendicular magnetic ﬁeld at the following values of the magnetc ﬁeld: d 218 G; e 348 G; f 409 G; j 260 G; k 101 G; l 79 G. Normal domains are bright, superconducting domains are dark

magnetic ﬁeld HC and superconducting domains with zero local magnetic ﬁeld, exist next to each other. This new state is referred to as the “intermediate state”. Similar to all spatial systems of domains, the interface separating a normal from a superconducting domain is associated with a speciﬁc wall energy. As we see from (8.16), this wall energy is proportional to the length difference n − km. Since initially one had expected, that the wall energy is always positive, and that the formation of a domain wall always consumes energy, one had concluded that the coherence length n must be larger than the magnetic penetration depth km. In Fig. 8.9 we show the intermediate state of a superconducting lead ﬁlm with 9.3 µm thickness at 4.2 K for different values of the magnetic ﬁeld oriented perpendicular to the ﬁlm. The images were obtained magneto-optically by means of a polarization microscope. The normal domains are bright, and the superconducting domains are dark. The critical magnetic ﬁeld of lead at 4.2 K is 550 G (TC = 7.2 K).

8.2 Type-II Superconductors

8.2

129

Type-II Superconductors

However, eventually this picture was shaken. Already in the 1930s the ﬁrst perturbing signals came from the Low Temperature Laboratory of Leo Vasilyevich Shubnikov in Kharkov in the Ukraine, where experiments on superconductivity had been started at an early stage. Again and again experiments in particular with superconducting alloys, yielded results which could be explained only with great difﬁculties in terms of the existing ideas. In 1953 the decisive breakthrough was achieved by the young theoretical physicist Alexei A. Abrikosov in Moscow. At the University he was a roommate of Nikolay Zavaritzkii, who performed experiments with superconducting thin ﬁlms at the famous Kapitza Institute for Physics Problems in order to check the predictions of the Ginzburg-Landau theory. Up to this time one was only interested in the case where the length difference n − km and, hence, the wall energy, is positive. Now for the ﬁrst time Abrikosov and Zavaritzkii seriously discussed the possibility, that the length difference could also become negative, if the coherence length n were smaller than the magnetic penetration depth km. Based on the Ginzburg-Landau theory, Abrikosov calculated the critical magnetic ﬁeld for the case, where the difference n − km is negative, and he could demonstrate, that only in this case could good agreement with Zavaritzkii’s experimental data, obtained with particularly carefully prepared thin ﬁlms, be achieved. Hence, they were apparently dealing with a still unknown, new kind of superconductor. Abrikosov and Zavaritzkii called them the “second group”. Eventually, they were referred to as type-II superconductors (with n < km), whereas the superconductors with positive wall energy are now called type-I superconductors (with n > km). Subsequently, Abrikosov has theoretically analyzed the type-II superconductors in more detail using the Ginzburg-Landau theory and found that, in a magnetic ﬁeld, they can assume a new state, in which the superconductor is intersected by a regular lattice consisting of individual “magnetic flux quanta”. The famous Abrikosov flux-line lattice had been discovered. The state of the superconductor containing the flux-line lattice is referred to as the mixed state (Fig. 8.10). Associated with each magnetic flux line, a spatially conﬁned, local magnetic ﬁeld passes like a thread through the superconductor. This spatially highly conﬁned magnetic ﬁeld is generated, as in a magnetic coil, by superconducting circular currents flowing around the thread of the local magnetic ﬁeld. We will return to this magnetic flux line further below. Abrikosov completed this work in the year 1953. However, the proposed ideas were so novel that they were not accepted by Lew Dawidowitsch Landau, who was Abrikosov’s thesis advisor. However, two years later, similar issues appeared in the turbulent flow of superfluid helium at low temperatures. In this case the circulation of the flow is also subject to quantum conditions similar to those of the circular supercurrents associated with the magnetic flux quanta. Only after the American Richard Phillips Feynman had theoretically discussed quantized vortex lines in rotating superfluid helium in this context, was Landau satisﬁed. In this way it happened that Abrikosov’s paper was published only in 1957.

130

8 The Winner: Superconductors

Fig. 8.10 Superconducting mixed state characterized by a lattice of quantized magnetic flux lines, proposed for the ﬁrst time by Abrikosov. a Schematics. A total of nine magnetic flux lines are shown. Each flux line (like a thread carrying a magnetic ﬁeld) is surrounded by superconducting circular currents. b Experimental demonstration, by means of the Bitter decoration technique, of the Abrikosov lattice of magnetic flux lines in a plate of superconducting niobium with 0.5 mm thickness. The many dark spots mark the locations at which the individual magnetic flux lines reach the surface of the superconducting plate (U. Essmann)

In his lecture in Stockholm on December 8, 2003, on the occasion of receiving the 2003 Nobel Prize in Physics, together with Vitaly L. Ginzburg and Anthony J. Leggett, Abrikosov recalled these developments: I made my derivation of the vortex lattice in 1953 but the publication was postponed since Landau ﬁrst disagreed with the whole idea. Only after R. Feynman published his paper on vortices in superfluid helium, and Landau accepted the idea of vortices, did he agree with my derivation, and I published my paper in 1957. Even then it did not attract attention, in spite of an English translation, and only after the discovery in the beginning of the sixties of superconducting alloys and compounds with high critical magnetic ﬁelds, did there appear an interest in my work. Nevertheless, even after that the experimentalists did not believe in the possibility of (the) existence of a vortex lattice incommensurable with the crystalline lattice. Only after the vortex lattice was observed experimentally, ﬁrst by neutron diffraction and then by (Bitter) decoration, did they have no more doubts. Now there exist many different ways to get images of the vortex lattice.

Being asked why Abrikosov did not push more strongly for his spectacular novel results at the time, he gave the following answer: The true reason why at the time I did not insist more strongly in my theory, arose from the fact that then all this did not appear so important. Superconductivity was still being considered an exotic phenomenon far from any practical applications. Furthermore, I was already occupied with the extension of quantum electrodynamics to high energies, which appeared to me much more important.

Magnetic flux quanta only penetrate into the interior of a type-II superconductor, when the “lower critical magnetic ﬁeld” HC1 is reached. Below HC1 the Meissner

8.2 Type-II Superconductors

131

effect still exists, and the magnetic ﬁeld vanishes within the interior of the superconductor. The mixed state is established above HC1 up to the “upper critical magnetic ﬁeld” HC2. A convincing ﬁrst experimental conﬁrmation of the existence of the Abrikosov flux-line lattice in the mixed state has been given by Uwe Essmann and Hermann Träuble from the Max Planck Institute for Metals Research in Stuttgart in the year 1967. They succeeded in the imaging of the flux-line lattice at the surface of the superconductor by sprinkling a powder of small ferromagnetic particles onto the surface. Since the powder is attracted by the locations where the flux lines reach the surface, the powder accumulates at these locations forming small piles which decorate the individual flux lines (Fig. 8.10). This decoration method was used for the ﬁrst time in the year 1931 by the American Francis Bitter for imaging the domain structure of ferromagnetic materials, and since that time it has been referred to as the Bitter technique.

8.3

Magnetic Flux Quantum

Because of the prediction of type-II superconductors and of the magnetic flux-line lattice by Abrikosov, the Ginzburg-Landau theory has achieved great success. By describing the superconducting state of the electrons in terms of a macroscopic quantum mechanical wave function, this theory provided a simple explanation of a series of fundamental phenomena in the ﬁeld of superconductivity. The magnetic flux quantization is an important example. Within a superconductor magnetic flux can exist only in integer multiples of a smallest unit h/2e = 2.068 10−15 Vs, representing the magnetic flux quantum. The quantity h is Planck’s constant, and e is the charge of an electron. This quantum condition immediately results from the fact, that the macroscopic wave function describing the superconducting state must reproduce itself exactly, if the spatial coordinate point of the wave function is moved once around the enclosed magnetic flux region and is returned exactly to the starting point. As the smallest unit of magnetic flux, the flux quantum is very tiny. For example, in the magnetic ﬁeld of the earth one square centimeter is intersected by about one million flux quanta. In beautiful experiments in the year 1961 the two Germans Robert Doll and Martin Näbauer and independently also the Americans Bascom Deaver and William Fairbank demonstrated the quantization of the magnetic flux in a superconductor. By placing a tiny superconducting tube of only about 10 µm in diameter in a small magnetic ﬁeld oriented parallel to the axis of the tube, Doll and Näbauer were able to show that the magnetic flux within the small hollow cylinder was either zero or amounted to an integer multiple of the flux quantum speciﬁed above (Fig. 8.11). A more detailed explanation of the step structure shown in Fig. 8.11b is illustrated in Fig. 8.12. Here in part (a) the superconducting shielding current Is is plotted versus the magnetic flux density Be. Be is oriented parallel to the axis of the small superconducting cylinder. The magnetic flux pR2Be (R = cylinder radius) passing through the cross-sectional area of the cylinder is indicated in units of the

132

8 The Winner: Superconductors

(b) quartz filament

superconductor

trapped magnetic flux

(a)

B (Gauss)

Fig. 8.11 Experimental proof of the magnetic flux quantization in a superconductor. a A tiny superconducting tube with only about 10 µm diameter is cooled down in the presence of a small magnetic ﬁeld oriented parallel to the axis of the tube. Below the critical temperature TC the magnetic ﬁeld is turned off, and the magnetic flux trapped within the tube is measured. b The frozen-in magnetic flux displays a quantized step structure as a function of the magnetic ﬁeld B, since only integer multiples of the magnetic flux quantum (h/2e) are allowed within the tube. The Figure shows the observation of 0, 1, and 2 magnetic flux quanta, respectively. Without magnetic flux quantization, the data points would fall on the straight dashed line (R. Doll and M. Näbauer)

Fig. 8.12 Experimental demonstration of the magnetic flux quantization during entry of magnetic flux into a small superconducting cylinder. a Superconducting shielding current Is plotted versus the magnetic flux density Be oriented parallel to the cylinder axis. b Number n of the magnetic flux quanta within the cylinder plotted versus Be. c Superposition of the applied magnetic ﬁeld (solid arrows) and of the magnetic ﬁeld generated by Is (dashed arrows) at the three points 1–3 from (a). Further details are given in the text

8.3 Magnetic Flux Quantum

133

magnetic flux quantum uo ¼ h=2e. (The vector uo is oriented parallel to the flux density B). Initially, the shielding current Is prevents the entry of magnetic flux into the cylinder due to the Meissner effect. When the magnetic flux density has reached the value Be ¼ uo =ð2pR2 Þ, the shielding current compensates exactly half a flux quantum uo =2 within the cylinder (point 1). If Be is increased further, the shielding current Is reverses its sign (instead of increasing further), such that exactly one flux quantum uo exists within the cylinder (half of which is generated by Is; point 2). When Be continues to be increased, ∣Is∣ decreases again until (at point 3) the state with Is = 0 is reached at Be ¼ uo =ðpR2 Þ. During further increasing Be, this process repeats itself. In this way, the steps of the number n of the magnetic flux quanta within the cylinder are generated (Figs. 8.11b and 8.12b). In Fig. 8.12c the superposition of the applied magnetic ﬁeld (solid arrows) and of the magnetic ﬁeld generated by Is (dashed arrows) is shown schematically for the three points 1–3 of Fig. 8.12a. The entry of the magnetic flux quanta uo into the cylinder effects, that the shielding current Is and the kinetic energy associated with it remain limited. Theoretically, the magnetic flux quantization is demonstrated as follows. Representing the superconducting state by a macroscopic wave function (order parameter) wðr; t) ¼ jwðr; t)jeiuðr;tÞ

ð8:17Þ

with an amplitude ∣w(r, t)∣ and a phase uðr; tÞ, then the exact reproduction of the state after a complete path around a ﬁxed point in the superconductor requires that the ring integral along this path is I grad u ds ¼ n 2p

ð8:18Þ

where n is an integer. In a magnetic ﬁeld, the generalized particle momentum is m vs ¼ h grad u e A

ð8:19Þ

which yields I

ðm vs þ e AÞ ds ¼ n h

ð8:20Þ

Here A is the vector potential and ds a line element. Assuming that the superconductor is sufﬁciently thick, we can ﬁnd an integration path where vs = 0. Then applying Stokes’ law, we have I Z Z A ds ¼ curl A da ¼ B da ð8:21Þ

134

8 The Winner: Superconductors

Fig. 8.13 Structure of a single flux line. Local magnetic ﬁeld h, density of the superconducting electrons ns, and the circulating superconducting current density js as a function of the distance r from the axis of the flux line

(da is an area element), and with e* = 2e because of Cooper pairing, (8.20) yields R the magnetic flux quantization: B da ¼ n 2he ¼ n uo . Now we will look more closely at a magnetic flux line in a type-II superconductor, discussed for the ﬁrst time by Abrikosov (Fig. 8.13). In its center each flux line has a normal core, the radius of which is approximately given by the coherence length n. The local magnetic ﬁeld associated with the flux line reaches a maximum in the center of the line and decreases toward the outside. This decrease in the magnetic ﬁeld mostly takes place within a radius given by the magnetic penetration depth km. This spatial conﬁnement of the local magnetic ﬁeld is accomplished by means of circulating superconducting currents flowing around the center of the flux line within a radial distance, in the range between the coherence length n and the magnetic penetration depth km. The expression (h/2e), indicated above for the magnetic flux quantum in superconductors, is exactly half of the value (h/e) of the magnetic flux quantum, which we have dealt with in Chap. 7 in the context of the fractional quantum-Hall-effect. The reason for this half-value is the fact that superconductivity is based on the Cooper pairs, which consist of two electrons. This subject will be taken up next.

8.4 BCS Theory, Energy Gap

8.4

135

BCS Theory, Energy Gap

It has taken nearly 50 years since the discovery of superconductivity, until for the ﬁrst time a microscopic theory was proposed which could explain satisfactorily the underlying mechanism. In the year 1957 the three Americans John Bardeen, Leon Cooper, and Robert Schrieffer achieved the long-expected theoretical breakthrough. Their theory, the “BCS theory”, quickly became very famous. The question why it took so long to produce a theoretical explanation of superconductivity, can be answered relatively simply. The energy difference of the electrons between their normal and their superconducting state is extremely small and much smaller than the Fermi energy. On the other hand, the uncertainty in the calculation of the different individual contributions to the energy of the electrons in the crystal is much larger than the energy gain during the transition into the superconducting state. Hence, the theory had to ﬁnd the exact point leading to superconductivity. The BCS theory is based on the central idea that, at low temperatures, a speciﬁc attractive force is acting between two electrons. Because of this attraction, two electrons combine into pairs in a distinctive way and experience an energy reduction in the form of binding energy. Such a formation of pairs accompanied by a reduction in energy had been theoretically derived by Leon Cooper in 1956. Therefore, the electron pairs are referred to as “Cooper pairs”. According to the BCS theory, the attractive force leading to the formation of the Cooper pairs is due to the distortions of the crystal lattice near the individual electrons, i.e., due to the phonons. In this way, the otherwise expected repulsive force between two electrons is overcompensated. Already by the early 1950s strong indications for the important role of the crystal lattice in the mechanism of superconductivity were obtained, based on experimental observations of the “isotope effect”. One generally speaks of an isotope effect, when the result depends on the mass of the atomic nuclei at constant electric charge of the nuclei, i.e., on the number of neutrons in the atomic nuclei. By careful study of the different and specially prepared pure isotopes of various superconducting materials such as, for example, lead, mercury, and tin, it was found, that the critical temperature TC is inversely proportional to the square-root of the mass of the lattice atoms: TC 1=Ma

ð8:22Þ

with the exponent a = 0.5. Hence, the crystal lattice must play some role in superconductivity. During pair formation, two electrons with opposite spin always combine with each other. Therefore, the total spin of an individual Cooper pair is zero, and the Pauli principle does not apply in this case. Hence, all Cooper pairs can occupy the same quantum state, which is described in terms of a macroscopic quantum mechanical wave function. However, not all electrons participate in the formation of Cooper pairs and in the macroscopic quantum state. Instead, only the electrons from a distinct small energy interval near the Fermi surface are involved. We see

136

8 The Winner: Superconductors

Fig. 8.14 Experimental proof of the energy gap in a superconductor by means of the tunneling experiment of Giaever. a A superconducting electrode A and a normal electrode B are separated from each other by a thin, electrically insulating barrier C, such that the electric current flow across the barrier is only possible because of the quantum mechanical tunneling process. b Electric current I plotted versus the voltage V in the case when both electrodes are metals in the normal state. c Electric current I plotted versus the voltage V in the case when one metal electrode is superconducting. The electric current can start to flow only when the electrical potential difference between the two electrodes has reached the value of the energy gap

again, how the concept of the Fermi surface plays a central role. Mathematically, the subject of superconductivity confronts us with a “manybody problem”, requiring special techniques for its theoretical treatment. The development of these necessary new methods started about 60–70 years ago in conjunction with quantum ﬁeld theory. The ﬁrst steps of this theory can be found in a paper published in the year 1928 by the German Pascual Jordan and Eugene Paul Wigner from Hungary. One main result of the BCS theory was the prediction that, in the superconducting state, a gap appears in the energy spectrum of the electrons at the Fermi energy, in which no energy states exist which can be occupied by electrons. The energy gap vanishes above the critical temperature TC. Below TC the energy gap increases with decreasing temperature in a distinct way and reaches its maximum value at a temperature of zero Kelvin. In the year 1960, Ivar Giaever presented an impressive proof of this energy gap by means of his famous tunneling experiment (Fig. 8.14). For some time he had been fascinated by the quantum-mechanical tunneling effect. Giaever was born in Norway and as a young mechanical engineer was employed at General Electric in Schenectady in the American Federal State of New York. At the Rensselaer Polytechnic Institute near the location of his employment, he had heard in a lecture about the new BCS theory and its prediction of a gap in the energy spectrum of the electrons. On his way home after the lecture he had the idea that the energy gap must directly affect the electric current flow between a superconducting and a normal electrode, if the two electrodes are separated from each other by a thin, electrically insulating barrier. Because of this barrier, the electric current flow is possible only by means of the quantum mechanical tunneling process. Hence, this arrangement is referred to as a tunnel junction. During the propagation of particles, the tunneling effect is caused by the fact, that the wave function of the particle can still seep through a high wall and can reach an appreciable value at the other side. However, in our tunnel junction the

8.4 BCS Theory, Energy Gap

137

tunneling current cannot flow as long as no allowed energy states in the superconductor are available for the electrons coming from the other electrode, because of the energy gap. Only when the potential difference between both electrodes has reached the value of the energy gap because of the applied electric voltage does the electric current flow become possible. We have a similar result, if both electrodes are superconducting. Hence, it should be possible to determine the superconducting energy gap just by means of a simple measurement of the electric voltage and the electric current in a tunnel junction. Giaever’s experiments have impressively conﬁrmed these expectations. After this pioneering step, tunneling experiments with superconductors have become an important source of information about the physics of superconductors. The BCS theory has been conﬁrmed by many further experiments and has quickly found wide acceptance. There exists a long list of physicists, who had tried before without success to construct a microscopic theory of the mechanism of superconductivity. Among others, this list includes the names Felix Bloch, Niels Bohr, Léon Brillouin, Jakov I. Frenkel, Werner Heisenberg, Ralph Kronig, Lew Dawidowitsch Landau, and Wolfgang Pauli. The fact that it is the formation of Cooper pairs occupying a macroscopic quantum state, which leads to superconductivity, is also visible in the magnitude of the magnetic flux quantum discussed above. Since the Cooper pairs are composed of two elementary charges, the magnetic flux quantum (h/2e) is only half as large as would be the case if the underlying elementary particles carried only a single elementary charge, leading to (h/e).

8.5

Josephson Effect

Soon after Giaever had published the result of his famous tunneling experiment, a student in Cambridge, England was interested in the underlying tunneling process: Brian David Josephson. He was tutored by Alfred Brian Pippard, and in 1961/1962 he attended lectures by the American Philip Warren Anderson about the new developments in the theory of superconductivity. Josephson was highly impressed by the concept of superconductivity in terms of a macroscopic quantum phenomenon, which extended far beyond the range of validity in individual atoms or molecules. When he theoretically analyzed the details of the electric current flow through the barrier of a tunnel junction between two superconductors, as it had been used by Giaever, he derived two equations for the electric current and for the electric voltage, respectively, which are known since as the Josephson equations: Is ¼ IC sin v

ð8:23Þ

@v 2e ¼ V @t h

ð8:24Þ

138

8 The Winner: Superconductors

In (8.23) the current of Cooper pairs flowing without electrical resistance is described. Equation (8.24) indicates that an electric voltage V across the tunnel junction is always accompanied by an alternating supercurrent between both superconductors oscillating at a high frequency. The frequency of these Josephson oscillations increases proportionally with the electric voltage. Equations (8.23) and (8.24) are based on the concept that superconductivity represents a macroscopic quantum phenomenon, described by the wave function (8.17) with an amplitude ∣w(r, t)∣ and a phase uðr; tÞ: The current-phase relation (8.23) indicates that the supercurrent Is flowing across a weak contact is connected with the phase difference v ¼ u2 u1 between both sides of the junction. IC is the critical current of the junction geometry. The Josephson equations (8.23) and (8.24) can be derived in different ways. One derivation given by Richard Feynman starts with the time-dependent Schrödinger equation for the two wave functions w1 and w2 of the two superconductors, which are still separated initially, and then a coupling between both is added. Denoting the two sides of the Josephson junction by the indices 1 and 2, respectively, the Schrödinger equations of the wave function for each side are i h

dw1 ¼ l1 w1 þ K w2 dt

ð8:25Þ

i h

dw2 ¼ l2 w2 þ K w1 dt

ð8:26Þ

and

Here K is a coupling constant, and l1;2 the chemical potential (energy) on each side. With the potential difference V between both sides we have l1 ¼ e V=2; l2 ¼ e V=2

ð8:27Þ

Connecting the wave function (8.17) with the density ns of the superconducting electrons according to ∣w∣2 = ns, we write 1=2

w1 ¼ ns1 eiu1 ;

1=2

w2 ¼ ns2 eiu2

ð8:28Þ

and by insertion into (8.25) we obtain i h eiu1

1 1=2

2ns1

1=2 n_ s1 h ns1 u_ 1 eiu1 ¼

e V 1=2 iu1 1=2 n e þ K ns2 eiu2 2 s1

ð8:29Þ

Insertion into (8.26) yields an analogous result. In (8.29) we divide by 1=2 h eiu1 =2 ns1 and ﬁnd

8.5 Josephson Effect

139

i n_ s1 2 ns1 u_ 1 ¼

e V K 2ns1 þ 2ðns1 ns2 Þ1=2 eiðu2 u1 Þ 2h h

ð8:30Þ

Equalizing the real parts on both sides yields 2ns1 u_ 1 ¼

e V 2K ns1 þ ðns1 ns2 Þ1=2 cosðu2 u1 Þ h h

and u_ 1 ¼

e V K ðns2 =ns1 Þ1=2 cosðu2 u1 Þ 2 h h

ð8:31Þ

Analogous one ﬁnds from (8.26) u_ 2 ¼

e V K ðns1 =ns2 Þ1=2 cosðu2 u1 Þ 2 h h

ð8:32Þ

In the case ns1 ¼ ns2 ¼ ns we have u_ 2 u_ 1 ¼

e V h

ð8:33Þ

Setting ðu2 u1 Þ ¼ v and noting the Cooper pairs, e* = 2e, ﬁnally we obtain (8.24). This last result reminds us of the Einstein relation 2 eV = DE = hx. In Sect. 8.7 we return to relation (8.24), when we discuss its application in the form of the Josephson voltage standard. Equalizing the imaginary parts in (8.30), we obtain n_ s1 ¼

2K ðns1 ns2 Þ1=2 sin v h

ð8:34Þ

and analogous from (8.26) n_ s2 ¼

2K ðns1 ns2 Þ1=2 sin v h

ð8:35Þ

With n_ s1 ¼ n_ s2 being proportional to the current Is, we recover the current-phase relation (8.23). Josephson made both predictions in the year 1962. At ﬁrst, his theory was met by scepticism and hardly any understanding, as often happens with completely new ideas. As an example, Felix Bloch speaks of a conversation he had with the, also highly renowned, American theoretical physicist Chen Ning Yang:

140

(a)

8 The Winner: Superconductors

(b)

(c)

normal tunneling current pair current

tunneling current between supercond.

Shapiro steps

voltage (volt) Fig. 8.15 Josephson oscillation of the supercurrent between the superconducting electrodes of a tunnel junction in the presence of an electric voltage across the junction. a In a Josephson junction, the two superconducting electrodes A and B are only weakly coupled to each other, for example, by means of a thin, electrically insulating barrier C, which allows electric current to flow only because of the quantum mechanical tunneling process. b The frequency m of the Josephson oscillation of the supercurrent between the two electrodes increases proportionally with the electric voltage V across the junction. At a voltage of one volt the frequency is about 483,000 GHz. c Electric current I plotted versus the voltage V of a Josephson junction. The solid and the dashed curve show the tunneling current in the case of superconductivity and in the case of normal conductance, respectively. At zero voltage we see the Josephson pair current flowing without resistance up to its maximum value I0. During irradiation of the junction with microwaves the current-voltage characteristic displays the “Shapiro steps”, which are caused by the combined action of the Josephson oscillation within the junction and the microwaves

Yang told me that he could not understand it, and asked whether I could. In all honesty I had to confess that I could not either, but we made a deal that whoever of us ﬁrst understood the effect would explain it to the other.

By 1963 Josephson’s theory had already been conﬁrmed experimentally (Fig. 8.15). The second Josephson equation also emphasizes again, that it is the Cooper pairs with their two elementary charges, which lead to superconductivity. In this context of our discussion of the Josephson effect between two superconductors, only weakly coupled to each other, a brief note in the protocol of the board meeting at the German Bureau of Standards (Physikalisch-Technische Reichsanstalt) in Berlin-Charlottenburg in March 1926 is interesting historically. At that time, Albert Einstein was a member of the board, and during the meeting he made the following remark: “Of particular interest is the question, of whether the location of the junction joining two superconductors also becomes superconducting”. The remark by Einstein at the board meeting of the Reichsanstalt is connected with the fact that, at the time, for explaining superconductivity he had proposed that it is caused by molecular conducting chains. In his commemorative address for Kamerlingh Onnes in 1923, Einstein discussed the state of superconductivity as follows:

8.5 Josephson Effect

141

So it appears unavoidable that the superconducting currents are carried by closed molecular chains (conducting chains), the electrons of which incessantly experience cyclical exchanges. Therefore, Kamerlingh Onnes compares the closed currents in superconductors with Ampère’s molecular currents. [ … ] It may appear unlikely, that different kinds of atoms can combine to form conducting chains. Hence, the transition from one superconducting metal to another is perhaps never superconducting.

Motivated by these ideas of Einstein, in 1932 Walther Meissner together with Ragnar Holm, working for the Siemens company in Berlin in its research laboratories, carried out experiments concerning the contact between two superconductors. They performed the measurements on superconducting tin (Sn) and lead (Pb) and investigated Sn-Sn, Pb-Pb, and Sn-Pb contacts. Meissner and Holm reported their results in an article in Zeitschrift für Physik and concluded: Between superconductors from the same or from different materials a superconducting contact is possible without welding both materials together. During entry of superconductivity the resistance of the contact layer also vanishes.

Hence, the model of the molecular conducting channels, proposed by Einstein, had been disproved. In this case, motivated by the ideas of Einstein, for the ﬁrst time the subject of thin contacts or micro-bridges between two superconductors, which subsequently would gain great signiﬁcance, was brought up. However, it took another 30 years, until Brian David Josephson in 1962 ﬁnally answered these questions.

8.6

Motion of the Magnetic Flux Quanta

Again and again, the scientists were concerned with the question whether, in a superconducting ring, the supercurrents really flow forever, or whether they decay perhaps extremely slowly. In the beginning of the 1960s, this question became very urgent, when at the Bell Laboratories Bernd T. Matthias, working together with Theodore Geballe, discovered the new superconducting niobium alloys Nb3Sn and NbZr. In this context we note that for a long time superconductor research had concentrated primarily on high-purity metals. An early exception of this trend is a brief report by Walther Meissner from 1929 dealing with the observation of superconductivity in a wire of copper-sulﬁde (CuS) with a critical temperature TC = 1.6 K. Subsequently, this discovery may have led Enrico Fermi at the University of Chicago to urge two young postdocs, Bernd Matthias and John Hulm, to start a wide search for more superconductors. Returning to Nb3Sn and NbZr, the tests performed by Gene Kunzler indicated promising high values of the critical electric current density and of the critical magnetic ﬁeld in these materials. The further experiments, performed in particular by the Korean Young Kim, showed that there exists a “critical state”, above which in a superconducting ring the current always decreases. The crucial idea then came from Philip W. Anderson, when he recognized that this process does not set in

142

8 The Winner: Superconductors

discontinuously, but is caused by the motion of the magnetic flux quanta. The concepts of flux creep and flux flow were born. This highly important consequence of the magnetic flux quanta (in addition to their influence on the magnetic properties) is due to the following. If, under the influence of a force, the flux quanta move within the superconductor, an electric ﬁeld and, hence, an electric voltage is generated. This “flux-flow voltage” is proportional to the velocity and to the number of the moving flux lines. An electric current of density j in the superconductor causes the Lorentz force f L ¼ j uo acting on the flux quanta. It is oriented perpendicular to the direction of the electric current and to the magnetic ﬁeld of the flux lines. The Lorentz force can cause a motion of the magnetic flux lines which, in turn, generates the electric ﬁeld E E ¼ vu B:

ð8:36Þ

vu is the velocity of the flux lines. This electric ﬁeld is always oriented perpendicularly to the motional direction and to the magnetic ﬁeld of the magnetic flux lines. Hence, in the case of the Lorentz force the electric ﬁeld and the electric current have the same direction, such that the flux-line motion in the superconductor causes electric losses. The process of the flux-line motion follows the (here simpliﬁed) force equation j uo g vu ¼ 0:

ð8:37Þ

Here g vu is the dissipative contribution and η a damping constant. In (8.37) the forces are given per unit length of the flux lines. From (8.36) and (8.37) we obtain the flux-flow resistivity qf ¼ uo B=g.

ð8:38Þ

It is exactly this mechanism, which always limits the electric current flow without electrical resistance and without losses in a superconductor. Therefore, it is of utmost interest, to prevent this process of flux-line motion as much as possible. In this last discussion we have simpliﬁed the situation by neglecting in (8.37) the effects of the pinning forces and a force component which causes the Hall-effect during the motion of the flux lines. In Fig. 8.16 as an example, we show the flux-flow voltage as a function of the electric current in a niobium foil for different values of the magnetic ﬁeld oriented perpendicular to the foil. Thickness of the foil = 18 µm, width of the foil = 4 mm, T = 4.22 K. The electric resistance ratio R(295 K)/R(4.2 K) was 620, where R(4.2 K) was measured in a perpendicular magnetic ﬁeld of 4000 G. The voltage sets in at a ﬁnite critical current and then shows an upward curvature, after which it increases linearly with increasing current as expected from (8.37) and (8.38). The ﬁnite critical current results from the pinning forces due to the spatial inhomogeneity of the superconductor, hindering as pinning centers the motion of the magnetic flux

8.6 Motion of the Magnetic Flux Quanta

143

Fig. 8.16 Flux-flow voltage versus the electric current in a niobium foil of 18 µm thickness and 4 mm width for different perpendicular magnetic ﬁelds. T = 4.22 K; TC = 9.2 K

lines. The slope of the linear curve sections represents the flux-flow resistance and increases with increasing external magnetic ﬁeld. In Fig. 8.17 we show schematically the speciﬁc flux-flow resistance qf plotted versus the external magnetic ﬁeld H. Initially, qf increases linearly with increasing H, then turning into a much steeper curve section, which near the upper critical magnetic ﬁeld HC2 approaches the normal value qn of the speciﬁc resistance. The motion of a magnetic flux quantum in a superconductor resulting in the flux-flow resistance and in the destruction of superconductivity is an example of a general principle of nature, according to which the generation and the motion of a local defect through an otherwise homogeneous system leads to major macroscopic effects. In other words: here a little cause can achieve a major effect. In Chap. 12 we will discuss a similar example, in which the generation and the motion of individual dislocations through an otherwise homogeneous crystal, affects the mechanical

144

8 The Winner: Superconductors

Fig. 8.17 Schematics of the speciﬁc flux-flow resistance qf in a type-II superconductor plotted versus the magnetic ﬁeld for different temperatures (T1 > T2 > T3 ; qn = normal resistance)

properties and results in the deformation of the crystal at unexpectedly small values of the mechanical tension. The motion of local vortices within a supra-fluid also plays a role in the dynamics of the neutron stars or pulsars. These stars rotate having a rotational frequency above 1/sec. However, one observes that for a long time this rotation becomes slower, until abruptly the rotational speed jumps to a higher value. Today this behavior is explained by the motion and abrupt jumps of local vortices.

Material scientists have been taking great pains to pin the magnetic flux lines at speciﬁc locations by introducing “pinning centers” into the superconductor. In this way, one hopes that the flux lines are not moving any longer under the influence of the Lorentz force, or that this motion and the electric losses only start to appear at electric currents as high as possible. In recent years great effort has been devoted to this subject in material science and metallurgy. These developments were motivated by the interest in the possibilities for the technical applications of superconductivity. Next we will turn to the technical applications and look at a few examples.

8.7

Technical Applications

For the applications of superconductivity in electronics and microelectronics the magnetic flux quantization and the Josephson effect are of central interest. Both phenomena are intimately connected with the nature of superconductivity as a macroscopic quantum phenomenon and with the description of the state of the Cooper pairs in terms of a quantum mechanical wave function. Here the limitation of the quantum-theoretical concepts to atomic and subatomic objects, is suspended. Instead, these concepts are directly technically utilized in devices and instruments. An electronic instrument used today in many different ways is the “SQUID” (abbreviated from Superconducting Quantum Interference Device). It is based on the magnetic flux quantization and the Josephson effect. A small closed superconducting loop is interrupted by two Josephson junctions connected in parallel. If the loop is penetrated by magnetic flux, within the loop the magnetic flux can exist only in units of integer multiples of a magnetic flux quantum. This quantum

8.7 Technical Applications

145

condition is satisﬁed by means of the induction of a circulating superconducting shielding current within the loop, in such a way that the generated additional magnetic flux in the loop, in combination with the external magnetic flux, exactly supplement each other to yield an integer multiple of a magnetic flux quantum (similar as it is shown in Fig. 8.12c). As a result one observes an exactly periodic modulation of the shielding current within the loop as a function of the external magnetic ﬁeld, where the length of the magnetic period corresponds exactly to one magnetic flux quantum in the loop. It is important that the circulating shielding current should always be added to an external electric current which is also flowing through the device. As a consequence, the measured electric voltage along the loop conﬁguration with the two parallel Josephson junctions also displays a periodic modulation. Since even a small fraction of a single modulation period of the magnetic ﬁeld can be resolved during the measurement of the electrical resistance, an extremely high sensitivity of the magnetic ﬁeld measurement is achieved. Today, the fabrication of SQUIDs is carried out usually by means of thin-ﬁlm and integrated circuit technology. As sensors for detecting magnetic ﬁelds, SQUIDs have the highest sensitivity which can be reached today. This fact results in many of the applications of SQUIDs, for example, in the ﬁeld of research or nondestructive material testing. Interesting applications are also found in medical diagnostics for detecting the magnetic ﬁelds generated by the electric currents from cardiac activity or in the brain. In this way, the new ﬁelds of magneto-cardiography and magneto-encephalography developed only because of extremely sensitive SQUIDs. For example, today instruments with a total of up to 275 SQUID channels are available for brain research, where the channels with the individual sensors are arranged in a three-dimensional way around the head of the test person or of the patient (Fig. 8.18). Very recently, highly miniaturized SQUIDs have been used also in SQUID-scanning microscopes. At an extremely high magnetic-ﬁeld sensitivity, these instruments achieve a spatial resolution as high as only a few µm, such that individual magnetic flux quanta in a superconductor can be nicely imaged. (In Fig. 9.8 of Chap. 9 we present an application of a SQUID-scanning microscope.) Presently, small spin systems in nano-particles are moving to the center of attention. The newest development of this SQUID instrumentation concerns the fabrication of ultra-small devices on sharp nano-scale tips (nano-SQUID-on-tip). By depositing superconducting lead or niobium at the apex of hollow quartz tubes, SQUID loops with an effective diameter of only 160 nm or even less than 100 nm could be achieved. It is estimated that the signal of a single electron spin located 10 nm below a SQUID-on-tip loop can be resolved with a spatial resolution of about 20 nm. We discussed above, that an electric voltage drop at a Josephson junction is always associated with a high-frequency oscillation of the supercurrent flowing between the two electrodes of the junction, as predicted by the second Josephson equation (8.24). Here an electric voltage of 10−3 V corresponds to an oscillation frequency of 483.6 GHz (Gigahertz). Vice versa, distinctly sharp electric voltage plateaus result at the current-carrying Josephson junction, if the junction is

146

8 The Winner: Superconductors

Fig. 8.18 Magneto-encephalography. Left: Whole system with the test person carrying the helmet containing the SQUID magnetic-ﬁeld sensors, within a magnetically shielded chamber. Right: View into the helmet having an arrangement of 151 SQUID sensors (Photos MEG International Services Ltd.)

irradiated with a high-frequency electromagnetic wave such as a microwave, for example. Then the magnitude of the voltage plateau is unequivocally ﬁxed by the frequency of the irradiating electromagnetic wave because of the second Josephson equation. This exact quantum condition between a frequency and an electric voltage, in combination with the fact that frequencies can be determined extremely accurately, was the reason why, since January 1, 1990, the legal deﬁnition of the electric voltage unit established by the National Bureaus of Standards is based on the Josephson effect in the form of the “Josephson voltage standard”. Ofﬁcially, a voltage of one volt corresponds to a frequency 483597.9 GHz. In Chap. 7 we discussed another quantum deﬁnition of an electric unit, namely the von-Klitzing effect for the deﬁnition of the unit of electrical resistance. Together with the Josephson oscillation as the combining mechanism between an electric voltage and a frequency, two sides of the famous quantum triangle consisting of current, voltage, and resistance, for the deﬁnition of the electric units, are now completed. The remaining third side, yielding the connection between an electric current and a frequency, is presently the subject of ongoing research in different laboratories. Here the goal is to deﬁne the electric current in terms of the frequency of transfer of individual electrons. With the example of the Josephson voltage standard we will conclude our discussion of the ﬁeld of Josephson electronics and Josephson technology, which today is already well developed for measuring electronics. For many years the relatively low values of the critical magnetic ﬁelds and of the critical currents had prevented the technical high-current applications of superconductivity in energy technology and in electric machinery. This changed only in

8.7 Technical Applications

147

the 1960s, when new superconducting materials with higher values of the critical electric current density and of the upper critical magnetic ﬁeld HC2 became known. Then the compounds NbTi with TC = 9.6 K and Nb3Sn with TC = 18 K, technically became highly relevant. Among the classical superconductors, thin layers of the compound Nb3Ge showed the highest critical temperature with TC = 23.2 K. For the fabrication of wires. special drawing procedures and different mechanical processing stages with an optimized combination of heat treatment and cold-work were developed. Particularly successful were the “multiﬁlamentary wires”, where many thin ﬁlaments of the superconducting material are imbedded within a copper matrix. This technique ensures that, during the breakdown of superconductivity, because of overloading a certain ﬁnite electrical conductivity still remains, and that on the other hand there exists a sufﬁciently large number of pinning centers in order to pin the magnetic flux quanta in the superconductor. One of the main applications of technical superconductors can be found in magnetic coils. Today, superconducting magnets are used in large numbers in research laboratories (Fig. 8.19). Particularly large versions serve as beam-guiding magnets of particle accelerators and are also important components of the associated particle-detector systems. Since a few years, the largest superconducting accelerator plant worldwide, the Large Hadron Collider (LHC), is operating at the European Nuclear Research Center (CERN) in Geneva. It is placed within a circular tunnel of 27 km length and, at full operation, accelerates protons up to energies of 7000 GeV. For beam guidance, a total of more than 1600 superconducting magnets, constructed from NbTi, are used. Most magnets weigh more than 27 t. For this more than 7000 km of NbTi wire were needed. In addition, more than 3500 superconducting correcting magnets are used. Only the correct adjustment of all magnets allows the storage of highly accurate proton beams, as they are required by the LHC. During operation, a total of 31,000 t material must be cooled down to 1.9 K. This requires 12 million liters of liquid nitrogen and 700,000 liters of liquid helium. (In Chap. 1 we had mentioned the extremely large cryogenic facilities installed at the LHC.) Another large-scale application of superconducting coils is found in the case of the magnetically levitated train. In particular the Japanese JR-Maglev project recently has seen promising advances. In 2015 during tests, a speed above 600 km/h has been reached. Superconducting coils generating magnetic ﬁelds of about 5 T are mounted within the train. Electrically well conducting loops are imbedded along the gliding track, in which strong eddy currents are generated during train motion. According to Lenz’ rule, the magnetic ﬁeld of the eddy currents repels the ﬁeld of the coils above. In this way the levitating force is generated. Since this repulsion becomes sufﬁciently strong only above a certain minimum speed, initially the train has to move on wheels, which are retracted when this speed is reached. During the past 15 years superconducting magnets for medical nuclear spin tomography have developed into the most important market of superconductor technology. This started in the beginning of the 1980s when the health authorities worldwide approved the use of nuclear spin tomography in medical diagnostics. Presently, the annual turnover of industry in this ﬁeld amounts to 2–3 billion €.

148

8 The Winner: Superconductors

Fig. 8.19 Superconducting magnetic coils. a Commercially available coil for research purposes. The coil is wound from niobium-titanium (NbTi) wire and can generate a magnetic ﬁeld of up to 9 T, corresponding to about one million times the magnetic ﬁeld of the earth (Oxford). b Superconducting model coil with its test set-up for a toroidal magnetic ﬁeld during lowering into the cryo-container of an experimental plant at the German Research Center Karlsruhe. The experimental plant serves to develop the technology of magnetic plasma conﬁnement for the nuclear fusion process. The outer dimensions of the oval model coil are 2.55 m 3.60 m 0.58 m. During its operation an electric current of 80,000 A is flowing through the coil. The total coil set-up weighs 107 tons and must be cooled down to 4.5 K. The available inner diameter and height of the cryo-container is 4.3 m and 6.6 m, respectively (Research Center Karlsruhe KIT)

Since, in a superconducting coil, direct current can flow without any losses for a practically arbitrarily long time, such coils offer an interesting possibility for the storage of electrical energy, in particular for the handling of short interruptions of the electric power supplied. Therefore, at present the development of superconducting magnetic energy-storage systems is pursued intensively. Nuclear fusion as a long-term option for a source of energy must rely necessarily, for energetic reasons, on superconducting coils to generate the magnetic ﬁelds needed for the conﬁnement of high-temperature plasma, in which the nuclear fusion process occurs. Hence, the largest superconducting magnet systems are developed presently for application in nuclear fusion reactors. Once technical superconductors with their highly improved superconducting material properties became available, then in the 1970s the investigation of the basic principles of superconducting electric power cables, based on the classical

8.7 Technical Applications

149

superconductors and cooled with liquid helium, had already been started. In this context several pilot projects were carried out worldwide. Today, about 95% of the electric power is transmitted using alternating current high-voltage open-air power lines. Because of their relatively low construction and repair costs, they have distinct advantages. The possible operation of superconducting electric power cables is particularly useful at such locations, where open-air power lines are ruled out as, for example, in regions with very high population density. Because of the discovery of high-temperature superconductivity, which we will discuss in the following Chap. 9, this high-current application of superconductivity has also received a strong impetus.

Chapter 9

The Big Surprise: High-Temperature Superconductivity

Abstract The discovery of high-temperature superconductors in 1986 started worldwide tremendous research activities which quickly resulted in the preparation of superconductors with a critical temperature above 130 K. These cuprate superconductors are highly anisotropic, with superconductivity residing in the copper-oxide planes. Initially, the granular structure of the ceramic materials needed to be optimized. Much progress was achieved by fabricating epitaxial ﬁlms. The symmetry of the wave function of the Cooper-pair condensate represents an important issue. Today, the Josephson effect of a single grain boundary is used in SQUIDs. The intrinsic Josephson effect in small multi-layer crystals is explored as a source of terahertz radiation. Major events were the discovery of superconductivity in MgB2 in 2001 and in iron-pnictides in 2008.

9.1

Cuprate Superconductors

In April 1986 the German Johannes Georg Bednorz together with the Swiss Karl Alexander Müller submitted a paper for publication in the Zeitschrift für Physik with the title “Possible High TC Superconductivity in the Ba-La-Cu-O System”. Both worked at the IBM Research Laboratory in Rüschlikon near Zurich. In compounds of barium, lanthanum, copper, and oxygen, with decreasing temperature, they had observed an abrupt drop in the electrical resistance by at least three orders of magnitude, with the drop starting at about 35 K. The two scientists presumed that they were dealing with a new kind of superconductivity. Because the superconductivity appeared to set in at a temperature, which was up to 12 K higher than the highest recorded value of the critical temperature of 23.2 K known at the time (since 12 years) for the compound Nb3Ge, caution and scepticism was called for. Therefore, the authors arranged with the editor of the Zeitschrift für Physik to hold the paper until a clear proof of the superconductivity was provided by an experimental demonstration of the Meissner effect. As we saw in Chap. 8, the Meissner effect represents the characteristic ﬁngerprint of superconductivity. The

© Springer Nature Switzerland AG 2019 R. P. Huebener, Conductors, Semiconductors, Superconductors, Undergraduate Lecture Notes in Physics, https://doi.org/10.1007/978-3-030-31420-0_9

151

152

9 The Big Surprise: High-Temperature Superconductivity

Meissner effect was then, indeed, conﬁrmed also for the Ba-La-Cu-O system, and Bednorz and Müller released their submitted paper for publication. Initially, Bednorz and Müller mostly faced scepticism. However, this lasted only a short time. Already by the end of 1986 their results had been conﬁrmed at the University of Tokyo and only a little later at the University of Houston in the American Federal State of Texas. Then in 1987, Paul Ching-Wu Chu, Maw- Kuen Wu, and their co-workers in Houston succeeded in another sensational advance. In a modiﬁcation of the original oxides, in which the larger lanthanum atom was replaced by the smaller yttrium atom, they observed an enormous increase in the critical temperature up to 92 K. Now the investigations into the “high-temperature superconductors” developed a breathtaking speed worldwide in many groups. The critical temperature of 92 K for the, just-discovered, new material YBa2Cu3O7 (abbreviated YBCO) is still distinctly higher than the boiling point of 77 K for liquid nitrogen. Therefore, the relatively expensive liquid helium as a cooling medium can be replaced by the much cheaper liquid nitrogen. In many places the increasingly hectic rush was so great, that temporarily new results were reported in daily newspapers such as, for example, in The New York Times, with an exact indication of the day and the hour they had been achieved. Perhaps the ﬁrst crucial point was the marathon session at the Spring Conference of the American Physical Society of March 18, 1987 in the Hilton Hotel in New York City, which lasted far beyond midnight and subsequently was accurately called the “Woodstock of Physics”. The discovery of high-temperature superconductivity by Bednorz and Müller resulted in an explosive growth worldwide of research and development in the ﬁeld of superconductivity. With respect to the international reaction, this discovery can be compared with the discovery of X-rays in 1895 by Wilhelm Conrad Röntgen or with the ﬁrst observation of nuclear ﬁssion in 1938 by Otto Hahn and Fritz Strassmann. It is estimated that, until the beginning of the year 2001 a total of about 100000 scientiﬁc papers on high-temperature superconductors had been published, since their discovery (Fig. 9.1). In particular the lecture given by Bednorz during the ceremony in which the Nobel Prize was awarded to him together with K. A. Müller on December 8, 1987 in Stockholm, gives a vivid and enlightening description of the path leading to their discovery of high-temperature superconductivity. We will quote a few passages from this lecture: “….We started the search for high-TC superconductivity in late summer 1983 with the La-Ni-O-System.” – Bednorz then talks about various steps, during which the nickel and the lanthanum were replaced by other elements, but without success. Then he continues: “The resistance behavior changed in a way we had already recorded in the previous case, and at that point we started wondering whether the target at which we were aiming really did exist. Would the path we decided to embark upon ﬁnally lead into a blind alley?” “It was in 1985 that the project entered this critical phase, and it probably only survived because the experimental situation, which had generally hampered our efforts, had been improved. The period of sharing another group’s equipment for resistivity measurements came to an end. … Thus the measuring time was transferred from late evening to normal

9.1 Cuprate Superconductors

153

liquid CF4

liquid N2

liq. H2

under high pressure

year Fig. 9.1 Critical temperature TC plotted versus the year of discovery of different superconductors. The steep branch of the curve on the right-hand side shows the different high-temperature superconductors. The entries marked with an asterisk indicate where the critical temperature could be increased further under high pressure. (C. W. Chu) working hours.” – After a brief summary of the further experiments Bednorz continues “…. But again, we observed no indication of superconductivity. The time to study the literature and reflect on the past had arrived.” “It was in late 1985 that the turning point was reached. I became aware of an article by the French scientists C. Michel, L. Er-Rakho, and B. Raveau, who had investigated a Ba-La-Cu oxide with perovskite structure exhibiting metallic conductivity in the temperature range between +300 and −100 °C….. In the Ba-La-Cu oxide with a perovskite-type structure containing Cu in two different valencies, all our concept requirements seemed to be fulﬁlled. I immediately decided to proceed to the ground-floor laboratory and start preparations for a series of solid solutions. “–Then there occurred a few interruptions of the experiments, and Bednorz continues in his lecture”…. in mid-January 1986, I recalled that when reading about the Ba-La-Cu oxide it had intuitively attracted my attention. I decided

154

9 The Big Surprise: High-Temperature Superconductivity

to restart my activities by measuring the new compound. When performing the four-point resistivity measurement, the temperature dependence did not seem to be anything special when compared with the dozens of samples measured earlier. During cooling, however, a metallic-like decrease was ﬁrst observed, followed by an increase at low temperatures….. My inner tension, always increasing as the temperature approached the 30 K range, started to be released when a sudden resistivity drop of 50% occurred at 11 K. Was this the ﬁrst indication of superconductivity?” “Alex (Müller) and I were really excited, as repeated measurements showed perfect reproducibility and an error could be excluded. Compositions, as well as the thermal treatment, were varied and within two weeks we were able to shift the onset of the resistivity drop to 35 K. This was an incredibly high value compared with the highest TC in the Nb3Ge superconductor.”

The substances of the discovered new class of the “cuprate superconductors” (Fig. 9.2) are oxides, which crystallographically have perovskite structure. The

Fig. 9.2 Crystal structure of different cuprate superconductors. At the six corners of the bright octahedrons or at the ﬁve corners of the bright pyramids there are oxygen atoms. The centers of the octahedrons, or of the basic square areas of the pyramids, are occupied by copper atoms. (IBM)

9.1 Cuprate Superconductors Table 9.1 Critical temperatures of different high-temperature superconductors

155 Compound

TC (K)

La2−xSrxCuO4 YBa2Cu3O7−x Bi2Sr2Ca2Cu3O10 Tl2Ba2Ca2Cu3O10+x HgBa2Ca2Cu3O8+x

38 92 110 125 133

most prominent structural element are copper-oxide (CuO2) planes, in which copper and oxygen atoms are arranged alternately, in this way forming a two-dimensional lattice. The elementary building blocks, from which the cuprate superconductors are assembled periodically in all three spatial directions, (the crystallographic unit cells), contain a different number of copper-oxide planes, depending upon the particular compound. Based upon the different possible chemical composition, one distinguishes between ﬁve main families of the cuprate superconductors, the parent compounds of which, together with their critical temperature TC, are listed in Table 9.1. The electrical and, in particular, the superconducting properties of these cuprates are determined by the copper-oxide planes and depend sensitively on their doping with electric charge carriers. In their undoped state the cuprates are electrical insulators, in which the elementary magnets of the copper atoms in the CuO2 planes are alternately oriented opposite to each other. Superconductivity is only observed if the electron concentration in the CuO2 planes is reduced by means of introducing positive holes into the electronic system (“hole doping”). This hole-doping can be achieved, for example, by the extraction of oxygen. Since, on the other hand, superconductivity only appears within a relatively narrow range of the doping concentration, during material preparation the oxygen concentration must be carefully controlled. The values of the critical temperature given in Table 9.1 correspond to the case of optimum doping with holes. The compound HgBa2Ca2Cu3O8+x with TC = 133 K shows the highest critical temperature observed up to now under normal pressure. Under high pressure the critical temperature of this compound reaches the even higher value of TC = 164 K. In addition to the cuprates, which become superconducting after hole doping, a few compounds have been found, showing superconductivity only after doping with additional electrons, i.e., with negative charges. However, in this case the doping-concentration range required for superconductivity is narrower, and the critical temperature is much lower, compared with the hole-doped compounds. The layered crystal structure of cuprate superconductors with the dominating role of the CuO2 planes (Fig. 9.3), results in an extremely strong dependence of all electrical and thermal transport properties upon the direction within the crystal. For example, in the normal state the electrical resistivity perpendicular to the CuO2 planes is up to several orders of magnitude larger than it is parallel to these planes. In many respects, the materials show quasi two-dimensional behavior. In the normal state of the cuprates, the temperature dependence of the physical properties

156

9 The Big Surprise: High-Temperature Superconductivity

Bi 1,5 nm

c

b

1.5 nm c b Fig. 9.3 High-resolution electron-microscopic image of the cuprate superconductor Bi2Sr2CaCu2O8+d. The two arrow-heads at the upper left show two rows of bismuth atoms. At the bottom, the direction of the crystallographic b- and c-axis is indicated. The c-axis is oriented perpendicular to the CuO2 planes of the cuprate. (O. Eibl)

such as electrical resistance, the Hall effect, as well as the Seebeck and Peltier effects, strongly deviates from the behavior usually observed in metals. In the high-temperature superconductors, the coherence length n, which characterizes the spatial rigidity of the superconducting properties, is much smaller than in the classical superconductors and has a similar magnitude to the dimensions of the crystallographic unit cell. We are dealing with extreme type-II superconductivity. Therefore, these materials are extremely sensitive against atomic defects and grain boundaries, both of which act as pinning centers for magnetic flux quanta (Fig. 9.4). The upper critical magnetic ﬁeld HC2 is up to more than 100–200 times

9.1 Cuprate Superconductors

157

(a) 0.72 mA

(b) 0.91 mA

(c) 1.2 mA

(d) 2.2 mA

(e) 8.7 mA

I

e - beam

Fig. 9.4 Granular structure of one of the ﬁrst prepared thin layers of the cuprate superconductor Y1Ba2Cu3O7. The layer is 30 µm wide and runs horizontally. The arrow-heads on the right-hand side mark the upper and the lower edge of the layer, respectively. Bright regions indicate the locations in which electrical resistance appears within the layer during electric current flow. The dark regions are superconducting. From (a) to (e) the electric current was increased successively from 0.7 mA at (a) up to 8.7 mA at (e). The images show the pronounced spatial inhomogeneity of the layer, having large spatial fluctuations of the local critical electric current density. The images were obtained using the method of low-temperature scanning electron microscopy. The temperature was 53 K

larger than the highest values for the classical superconductors. One of the ﬁrst questions which had to be answered for the newly discovered materials, concerned the issue of whether the formation of Cooper pairs is fundamental to superconductivity, similar to the classical superconductors. For cuprate superconductors, this question of pair formation had received a clear positive answer early on. Here deﬁnite indications for the appearance of the double elementary charge of the Cooper pairs came from the magnitude of the magnetic flux quantum and from the quantitative relation between the electric voltage and the frequency of the Josephson effect.

158

9 The Big Surprise: High-Temperature Superconductivity

Fig. 9.5 Illustration of the wave function with s-wave symmetry (left) and with dx2 y2 -symmetry (right) in k-space (kx − ky plane). The latter symmetry dominates in the CuO2 planes of the cuprate superconductors

9.2

Symmetry of the Wave Function

The spatial symmetry of the wave function, describing the superconducting ground state of the Cooper pairs, represents another important issue with the high-temperature superconductors. In Chap. 5 we noted, that the states of the electrons in the form of waves propagating within the crystal are determined by the wave vector k, and saw how these wave vectors build up the three-dimensional kspace or momentum space. Since in the cuprates the superconductivity essentially is concentrated in the CuO2 planes, we can now practically restrict ourselves to two-dimensional momentum space within these planes. Then the question remains: Does the wave function depend on the direction within this momentum space or not? For the classical superconductors, in general there is no such dependence on the direction, and one speaks of the “s-wave symmetry”. However, for the cuprate superconductors the situation is different. For the hole-doped high-temperature superconductors a strong directional dependence of the wave function was observed, which is dominated by the atomic d-orbitals. In order to illustrate this behavior, the wave function is plotted in two-dimensional k-space of the CuO2 planes. Figure 9.5 shows such a polar plot with the four lobes of the d-orbitals, which alternately have a positive and a negative sign and display nodes and antinodes depending on the polar angle. In the case of dx2 y2 -symmetry, the nodes and antinodes are arranged along the indicated crystallographic directions. For comparison, the isotropic wave function with s-wave symmetry, which usually appears in the classical superconductors, is also shown. In order to identify the directions of the nodes and antinodes within the scheme of the CuO2 planes, in Fig. 9.6 we show the square CuO2 lattice. If we start in momentum space with a speciﬁc direction of the wave vector and perform, in the direction of the wave vector, a complete rotation around the center of the system of coordinates, then for d-wave symmetry the wave function changes

9.2 Symmetry of the Wave Function

159

Fig. 9.6 Scheme of the square CuO2 lattice. The unit cell is marked by the solid line. The lattice constant a is indicated

its sign four times until we come back to the starting direction. During this rotation the wave function passes four times through the value zero. These directions with zero value are called nodes, as is common with vibrating strings. At the nodes the energy gap in the superconductor vanishes, and it increases again at both sides of the nodes. For hole-doped high-temperature superconductors, the d-wave symmetry of the wave function of the Cooper pairs, with its sign changes and its nodes, leads to many important consequences in the physical properties of the superconducting state of these materials. In this context, we will discuss below a beautiful experiment for the detection of half-integer magnetic flux quanta. For electron-doped high-temperature superconductors the question of the spatial symmetry of the wave function of the Cooper pairs is not yet completely clariﬁed, since experimental observations do not yet allow an unequivocal conclusion. Whereas the formation of Cooper pairs can be stated deﬁnitely as a fundamental principle also for high-temperature superconductors, the underlying microscopic pairing mechanism still remains unclear for the cuprates and remains a theoretical and experimental challenge. The layered structure of the cuprate superconductors with the CuO2 planes arranged on top of each other, also affects the magnetic flux lines, which Abrikosov had predicted ﬁrst for the type-II superconductors, and which in the mixed state intersect the superconductor like a forest of poles along the direction of the magnetic ﬁeld. We only consider the case where the magnetic ﬁeld is oriented perpendicular to the CuO2 planes. Since the superconducting property is highly concentrated within these planes, the flux lines are also generated only along a short distance on the planes and are interrupted between the planes. Now the continuous magnetic flux line, according to the theory of Abrikosov, is separated into short disks, which are located at the CuO2 planes, and which are stacked exactly on top of each other. Often these disks are referred to as “pancakes”. Because of this separation of the magnetic flux lines into many small individual disks, the magnetic flux-line lattice now displays a large number of new properties, which are absent in

160

9 The Big Surprise: High-Temperature Superconductivity

the original Abrikosov lattice. For example, individual disks can leave the arrangement where they are stacked exactly on top of each other, and a process like the melting and evaporation of the perfectly-stacked conﬁguration of the disks becomes possible. In Chap. 8 we discussed that, because of the motion of the magnetic flux lines, an electric voltage is generated in the superconductor, and noted that this leads to electric losses, if the flux-line motion is caused by the Lorentz force produced by an electric current. Because of the decomposition of the flux lines into the individual disks (pancakes), in the high-temperature superconductors, this loss mechanism is particularly important, since the motional freedom of the individual small disks is much stronger than that of the complete and, more or less rigid, Abrikosov flux lines. Therefore, the prevention of the motion of the disks by the introduction of pinning centers into the superconductor represents a highly important task. In this context we recall that the radius of the normal core in the center of each flux line is given by the coherence length n, which is much smaller in the cuprates than in the classical superconductors. Hence, the minimum size of the pinning centers only needs to reach about an atomic length scale, in order to be effective. This explains why even only local deviations from stoichiometry, such as, for example, missing oxygen atoms in the CuO2 planes and grain boundaries on an atomic scale, represent highly effective pinning centers in the high-temperature superconductors.

9.3

Grain Boundaries

Soon after the discovery of the cuprate high-temperature superconductors, a severe problem with these materials became apparent. As ceramics, the materials were prepared initially with a granular structure, where the individual grains were separated from each other by a dense network of grain boundaries. Since, in general, within these grain boundaries the superconductivity is weakened or even interrupted, during electrical current flow a ﬁnite electrical resistivity was observed, and hence no pure superconductivity appeared. An early experiment demonstrating the granular structure of the cuprate superconductor Y1Ba2Cu3O7 is shown in Fig. 9.4. This problem deﬁned two obvious goals for additional research and development. On the one hand, methods had to be found for strongly reducing the number of grain boundaries in the material. On the other hand, the physical properties of the grain boundaries themselves had to be investigated exactly. Regarding the ﬁrst goal, impressive progress could be achieved relatively quickly. Here above all it was thin-ﬁlm technology which allowed the preparation of thin, single-crystalline layers of the high-temperature superconductors deposited on suitable substrates. These “epitaxial layers” contain hardly any grain boundaries and remain clearly superconducting up to critical electric current densities of more than one million A/cm2 at the temperature of 77 K, the boiling point of liquid nitrogen.

9.3 Grain Boundaries

161

The pursuit of the second goal, namely the clariﬁcation of the physical properties of the grain boundaries, resulted then in an unexpected but highly interesting development. Here it was mainly scientists at the Thomas J. Watson Research Center of IBM in Yorktown Heights in the American Federal State of New York, which dominated this development. In order to study the physical behavior of a single grain boundary, in his IBM laboratory Chang C. Tsuei selected a thin layer of the high-temperature superconductor Y1Ba2Cu3O7 showing relatively large single-crystalline areas separated from each other by very long individual grain boundaries. Now only a narrow conducting bridge had to be fabricated out of the YBCO layer in such a way, that the bridge was running nearly perpendicular across the grain boundary. This allowed electrical measurements to be performed on a single grain boundary. During the time when Tsuei prepared his experiments using a spontaneously generated single grain boundary, his IBM colleague Praveen Chaudhari proposed the idea of generating the grain boundary in a controlled way by means of a specially prepared substrate for depositing the layer of the cuprate superconductor. During the further developments, also the postdoc Jochen Mannhart was heavily involved. With the method used by Tsuei for achieving the epitaxial growth of the single-crystalline layer of the high-temperature superconductor, the crystallographic orientation of the single-crystalline substrate is reproduced exactly by the superconducting layer deposited on top. If for the substrate one uses an artiﬁcially prepared so-called bicrystal, in which two single-crystalline parts with different crystallographic orientation are separated from each other by an atomically sharp grain boundary, the grain boundary of the substrate is transferred exactly to the superconducting layer on top. This bicrystal is fabricated by cutting up a single-crystal into proper pieces and by fusing two pieces, with a different crystal orientation, together again (Fig. 9.7). The bicrystal technique turned out to be highly successful and subsequently permitted many experiments with well-deﬁned grain boundaries in superconducting thin layers. In particular, the Josephson effect at a single grain boundary was observed. This technique then developed into an important method for the preparation of Josephson junctions in thin layers of high-temperature superconductors. Furthermore, this approach also served extremely well for the fabrication of SQUIDs based on high-temperature superconductors. The different signs of the dx2 y2 -wave function appearing at different polar angles, respectively, can lead to important consequences, if two crystals with different orientation are connected with each other by means of a well-deﬁned grain boundary (bicrystal technique, Fig. 9.7). The case, at which a positive lobe of the wave function, at the opposite side of the junction runs into a negative lobe, is referred to as p-junction. A closed ring, containing such a p-junction, violates the uniqueness of the wave function (frustration), since, during a complete revolution, a sign change of the wave function remains. In this case, the frustration is removed by the spontaneous generation of a half-integer magnetic flux quantum. Eventually, an extension of this principle was utilized by Chang Tsuei for proving experimentally the d-wave symmetry of the Cooper pair wave function in

162

9 The Big Surprise: High-Temperature Superconductivity

Fig. 9.7 Bicrystal technique for the controlled preparation of a single grain boundary within a superconducting cuprate layer. As the substrate one uses an artiﬁcially prepared bicrystal, in which two differently oriented single-crystalline parts of the crystal are separated from each other by an atomically sharp grain boundary. The grain boundary within the substrate is then exactly transferred to the superconducting layer on top. On both sides of the grain boundary there now exist single-crystalline superconducting layers with different crystallographic orientation

hole-doped high-temperature superconductors (Fig. 9.8). We discussed above that, for d-wave symmetry, the wave function changes its sign four times during a complete rotation of the direction of the wave vector. Therefore, each time after only half a full rotation, the same sign of the wave function appears again. By joining together three angular sections like the pieces of a round cake in each of which the crystallographic orientation of the superconducting layer is different, it can be achieved that at one of the three grain boundaries a sign change of the wave function between the two sides takes place. If this is the case, after a complete rotation of the direction around the common meeting point of the three angular sections, the wave function no longer reproduces itself, but instead a sign change remains due to the generation of a p-junction. As a necessary consequence, at the common meeting point of the three grain boundaries, an exactly half-integer magnetic flux quantum is spontaneously generated. Chang C. Tsuei, and collaborators have succeeded in detecting this half-integer magnetic flux quantum by means of a SQUID-scanning microscope. The fabrication of the three angular sections of the superconducting layer, each with a different crystal orientation and separated from each other by sharp grain boundaries, could be achieved using a “tricrystal” as a substrate, where this tricrystal was composed of three correspondingly oriented angular sections. In the case of the tricrystal, the cutting and fusing process for producing the bicrystals had to be extended accordingly. This tricrystal experiment and the detection of the spontaneously generated half-integer magnetic flux quantum at the common meeting point of the three grain boundaries, represents one of the most spectacular demonstrations proving the d-wave symmetry of the pair wave function in hole-doped high-temperature superconductors.

9.4 Intrinsic Josephson Junction

163

Fig. 9.8 Tricrystal experiment of Tsuei and coworkers for proving the d-wave symmetry of the quantum mechanical wave function of Cooper pairs in the cuprate superconductor Y1Ba2Cu3O7. The substrate is an artiﬁcially prepared tricrystal, in which three differently oriented single-crystalline parts of the crystal are separated from each other by atomically sharp grain boundaries. This crystalline structure, including its grain boundaries, is exactly transferred to the superconducting layer prepared on top. The grain boundaries are marked by straight white lines. Within the three crystal parts, separated from each other by the grain boundaries, the differently oriented d-wave symmetry pattern of the Cooper pair wave function is indicated by the diagrams with the four lobes. At different locations, a total of four superconducting rings are fabricated from the YBaCuO layer, whereas the remaining part of the layer is removed. The orientations of the three crystal parts are chosen such that, in the presence of d-wave symmetry of the wave function, within the ring around the common meeting point of the three crystal parts, an exactly half-integer magnetic flux quantum is spontaneously generated, whereas nothing happens at the three other rings. The image was obtained by means of a SQUID scanning microscope, and it clearly shows the half-integer magnetic flux quantum for the ring in the middle around the common meeting point of the three crystal parts. The other rings are only weakly visible. (C. C. Tsuei)

9.4

Intrinsic Josephson Junction

The crystal structure of the cuprate superconductors suggests a Josephson contact, in which the superconducting copper-oxide planes are separated from each other by intermediate layers, which are only weakly electrically conducting. In a crystal of these materials there are up to many thousand Josephson junctions of this type stapled upon each other. In 1992, Reinhold Kleiner and Paul Müller, at the time working at the Walther-Meissner Institute for Low Temperature Research of the Bavarian Academy of Science in Garching near Munich, have succeeded in discovering the “intrinsic Josephson effect” in small single crystals of the cuprate superconductor Bi2Sr2CaCu2O8 (BSCCO). During the initial experiments a small superconducting BSCCO-crystal was clamped between two contact pins such that an electric current flow perpendicular to the copper-oxide planes occurred. Above a critical value of the current, an electric voltage appeared along the crystal which, according to the second Josephson equation (8.19), was accompanied by high-frequency Josephson

164

9 The Big Surprise: High-Temperature Superconductivity

Fig. 9.9 Intrinsic Josephson contact as a source of microwaves. Left: Scheme of a staple of three Josephson contacts of a superconducting Bi2Sr2CaCu2O8 (BSCCO) crystal. The copper-oxide planes (shown in dark color) run along the base of the CuO-pyramids. Right: Emitted microwave spectrum of a BSCCO-crystal. (R. Kleiner)

alternating current. In particular, the emitted microwaves could be detected. Since the stapled Josephson contacts oscillate synchronously, the emitted power of the electromagnetic radiation increases quadratically with the number of contacts in the staple. Presently, for the study and application of the intrinsic Josephson effect, small “mesas” made of BSCCO are prepared on a suitable substrate and are covered by metal layers for electrical contacting (Fig. 9.9). Currently, these developments are highly active aiming at a radiation source of microwaves in the frequency range of about 0.5 – 2 terahertz (THz = 1012 s−1), since up to now this frequency range is hardly accessible (terahertz gap). Presently (2019) the power output of a single mesa is up to 0.2 mW, whereas for a synchronized array of several mesas it amounts up to 0.6 mW. This limit is mainly due to electric heating effects within the device.

9.5

More New Superconductors: MgB2, Iron Pnictides

The surprises caused by the discovery of new superconducting materials with relatively high values of the critical temperature were not yet over with the appearance of the cuprate superconductors. In March 2001 the group of Jun Akimitsu at the Aoyama-Gakuin University in Tokyo reported in the journal “Nature”, that the compound MgB2, consisting only of two elements, is superconducting with the critical temperature TC = 39 K. Already by January 2001 Akimitsu had announced his discovery at a conference in Japan, and immediately

9.5 More New Superconductors: MgB2, Iron Pnictides

165

many groups started research activities to ﬁnd out the physical properties of this new superconductor. Similar to the cuprates, the crystal structure of the magnesium-diboride (MgB2) shows a layered conﬁguration. Planes of hexagonally arranged magnesium atoms and planes of boron atoms ordered in a honeycomb pattern, like graphite, are placed alternately on top of each other. As expected it was again found, that the superconductivity is based on the formation of Cooper pairs. Similar to the classical superconductors, the wave function of the pairs does not show an appreciable dependence on the direction, apparently displaying s-wave symmetry. Early in 2008, the group of Hideo Hosono in Japan reported another surprise: In the compound LaOFeAs of lanthanum (La), oxygen (O), iron (Fe), and arsenic (As), they had discovered superconductivity, following its doping with fluorine (F). In the case of the composition LaO1−xFxFeAs at x = 0.07 the critical temperature TC = 26 K was found. This new class of superconductors containing iron and arsenic belongs to the group of the iron pnictides. In the family ReO1−xFxFeAs additional superconductors were found rather quickly, after lanthanum was replaced by other elements of the rare earths (RE) such as praseodymium (Pr), neodymium (Nd), or samarium (Sm). In this way, values of the critical temperature up to the record value TC = 56 K of Sr0.5Sm0.5FeAsF could be achieved. In spite of their pronounced layered structure, in their electronic transport properties the iron-pnictides do not show appreciable anisotropy (like the cuprates). The important structural elements are planar layers of iron atoms surrounded by tetrahedrically coordinated As or Se anions playing the role of the CuO planes in the cuprates (Fig. 9.10). The layers are arranged in a stacked sequence separated by alkali, alkaline-earth, or rare-earth and oxygen blocking layers, in which oxygen is replaced partly by fluorine acting as dopant. Similar to the case of the cuprates 22 years earlier, worldwide the research dealing with the iron-pnictides grew explosively. Similar to the cuprates, in their undoped state the iron- pnictides are ordered magnetically, but they are electrically conducting contrary to the cuprates. They are an anti-ferromagnetic semi-metal. It appears, that in this case superconductivity and magnetism are connected with each other. An overview of the different iron-pnictides discovered up to 2015 is shown in Fig. 9.11. The different families are distinguished by the notation 11, 111, 122, 1111, etc., respectively. By 2010 more than 50 iron-pnictide compounds had been found. The pairing mechanism remains unclear. However, a large amount of evidence points to magnetic spin fluctuations.

Fig. 9.10 Layer of FeAs (or similarly of FeSe) arranged between layers of lanthanum-oxide perhaps doped with fluorine

166

9 The Big Surprise: High-Temperature Superconductivity

Fig. 9.11 Critical temperature TC plotted versus the time of discovery of the different iron-pnictide superconductors (Silvia Haindl)

9.6

Technical Applications

Because of the relatively high values of their critical temperature, compared with the classical superconductors (with the possibility of utilizing superconductivity after cooling down to only 77 K with liquid nitrogen) high-temperature superconductors quickly became very useful for technical applications. Here the applications in the ﬁeld of electronics and microelectronics, as well as the applications at high electric currents and in power electronics appear equally interesting. The following examples will serve as an illustration. Today, the principle of the bicrystal substrates for the fabrication of Josephson grain-boundary junctions and SQUIDs from thin layers of high-temperature superconductors has already found wide applications in electronic measuring instruments. High-frequency ﬁlters fabricated from thin layers of high-temperature superconductors appear very promising. Here it is in particular the increased sharpness of the high-frequency channels, achieved with the superconducting layers, which allows many more channels in the available frequency bands to be accommodated than in the past. For example, more than a few hundred base stations for mobile telephone communication, based on this technology, are already operating in the USA. However, following a rapid growth of this superconducting technology, advances in the newer generations of mobile telephones eliminated the need for such superconducting ﬁlters, and their acceptance decreased. Regarding the applications at high electric currents, the development of magnetic coils fabricated from high-temperature superconductors is being intensively investigated. Last but not least, superconducting systems for the limitation of electric fault currents in energy technology are in a promising stage of development.

9.6 Technical Applications

167

Such systems are meant to quickly interrupt the electric current under overload conditions, if damages to the electric power lines are expected due to overload. Presently (2013) an interesting new development based on wind energy emerges in the case of generators made of high-temperature superconductors for electric currents. Their intended operation would reduce the weight of the generators located at the upper end of the mast to about half the value of the current technology, or at the same weight it would double the power. In Japan, the development of a superconducting dc cable cooled with liquid nitrogen and projected for 5 GW power (Ishikari Project) is taken up.

Chapter 10

Magnetism: Order Among the Elementary Magnets

Abstract Electrons represent elementary magnets because of their spin magnetic moment, leading to paramagnetism, and their orbital magnetic moment, causing diamagnetism. In an external magnetic ﬁeld the magnetization of a paramagnet is described classically by the Langevin function, to be replaced by the Brillouin function in the case of quantization effects. In a ferromagnet the elementary magnets are spontaneously oriented along a distinct direction. The ﬁrst quantum mechanical explanation was proposed by Heisenberg, based on the exchange interaction between the electrons of two atoms. The perfect order of the elementary magnets can be perturbed due to the thermal excitation of spin waves, which also contribute to the speciﬁc heat and affect the electronic transport properties. In addition to ferromagnetic order, other forms of the spin magnetic order are possible, such as antiferromagnetism. The recent advances in the fabrication of well-controlled multilayer structures lead to important technical applications of giant magneto-resistance and to the birth of the new ﬁeld of spintronics.

In crystals, the role of the electrons as elementary magnets leads to important consequences, which we will discuss in this chapter. This quality of the electrons to act as elementary magnets, originates for two reasons: the angular momentum or spin possessed by each electron, and the orbital momentum resulting from the orbital motion of each electron. The ﬁrst cause leads to the spin magnetic moment, and the second cause to the orbital magnetic moment. The half-integer spin and the associated magnetic moment as fundamental properties of the electrons were found theoretically by the Englishman Paul Adrien Maurice Dirac in the year 1928, when he applied the physics of the Special Theory of Relativity to the quantum mechanical wave equation of the electron. Because of the quantization of the direction of the angular momentum, in a given direction only the parallel or the antiparallel orientation of the spins are allowed. With his concept of spin, Dirac had found the explanation for many experimental observations, which had remained unexplained till then, and which in the words of Wolfgang Pauli at that time had

© Springer Nature Switzerland AG 2019 R. P. Huebener, Conductors, Semiconductors, Superconductors, Undergraduate Lecture Notes in Physics, https://doi.org/10.1007/978-3-030-31420-0_10

169

170

10

Magnetism: Order Among the Elementary Magnets

indicated in the energy spectra (here in the English translation) “a peculiar ambiguity of the quantum theoretical qualities of the light-emitting electron, which cannot be understood classically.”

10.1

Diamagnetism

The diamagnetism is due to the orbital magnetic moment, and is a magnetic property of all substances. However, it can be overlaid by other magnetic phenomena. Diamagnetism appears in its pure form, if the spin magnetic moments of all atomic electrons exactly compensate each other, such that only the orbital magnetic moments remain. This complete compensation arises in the case of atoms with closed inner electronic shells and of atoms with an even number of electrons. In an external magnetic ﬁeld, in diamagnetic materials, circulating currents are induced within the atoms, which generate a magnetic ﬁeld oriented oppositely to the external magnetic ﬁeld. Here the “Lenz rule” is obeyed. This rule requires, that the induced electric currents always weaken the magnetic ﬁeld which is acting as their external cause. Therefore, diamagnetic susceptibility is negative. The orbital part of the magnetism of the electrons in the conduction band of a metal yields a diamagnetic contribution, which Lew Dawidowitsch Landau calculated for the ﬁrst time in the year 1930, using exact quantum mechanical theory. We have discussed this theory of Landau in Chap. 7. We have already seen an example of perfect diamagnetism in the context of the Meissner effect of superconductivity. The diamagnetism is a result of the change of the orbital motion of the electrons due to an external magnetic ﬁeld and concerns only the magnetic moments caused by the magnetic flux density B. The magnetic properties of a material are quantiﬁed in terms of its magnetization M, which is deﬁned as the magnetic moment per volume. In the case of M we have the relation M ¼ vB;

ð10:1Þ

where v denotes the magnetic susceptibility. In the case of diamagnetism we have v < 0. In a magnetic ﬁeld, the electron orbits experience a precession motion with the Larmor frequency xL ¼ eB=2m:

ð10:2Þ

Here m is the electron mass. The Larmor precession corresponds to a circular current proportional to (−e) xL. This leads to the magnetic moment l in form of the product l = (circular current ring area). As shown by Paul Langevin, one ﬁnds for the (negative) susceptibility

10.1

Diamagnetism

171

v \r2[ ;

ð10:3Þ

where denotes the average quadratic radial extension of the electron orbit within the atom. The diamagnetic contribution of the ions to the susceptibility in dielectric solids agrees well with the result (10.3).

10.2

Paramagnetism

If the electron shells are not closed, or for an odd number of electrons per atom, there remain in the crystal spin magnetic moments, which are not completely compensated. In this case we are dealing with paramagnetism. Initially, in paramagnetic materials, the spin magnetic moments are completely disordered. However, as soon as an external magnetic ﬁeld exists, the spin moments turn into the direction of this magnetic ﬁeld. Here the electrons behave similarly to a compass needle, which turns into the direction of the earth’s magnetic ﬁeld. However, the complete redirection of the spin magnetic moments is prevented because of the thermal motion of the elementary magnets. This thermal motion of the elementary magnets increases with increasing temperature. Hence, the degree of redirection of the spin magnetic moments decreases correspondingly. This results in the famous Curie law, indicating that the magnetic susceptibility, which is positive in this case, is inversely proportional to the temperature. The Frenchman Pierre Curie was married to Marie Curie, who had discovered the element radium. He published his law in the year 1895. This was the ﬁrst time that a law in the ﬁeld of the magnetism of materials had been formulated. Curie’s publication with more than one hundred pages summarized the results of an extensive research program, in which many substances had been investigated over a large range of magnetic ﬁeld and temperature. Curie’s name stands at the beginning of a series of French scientists, who had made France, at an early stage, an important center of research in the ﬁeld of magnetism. Among others, this series of French scientists prominent in the ﬁeld of magnetism includes Paul Langevin, Pierre Weiss, Léon Brillouin, and Louis Eugene Felix Néel. Paul Langevin, a young co-worker of Pierre Curie, analyzed theoretically paramagnetic behavior. We will briefly sketch his ideas. Starting from the potential energy U ¼ l B ¼ l B cos h

ð10:4Þ

of a magnetic moment l in the magnetic ﬁeld B, Langevin calculated the average value from the classical Boltzmann distribution in the following way. (h is the angle between the vectors l and B). According to Boltzmann, the probability of the direction of the magnetic moment l with the corresponding energy U is proportional to exp(−U/kBT). Therefore, (with the solid angle dX) we have

172

10

Magnetism: Order Among the Elementary Magnets

R \cos h[ ¼

exp kUT cos h dX B R exp kUT dX

ð10:5Þ

B

Rp ¼

0

expðl B cos h=kB TÞ2p sin h cos hdh Rp 0 expðl B cos h=kB TÞ2p sin hdh

ð10:6Þ

and after a few steps 1 \cos h[ ¼ coth x LðxÞ; x L(x) is referred to as magnetization one ﬁnds

Langevin

x ¼ l B=kB T: function.

\M[ ¼ Nl\cos h[ ¼ Nl LðxÞ;

For

ð10:7Þ the

average ð10:8Þ

where N denotes the number of the magnetic moments µ per volume. The function L(x) is shown in Fig. 10.1. In the case x 1 (high temperatures) we have L(x) x/3, and we obtain \M[ ¼ Nl2 B=3 kB T ¼

C B: T

ð10:9Þ

This is Curie’s law. C = N l2/3 kB is the Curie-constant. On the other hand, in the case x 1 (low temperatures) we obtain saturation of the magnetization. From (10.7)–(10.9) we see, that the dependence of the magnetization on the temperature and on the magnetic ﬁeld is determined only by the ratio of the magnetic ﬁeld and the temperature. In the limit of small magnetic ﬁelds and high temperatures, Langevin obtained again the Curie law, whereas in the opposite limit he found that the magnetization approaches a constant value. Langevin had obtained his result (10.8) still within the context of classical physics. If the quantization of the spin direction, required by quantum mechanics, is

Fig. 10.1 Langevin function L(x) according to the deﬁnition in (10.7)

10.2

Paramagnetism

173

taken into account, the results are qualitatively similar to the classical case. We will briefly indicate this. As shown by quantum theory, the magnetic moment of an isolated atom is l ¼ g lB J=h

ð10:10Þ

lB ¼ e h=2 m

ð10:11Þ

Here

is Bohr’s magneton. J is the total angular momentum, the sum of the vectors of the angular momentum of the electron orbits (L) and of the spins (S): J ¼ L þ S:

ð10:12Þ

In (10.10) g denotes the “Landé-g-factor”: g ¼ 1þ

JðJ þ 1Þ þ SðS þ 1Þ LðL þ 1Þ : 2J ðJ þ 1Þ

ð10:13Þ

In a magnetic ﬁeld, the quantized energy levels of an elementary magnetic moment are U ¼ mJ g lB B;

mJ ¼ J; J1; J 2; . . .; J:

ð10:14Þ

In the case of a single spin and L = 0 we obtain mJ = ± ½ and g = 2: U ¼ lB B:

ð10:15Þ

In thermal equilibrium, the magnetization of this two-level-system is \M[ ¼ N lB tanh x;

x ¼ lB B=kB T:

ð10:16Þ

In the limit x 1 (high temperatures) we ﬁnd \M[ ¼ N l2B B=kB T;

ð10:17Þ

similar to Curie’s law. In the general case with 2J + 1 energy levels according to (10.14), in thermal equilibrium the magnetization is \M[ ¼ N lB BJ ðx);

x ¼ lB B=kB T:

ð10:18Þ

The function BJ(x) is the Brillouin function (which here we will not discuss any further). In the limit x 1 (high temperatures) we obtain again the form of Curie’s law * B/T.

174

10

Magnetism: Order Among the Elementary Magnets

In the year 1905, Langevin had already predicted the magneto-caloric effect in paramagnetic substances. This effect is fundamental to the method of adiabatic demagnetization we discussed in Chap. 1 as a technique for cooling to low temperatures. Here the heat energy exchanged during the redirection of the magnetic moments of the electrons parallel to the external magnetic ﬁeld, plays a central role. In the conduction band of a metal, the spin magnetic moment of the electrons also generates a contribution to the paramagnetism. Classically, we would again expect a behavior according to the Curie law, with the result that the paramagnetic susceptibility is inversely proportional to the temperature. However, because of the Pauli exclusion principle, the electrons in the conduction band must obey the rules of quantum statistics. As we have discussed before in Chap. 5, therefore, only the fraction of electrons in the conduction band, given by the reduction factor kBT/eF, can contribute to the paramagnetism. By multiplying the Curie law with the factor kBT/eF, we obtain \M[ ¼ N l2B B=eF :

ð10:19Þ

We see that the temperature in the expression of the paramagnetic susceptibility is cancelled, and that the latter quantity is independent of the temperature, in good agreement with experimental observations. This result is similar to the case of the speciﬁc heat of the conduction electrons, which we discussed in Chap. 5. Wolfgang Pauli was the ﬁrst to propose this theory of the spin paramagnetism of electrons in metals. In a detailed analysis, one ﬁnds for the electrons in the conduction band of a metal, that the negative contribution to the magnetic susceptibility which is due to diamagnetism according to Landau, is three times smaller than the positive contribution which is due to paramagnetism according to Pauli. Hence, in the ﬁnal result, paramagnetism prevails for the electrons of the conduction band in metals.

10.3

Ferromagnetism

In addition to the phenomena of diamagnetism and paramagnetism, both of which are induced by an external magnetic ﬁeld, there exists still another form of magnetism, in which the elementary magnets in the crystal orient themselves spontaneously along a distinct direction. In this case, the command by an external magnetic ﬁeld to order is no longer needed. Now we are dealing with ferromagnetism and its various modiﬁcations. For example, one of these modiﬁcations is antiferromagnetism. The ferromagnetism confronts us with the following central question: Why is it that the magnetic moments of the electrons of neighboring atoms within the crystal orient themselves spontaneously, i.e., without an external magnetic ﬁeld, exactly along the same direction and assume a perfectly ordered state just on their own?

10.3

Ferromagnetism

175

The complete theory of ferromagnetism had to wait for the development of quantum mechanics. The crucial answer, which subsequently also became the guiding principle for all further developments, was given by Werner Heisenberg in the year 1928. Heisenberg’s answer was preceded by an intensive correspondence with Wolfgang Pauli for almost two years. The basic idea of Heisenberg again originated from the exact identity of the electrons as elementary particles and that the resulting symmetry requirement should be satisﬁed by the quantum mechanical wave function during the exchange of two electrons. Taking the crystal as an extended molecule, at the time Heisenberg could utilize the concept of the exchange energy, which had just been developed, for, say the two electrons of the helium atom or of the hydrogen molecule (H2). He introduced the concept of the exchange interaction between two atoms 1 and 2 with the spins S1 and S2 and obtained the exchange energy (Heisenberg model) U ¼ 2 JS1 S2

ð10:20Þ

d r1 d r2 wa ðr1 Þwb ðr2 ÞVðr1 r2 Þwa ðr2 Þwb ðr1 Þ:

ð10:21Þ

with the exchange integral ZZ J¼

In the case of ferromagnetism, we have J > 0, and the parallel spin orientation is energetically favored. The exact theoretical calculation of the exchange integral (10.21) requires a detailed discussion (which we do not undertake). For the ﬁrst time, in this context, Heisenberg treated the interaction between the electrons in a crystal using quantum mechanics. It became clear that the parallel orientation of the spin magnetic moments of the electrons from neighboring atoms in the crystal, leading to the ferromagnetism, depends on the form of the electron wave function and on the number of nearest neighbors in the crystal lattice. At that time the mathematical formalism needed for answering many of the questions, was still only in its ﬁrst stage and had to be developed along with the quantum theory of ferromagnetism. For this, Heisenberg had given the initial momentum. A phenomenological understanding of ferromagnetism had already been reached earlier. In the year 1907 the Frenchman Pierre Weiss had proposed the hypothesis of the molecular ﬁeld or the exchange ﬁeld, which quickly became highly successful. Without explaining its microscopic origin, he had postulated an average effective magnetic ﬁeld within the crystal, producing the exact order among the elementary magnets. In this way, the idea of the quantum mechanical exchange energy, appearing only about 20 years later, was substituted by the concept of the effective “Weiss ﬁeld”. It is exactly this effective magnetic ﬁeld, which causes the spatial order of the magnetic moments of the individual atoms or molecules. Based on the material data, for some substances one can derive values of the Weiss ﬁeld which are distinctly higher than 103 T (about ten million times higher than the earth’s magnetic ﬁeld). Also in this way the large magnitude of the quantum mechanical exchange energy of the magnetism, conceived later, can be illustrated.

176

10

Magnetism: Order Among the Elementary Magnets

During his PhD thesis Weiss concentrated on magnetism, and later always remained close to this subject. As a child, together with his family, he had to leave his home land of Alsace, after the province had been occupied by Prussia in 1870. In the year 1902 he had accepted an offer from the ETH in Zurich. Only in 1919 after the First World War could he return to Strassburg in his home country, when he became the director of the Physics Institute of the University.

In the case of the Weiss ﬁeld BW we assume BW = kM, where k is a constant, which depends on temperature. In a cooperative way, each individual magnetic moment feels the average magnetization of all the others (molecular-ﬁeld approximation). However, the spontaneous alignment of the elementary magnets along the same direction in a ferromagnet cannot be maintained up to arbitrarily high temperatures. Instead, it vanishes abruptly at the “Curie temperature” TCU. Above the temperature TCU we only have paramagnetism. In the paramagnetic state (above TCU), in the presence of an external magnetic ﬁeld Ba, we have M ¼ vp ðBa þ BW Þ ¼ vp ðBa þ kMÞ

ð10:22Þ

with the paramagnetic susceptibility vp = C/T from (10.9). From (10.22) we obtain Mð1

C C kÞ ¼ Ba T T

ð10:23Þ

and v ¼ M=Ba ¼ C=ðT TCU Þ;

TCU C k;

ðT ! TCU from aboveÞ

ð10:24Þ

A more accurate treatment yields v ¼ C=ðT TCU Þ1:33 ;

ðT ! TCU from aboveÞ

ð10:25Þ

with the “critical exponent” 1.33, in agreement with experiment. For the temperature dependence of the magnetic susceptibility, instead of the Curie law, the Curie-Weiss law is valid: the magnetic susceptibility is inversely proportional to the temperature distance T – TCU from the Curie temperature. Below the Curie temperature, the spontaneous magnetization is found again using the molecular-ﬁeld approximation BW = kM. In the case of a two-level system (S = ½), by insertion into (10.16), one obtains M ¼ N lB tanhðlB k M=kB TÞ:

ð10:26Þ

After introducing the quantities m M/(N lB) and t T/TCU = kBT/(N l2B k) we obtain

10.3

Ferromagnetism

177

Fig. 10.2 Schematical presentation of the graphical solution of the transcendental (10.27). At the critical point t = 1, the intersection point is located at m = 0. In the case t ! 0, the intersection point approaches m = 1

m ¼ tanhðm=tÞ:

ð10:27Þ

(Here we have used the notation TCU = C k, with C = N l2B/kB from (10.17).) The transcendental (10.27) can be solved graphically, as it is indicated schematically in Fig. 10.2. The graphical solution yields the temperature dependence of the magnetization shown in Fig. 10.3. This is the behavior in the case of a phase transition of second order, where the magnetization represents the order parameter. From Fig. 10.3 we see, that below TCU the spontaneous magnetization steeply increases with decreasing temperature, and at low temperatures it approaches a constant saturation value. Iron (Fe), cobalt (Co), and nickel (Ni) are well known ferromagnetic elements. The values of the Curie temperature are for iron, 1043 K; for cobalt, 1390 K; and for nickel, 630 K. Eventually, a difﬁculty in the understanding of the ferromagnetic order of elementary magnets became more and more apparent: at low temperatures the magnetization turned out to be much smaller than expected if all elementary magnets in the whole crystal were oriented exactly along the same direction. Again, the solution of this problem was provided mostly by Pierre Weiss. Due to energetic reasons the crystal is divided into many individual regions, in each of which all elementary magnets are still well ordered and point exactly in the same direction. Fig. 10.3 Magnetization of a ferromagnet, normalized by its saturation value, plotted versus the reduced temperature T/TCU. The magnetization vanishes abruptly at the Curie temperature TCU

178

10

Magnetism: Order Among the Elementary Magnets

Fig. 10.4 Magnetic domains according to Weiss in non-magnetized iron, schematically

However, between the different regions, the magnetization of each shows a different orientation, such that in their total sum they largely cancel each other. For the individual regions Weiss introduced the notation “magnetic domains” (Fig. 10.4). In beautiful experiments during the year 1931 the American Francis Bitter observed the boundary regions between the domains by sprinkling a ﬁne magnetic powder onto the surface of a magnetized sample. Since the magnetic powder is attracted to these boundary regions, the domain structure is marked in this way. Today this method is referred to as the Bitter decoration technique. In a different way, about 10 years earlier, Heinrich Barkhausen had obtained impressive indications of the existence of the magnetic domains in ferromagnetic substances. While increasing the magnetic ﬁeld he observed that the magnetization increased discontinuously, showing distinct small jumps when one domain after another reorients its magnetization in the external magnetic ﬁeld. He could detect these “Barkhausen jumps” by means of the induced and ampliﬁed electric currents in a coil wound around the sample. Immediately after completion of his Ph.D. thesis, Felix Bloch theoretically analyzed the physical property of the boundary wall separating two magnetic domains with different directions of their magnetization. In this context he had to develop a model describing the rotation of the direction of magnetization within the domain wall from the direction in one domain to the direction in the other. Based on Heisenberg’s concept of the exchange energy of two neighboring spin magnetic moments, Bloch calculated the energy needed for rotating the two spin magnetic moments slightly away from their exactly parallel orientation. This rotation is then repeated stepwise from one magnetic spin pair to the next, such that, after a distinct number of steps, a complete rotation of the magnetization from the original direction to the direction in the neighboring domain is accomplished. The region

10.3

Ferromagnetism

179

within the crystal, in which this complete rotation takes place, is referred to as the Bloch wall. The Bloch wall is associated with a distinct wall energy. For example, in iron, the thickness of the Bloch wall amounts to about 300 atomic distances in the crystal lattice.

10.4

Spin Waves

In the state with the lowest energy, the “ground state”, of a ferromagnet, all spins are oriented exactly parallel to each other. However, the ground state is adopted only in the limit of vanishing temperature. At ﬁnite temperatures, deviations from the exactly parallel spin orientation appear in the form of thermally excited “spin waves” (Fig. 10.5). Spin waves are oscillations of the spin orientation, which possess a quantized excitation energy ħx. The role of the spin waves is similar to that of the phonons, which are the quantized lattice vibrations and cause the deviations from the perfectly periodical spatial arrangement of the atomic or molecular building blocks of the crystal. We have covered phonons in Chap. 3. Spin waves are quantized energetic excitations in a magnetic single crystal. The energy quanta of the spin waves are called magnons. In their form of energetic excitations, magnons are indistinguishable elementary particles, which, similar to the phonons, are ruled by Bose-Einstein statistics. Intuitively, magnons represent more or less pronounced deviations of the spin magnetic moments from a ﬁxed single preferential direction. These deviations propagate like a wave through the crystal. This concept of the spin waves in the theory of ferromagnetism also originated from Felix Bloch and can be found in his Habilitation Thesis which he published in 1932. Following his dissertation dealing with the quantum mechanics of mobile electrons in the crystal lattice, Bloch had turned to the theory of ferromagnetism, after Werner Heisenberg, his professor, had formulated the fundamental principles of this theory. We will briefly discuss the thermal excitation of spin waves or magnons. We consider a linear chain of N spins, all of which are oriented parallel to each other. According to (10.20) the total energy is U ¼ 2 J

N X

Sp Sp þ 1 :

ð10:28Þ

p¼1

From this we obtain the energy of the ground state UO ¼ 2 N JS2 :

ð10:29Þ

As a possible excitation, we look at the case, where a single spin is oriented antiparallel to its neighbors (Fig. 10.5b). The energy increase DU amounts to

180

10

Magnetism: Order Among the Elementary Magnets

Fig. 10.5 Elementary magnets in a simple ferromagnet. a In the ground state all elementary magnets are oriented in the same direction. b A possible excitation from the ground state: one spin is flipped over. c Spin wave in a chain of spins in a perspective presentation

DU ¼ 2 J 2S2 þ 2S2 ¼ 8 JS2 ;

ð10:30Þ

where in the bracket we have separately listed the interaction with the left and the right neighbor. However, a much smaller excitation energy is needed, if the change in the spin orientation occurs only gradually. Exactly this is accomplished by the excitation of spin waves (Fig. 10.5c). In the case of the ferromagnetic magnons one obtains the dispersion relation from the equation for the temporal change of the angular momenta of the spins. In the limit of small excitation amplitudes, one ﬁnds the dispersion relation hx ¼ 4 JSð1 cos kaÞ;

ð10:31Þ

where a denotes the lattice constant of the chain and k the wave number. In the limit of large wave lengths (ka 1), from (10.31) one obtains hx ¼ 2 J S a2 k2 :

ð10:32Þ

We note, that the dependence x * k2 is different than in the case of phonons with x * K (see (3.5) and (3.6)). These results can be easily extended to the three-dimensional crystal lattice. In the case of the thermally excited magnons the Bose-Einstein distribution (3.2) is valid. The energy of the magnons is Z hx ð10:33Þ U ¼ dx DðxÞhnx i

10.4

Spin Waves

181

analogous to (3.3), where the integral is taken over the ﬁrst Brillouin zone. In the limit of low temperatures (ka 1), for the density of states one ﬁnds D(x) * x1/2, yielding U * T5/2. The resulting speciﬁc heat of the magnons is CV ¼

@U T3=2 : @T V

ð10:34Þ

Because of the thermal excitation of magnons, the magnetization is reduced by the amount DM = M(0) – M(T). The ﬁnal result is DM=Mð0Þ T3=2 :

ð10:35Þ

We see that the thermal excitation of spin waves or magnons affects the speciﬁc heat and the saturation magnetization of a ferromagnet. In both cases the contribution of the magnons leads to the famous T3/2 law derived by Felix Bloch for the temperature dependence of the quantities. Magnons contribute also to the heat conductivity in crystals, and they influence the electrical transport properties such as the electrical conductivity and the thermoelectric phenomena. Similar to the case for phonons, the energy spectra of the magnons can also be determined experimentally by means of inelastic neutron scattering.

10.5

Antiferromagnetism

In addition to the parallel orientation of the spin magnetic moments of ferromagnetism, there also exists the case where the spins of the neighboring atoms in the crystal are oriented exactly antiparallel to each other. This case is referred to as antiferromagnetism. For antiferromagnetism the “quantum mechanical exchange integral” (10.21) is negative, whereas for ferromagnetism it is positive. Already in the late 1920s, the Frenchman Louis Eugene Felix Néel had the idea that there must also exist another kind of magnetic order in crystals, in which the spin magnetic moments of neighboring atoms are oriented exactly antiparallel to each other. After completing his studies in Paris, in the year 1928, Néel took the position of assistant of Pierre Weiss in Strassburg. Néel devoted his whole career to magnetism, up to 1940 in Strassburg and subsequently in Grenoble. Later on, largely due to Néel, has Grenoble developed into the important center of Materials Science and Solid State Physics in France, for which it is today well known everywhere. In his early idea of antiparallel spin orientation of neighboring atoms in the crystal, Néel had assumed that two lattices were penetrating each other, each of these “sublattices” by itself showing ferromagnetic order, but both being magnetized exactly in opposite direction to each other. Hence, overall the crystal remains magnetically neutral.

182

10

Magnetism: Order Among the Elementary Magnets

Therefore, the experimental evidence for such a novel possibility of magnetic order contemplated by Néel was difﬁcult to obtain. In 1938 measurements with manganeseoxide (MnO) yielded the ﬁrst positive results. The ﬁnal conﬁrmation of the hypothesis of the two sublattices penetrating each other, which are magnetized in opposite directions to each other, was achieved in the year 1949 by means of elastic neutron diffraction experiments. The antiferromagnetic order vanishes above the “Néel temperature”. The notation antiferromagnetism was proposed in 1938 by the American Francis Bitter in a theoretical paper. A famous example, much discussed in recent years, is the antiferromagnetic order of the spin magnetic moments of copper atoms in the copper-oxide planes in the undoped state of materials showing high-temperature superconductivity after doping. In an antiferromagnetic material, at ﬁnite temperatures, antiferromagnetic spin waves are thermally excited. One refers to antiferromagnetic magnons. Antiferromagnetic spin waves show the dispersion relation hx ¼ 4jJjSjsin kaj

ð10:36Þ

similar to the case of phonons (see (3.5)). In the limit ka 1 we have hx ¼ 4jJjSjkaj:

ð10:37Þ

Antiferromagnetic spin waves contribute to the speciﬁc heat and to the heat conductivity of the crystals, with a temperature dependence proportional to T3 at low temperatures, similar to phonons. Again, their energy spectrum can be determined experimentally by means of inelastic neutron scattering. In addition to the two discussed magnetic ordering phenomena of ferromagnetism and antiferromagnetism, there also exist other forms of ordered magnetic structures. However, we will not discuss these in further detail. In this chapter our whole discussion of magnetism has been limited to the electrons acting as elementary magnets. However, there also exists nuclear magnetism associated with the atomic nuclei and their quality as elementary magnets. Since the elementary magnets of atomic nuclei are about two thousand times weaker than those of electrons, the effects of nuclear magnetism are restricted only to very low temperatures. For example, in the paramagnetism of atomic nuclei, the ratio between the magnetic ﬁeld and the temperature must be two thousand times larger compared with the paramagnetism of electrons, in order to achieve the same degree of alignment of the nuclear spins. Therefore, we will refrain from any further discussion of nuclear magnetism.

10.6

10.6

Technical Applications, Giant Magneto-Resistance, Spintronics

183

Technical Applications, Giant Magneto-Resistance, Spintronics

For a long time ferromagnetic materials have been interesting for their technical applications. In many ofﬁces and homes we ﬁnd small sticking magnets. There are of course more ambitious applications of permanent magnets in electric and in transportation technology. Often magnetic couplings provide distinct advantages. The magnetic “hardness” of a material for a permanent magnet plays an important role in their applications. One distinguishes between magnetic soft and magnetic hard materials. The magnetic hardness is quantiﬁed in terms of the “coercive ﬁeld” HC. The latter indicates the value HC of the magnetic ﬁeld, at which the unmagnetized state of the material is again reestablished, if this magnetic ﬁeld is applied a second time in a direction opposite to that of the original magnetization of the material. This is shown schematically in Fig. 10.6, where the magnetic flux density B is plotted versus the applied magnetic ﬁeld H in the case of a magnetic soft and of a magnetic hard material. A soft material shows a small value of HC and little hysteresis, in contrast to a magnetic hard material with a large value of HC and large hysteresis. In this context we remember that, in all individual magnetic domains we have discussed above, at ﬁrst the magnetization must be rotated into the same direction by means of a suitably applied magnetic ﬁeld, in order to obtain a strong permanent magnet. Alloys consisting of aluminum, nickel, and cobalt (AlNiCo) belong to the oldest and mostly tried materials for permanent magnets. Record values of the coercive ﬁeld are achieved in alloys of samarium and cobalt (SmCo5). Sinter materials such as, for example, barium- or strontium-ferrite, fabricated from a magnetic powder of small single-domain particles, are economically highly attractive. For the large-scale technical project of the magnetic suspension train “Transrapid” the latter sinter materials are particularly suitable as levitation magnets. Fig. 10.6 Magnetic flux density B plotted versus the applied magnetic ﬁeld H in the case of a magnetic soft (left) and a magnetic hard (right) material

magneƟc soŌ

hard

H C = coercive field B r = remanence

184

10

Magnetism: Order Among the Elementary Magnets

In recent years magnetism has increasingly entered the ﬁeld of microelectronics, where it has triggered very interesting developments. In this case, in addition to the electric charge, the spin and the associated magnetic moment of the electron play a signiﬁcant role in magneto-electronic devices. The large advances in technology for the preparation of thin layers and multi-layer packages have been an important prerequisite for this development. Here nearly atomic accuracy in the fabrication of the layers has been achieved. Today this ﬁeld is referred to as magneto-electronics, spin-electronics, or spintronics. While usually in electronic circuits the spins of the electrons are arbitrarily oriented and do not influence the electric current flow, in spintronics “spin-polarized” electric currents are used, where the spin of the mobile electrons is oriented in a speciﬁc direction. In this case the spin serves to control the electric current flow. Important ﬁelds for the application of magneto-electronics exist in magnetic technology for data handling in computers, for example, in the reading heads for hard disks and in the magnetic elements for data storage. In addition, we mention the magneto-sensorics in automotive technology, mechanical engineering, and in medicine. At present a highly promising goal for the not too distant future is a close combination of magneto-electronics with semiconductor technology. In the previous generation of magnetic sensors, for example, in the reading heads for extracting data stored in hard disks, the electrical resistance change of a ferromagnetic layer due to an external magnetic ﬁeld, is utilized. The magnetic data storage is based on small magnetic domains, which represent the “0” or “1” of the digital information by means of their different magnetization. In the reading head the electrical resistance change serves to detect the local magnetic ﬁeld at the surface of the hard disk and thus the digital information. In the year 1988, this technology experienced an important advance, when Peter Grünberg at the German Research Center in Jülich and, nearly simultaneously, Albert Fert at the Université Paris Sud discovered the “giant magneto-resistance”. Two years prior to this discovery, Peter Grünberg had observed an unusual magnetic behavior in a multi-layer package consisting of iron and chromium. Apparently, there is a coupling between two ferromagnetic layers of iron, which are separated from each other by a thin, nonmagnetic and metallic layer of chromium, such that the magnetization of neighboring iron layers is oriented either parallel or antiparallel. Which of these two kinds of couplings occurs, depends on the thickness of the nonmagnetic layer in-between, and varies between antiparallel and parallel with increasing thickness of the layer. Now, during electric current flow along the package of the layers, the electrical resistance depends sensitively on whether two neighboring iron layers are magnetized in the same or the opposite direction. (From a simple energy argument we would expect, that two neighboring iron layers would be magnetized in mutually opposite direction, because in this case the magnetic ﬁelds of the return flux would cancel each other between both layers, and the magnetic ﬁeld-energy would be reduced correspondingly). For our further discussion we assume a multi-layer package, consisting of several ferromagnetic iron layers, where two neighboring iron layers are separated from each other by a thin nonmagnetic chromium layer, respectively. In the absence

10.6

Technical Applications, Giant Magneto-Resistance, Spintronics

185

Fig. 10.7 Giant magneto-resistance: Electrical resistance (in units of the resistance at zero magnetic ﬁeld) plotted as a function of the external magnetic ﬁeld B for different iron-chromium multi-layers at the temperature of 4.2 K. HS denotes the magnetic ﬁeld, at which the magnetizations of the iron layers become oriented in parallel. Identiﬁcation of the multi-layer structures: for example, (Fe 3.0 nm/Cr 1.2 nm)35 denotes a multi-layer package consisting of 35 double layers of one 3.0 nm layer of iron and one 1.2 nm layer of chromium. (M. N. Baibich)

of a magnetic ﬁeld, two neighboring iron layers are assumed to be magnetized in opposite direction with respect to each other. In this case of “antiferromagnetic coupling” between the layers the electric current flow along the package is hindered because of a relatively large resistance. If an external magnetic ﬁeld is applied parallel to the multi-layer package, in all iron layers the magnetization orients itself along the direction of the magnetic ﬁeld, and the electrical resistance shows a strong decrease with increasing magnetic ﬁeld. This is the basic principle of giant magneto-resistance (Fig. 10.7). Such a multi-layer arrangement can still be generalized by dropping the requirement of the antiferromagnetic coupling between the layers. For example, one can imagine magnetic multi-layer systems, in which the magnetization in one ferromagnetic layer is ﬁxed, whereas in the other layer the magnetization can be rotated back and forth. This can be accomplished by means of a large difference in the coercive ﬁeld of the two ferromagnetic layers. In this case a relatively thick nonmagnetic layer in between is also possible. Such multi-layer systems showing giant magneto-resistance even without antiferromagnetic coupling between the layers are referred to as spin valves. The giant magneto-resistance of the spin valves has technically been applied for some time in the reading heads for extracting the data stored in computer hard drives. Within 10 years of the discovery, this technical application has developed into a billion-dollar business. Whereas in one of the two ferromagnetic layers the

186

10

Magnetism: Order Among the Elementary Magnets

direction of the magnetization is ﬁxed, in the other layer the direction is freely adjustable. As the reading head glides along the surface of the hard disk, because of the small magnetic ﬁelds representing the stored digital information in the form of “0” or “1”, the magnetization in this other ferromagnetic layer is rotated back and forth. Simultaneously, the electric current flow changes correspondingly, in this way yielding the output signal. Since still weaker magnetic ﬁelds can be detected by these reading heads, compared with their predecessors, the density of the data stored in the hard disk can be increased by about a factor of three. The magnetic tunnel junction, consisting of three layers, represents another magneto-electronic device. In this case, two ferromagnetic metal layers are separated from each other by an electrically insulating metal-oxide layer with a thickness of only 1 nm. Electric current flow across the junction is only possible because of the quantum mechanical tunneling process. Similar to the spin valve discussed above, the electric tunneling current can flow without additional resistance only if both ferromagnetic layers are magnetized in the same direction. In the opposite case, the tunneling current experiences a high resistance. Again, the direction of the magnetization in one of the two ferromagnetic layers is ﬁxed, whereas in the other layer it can be pointed in the parallel (“0”) or in the antiparallel (“1”) direction, and in this way it can be used for the storage of a unit of digital information. A program for the mass production of these “MRAMs” (magnetic random-access memories) for data storage, based on magnetic tunnel junctions, has been started jointly by the Companies IBM and Inﬁneon. The industrial fabrication of 256-kbyte MRAM chips has been reported recently. As the last example of magneto-electronic devices we discuss an interesting proposal of a ﬁeld-effect transistor operating with spin-polarized electric currents (Fig. 10.8). In this case the electric current is carried by a two-dimensional electron gas at the interface of a semiconductor heterostructure of indium-galliumarsenide (InGaAs) and indium-aluminumarsenide (InAlAs). The two-dimensional electron gas at a semiconductor interface had already appeared in Chap. 7 in our discussion

Fig. 10.8 Schematics of a spin-polarized ﬁeld-effect transistor. The electric current passes through the two-dimensional electron gas at the interface of a semiconductor heterostructure of InGaAs and InAlAs. The current flow is controlled by the voltage Vg applied to the gate electrode

two-dimens. electron gas

10.6

Technical Applications, Giant Magneto-Resistance, Spintronics

187

of the integral and the fractional quantum Hall effect. In the present case, the two-dimensional electron gas represents a current channel with a very high mobility of the electrons. Furthermore, the channel is assumed to be free of collision processes, which can flip the spin of the moving electrons. At both ends of the channel, ferromagnetic metal contacts inject spin-polarized electrons into the channel or extract them again. At the top surface of the semiconductor heterostructure a metal electrode is attached, with which an electric gate voltage can be applied perpendicular to the current channel. The current flow into the magnetized metal contact acting as the collector depends sensitively upon the direction of the spin polarization of the incoming electrons. The electric current can flow almost without any hindrance only if the spins of the electrons are pointing in the same direction as the magnetization in the collector. Otherwise, the current experiences a relatively high resistance. However, in the electric ﬁeld generated perpendicular to the current channel by means of the gate voltage, the spins of the rapidly traversing electrons are rotated. Hence, the electrical resistance of the transistor can be controlled and modulated by means of the gate voltage. Here the rotation of the spin orientation in the electric ﬁeld directed perpendicular to the current channel, is caused by an effect which is explained only by the theory of relativity and which we do not pursue any further here. The examples discussed clearly demonstrate the high potential of magneto-electronics for technical development, which is by no means yet exhausted. Today the most important memory systems for data storage are based on magnetic devices. It is interesting to recall again the impressive development of storage density on hard disks. In a little more than 40 years, from 1956 until 2000, storage density increased by a factor of about ten million. In the year 2000 it was about 2.6 GB per cm2, and in the year 2011 it reached about 65 GB per cm2 (GB = 109 bits). Another important advantage of spintronics results from the fact that the rotation process of the electron spin consumes only very little energy and occurs extremely quickly.

Chapter 11

Nanostructures: Superlattices, Quantum Wires, and Quantum Dots

Abstract The advanced microfabrication techniques can produce objects which are sufﬁciently small, that new quantum effects appear. After discussing superlattices and Bloch oscillations, we turn to the Landauer transmission channels and the quantized conductance of quantum wires. The fullerenes are carbon molecules consisting of different distinct numbers of carbon atoms. Their outgrowth in form of carbon nanotubes represents a promising structure for molecular electronics. Conducting layers of graphene with a thickness of only a single carbon atom display a fascinating electronic band structure, where the concentration of charge carriers can be varied strongly by means of an attached gate electrode. Quantum dots ﬁnd increasing use in optoelectronics. Topological insulators show surprising current-carrying edge or surface states. The topological properties of the electronic band structure and possible contact points between the valence band and the conduction band and band crossings turned into important points of modern developments.

In December of 1959 Richard P. Feynman, one of the most brilliant American physicists of the last century, presented a visionary and highly acclaimed lecture with the title “There is Plenty of Room at the Bottom”. At that time Feynman had already foreseen something that would be conﬁrmed impressively during the following decades because of the rapidly advancing miniaturization in the ﬁeld of microelectronics. He derived one of his leading ideas from the perception of molecular biology at that time, that only about 50 atoms within the DNA double helix are needed for one bit of biological information. The winter of 1952/1953, when Rosalind Franklin of Kings College in London had, with her X-ray images, conﬁrmed for the ﬁrst time the double helix structure of DNA, was still relatively close. If, for comparison, we assume a geometric structure size of an electronic device of 45 nm, the limit which can just be reached by 2012, we ﬁnd for the total number of crystal atoms within a little cube having sides of length 45 nm, the huge number of one million atoms. Here we have taken an average distance of 0.5 nm between the atoms in the crystal. From this comparison we can clearly see, how

© Springer Nature Switzerland AG 2019 R. P. Huebener, Conductors, Semiconductors, Superconductors, Undergraduate Lecture Notes in Physics, https://doi.org/10.1007/978-3-030-31420-0_11

189

190

11

Nanostructures: Superlattices, Quantum Wires, and Quantum Dots

much room there still is today “at the bottom”, compared with the molecular level of biology. It has been the drive for continuous miniaturization in the ﬁeld of microelectronics, which has provided the motivation for improvements in the methods of fabricating microstructured solid objects. In this context, great advances were achieved in the technique for the preparation of thin layers and of multi-layer packages of the relevant materials. Special tricks employed during the deposition on the substrate and during the subsequent etching process, made it possible to fabricate smaller and smaller objects from the thin layers. In the meantime lithography methods have been extended to ultraviolet light and X-rays, in order to achieve higher spatial resolution with much shorter wave lengths. Also, electron beams with high energy are utilized for lithography, and, recently, high-energy ion beams of helium and hydrogen ions have been tested for their suitability to achieve still smaller structural sizes. In many cases these fabrication processes must be carried out in ultra-high vacuum, and only ultra-pure materials can be used. The word “ultra” now appears more and more often in this ﬁeld. Together with the technology for the fabrication of thin layers, the methods for controlling and analyzing the structure and composition of the layers have been continuously improved, and today reach nearly atomic accuracy, if needed. Layers and multi-layer packages of different materials stacked on top of each other can be fabricated, having a microscopically single-crystalline structure. Transmission electron microscopy and scanning probe microscopy allow the analysis of the materials and in particular of their surfaces with atomic spatial resolution. In the meantime, scanning probe microscopy has been applied successfully also at low temperatures. Finally, the techniques for micromanipulation have been developed further, such that it has become possible to perform electric and mechanical measurements even on single atoms and molecules. During the continuously advancing miniaturization of fabricated objects, one ﬁnally reaches spatial scales at which new quantum effects appear. These effects always result because of the nature of the electrons acting as quantum mechanical matter waves. In the following we will illustrate this effect with a few examples.

11.1

Superlattices, Bloch Oscillations

As we discussed in Chap. 2, in a crystal the elementary cell repeats itself along all three spatial directions and in this way generates the three-dimensional periodic structure. This principle is also found in the case of the superlattices, in which the composition of a material is periodically modulated along one spatial direction (Fig. 11.1). Such multi-layer structures are fabricated by means of modern thin-ﬁlm technology. In the year 1970 Leo Esaki and Ray Tsu started to think about and to fabricate “superlattices” out of semiconductors. At the time both worked at the American Thomas J. Watson Research Center of IBM in Yorktown Heights in the Federal State

11.1

Superlattices, Bloch Oscillations

191

Fig. 11.1 In a superlattice, thin layers of two different metals or semiconductors are alternately stacked on top of each other with high regularity

of New York. Already by the late 1950s Esaki had gained much attention because of his research dealing with the electrical behavior of the “Esaki diode”. Then he had studied the unusual features of the electrical resistance of p-n junctions in semiconductors and had identiﬁed the quantum mechanical tunneling process as the crucial underlying mechanism. The quantum mechanical tunneling process allows a particle to pass through a relatively high energy barrier, which classically would be impossible. This process would also play a central role in the Esaki superlattices made from semiconductors. Such a superlattice is fabricated by alternately placing thin layers of two different metals or semiconductors on top of each other during the deposition process. Here great attention must be paid to the atomic accuracy of each layer and to the perfect periodicity of the spatial sequence of the layers. For his experiments Esaki utilized superlattices fabricated from the two semiconductors galliumarsenide and aluminum-galliumarsenide (GaAs/AlGaAs), since this combination of materials yielded samples with the highest quality. As we have discussed in Chap. 7, later on the same semiconductor system GaAs/AlGaAs was used for the fabrication of the two-dimensional electron gas, in which the fractional quantum Hall effect was discovered. In his superlattices, Esaki has stacked up to 100 double layers of GaAs and AlGaAs on top of each other. In such a superlattice the length of a spatial period is about 10 nm, and hence this length is 20–40 times larger than the distance between the atoms in a typical crystal lattice. Here the superlattice structure only exists along one direction, namely perpendicular to the planes of the individual layers. Whereas the quantum mechanical wave function of the electrons does not change very much along the directions parallel to the planes of the layers in the superlattice, along the perpendicular direction the periodicity of the superlattice has a strong influence. Exactly in the same way as electrons, in the form of matter waves, experience Bragg reflection at the crystal lattice, leading to the gaps in the energy spectrum of the electrons, so Bragg reflection also occurs at the periodic structure of the superlattice, and new energy gaps appear. In Chap. 4 we have treated the appearance of Bragg reflection (Fig. 4.4), when the wave vector k of the electrons reaches the boundary of a Brillouin zone and the forbidden gaps in the energy spectrum (Figs. 4.3 and 4.5).

192

11

Nanostructures: Superlattices, Quantum Wires, and Quantum Dots

In the example shown in Fig. 2.9 Bragg reflection occurs at the values kx = p/a and ky = p/b of the wave vector k, where a and b denote the lattice constants along the xand y-direction, respectively. In a superlattice, the (super-) lattice constant along the direction of the modulation (perpendicular to the planes of the layers) is much larger than the lattice constant of the underlying crystal. The wave number, at which the Bragg reflection takes place, is inversely proportional to the distance between two neighboring lattice points within the underlying spatially periodic lattice structure. Therefore, in superlattices Bragg reflection is expected already at correspondingly much smaller values of the wave vector compared with the case of the crystal lattice. As a result, along the directions perpendicular to the layers of the superlattice, there exist energy bands which are much narrower than the usual energy bands, and which are referred to as “minibands”. The existence of these minibands leads to important changes in the electrical properties of the semiconductor superlattice. Ultimately, this was the reason why Esaki studied his superlattices at the time. He was hoping that new and particularly fast electric oscillators would be discovered. If an electric voltage is applied to the superlattice parallel to the direction of the modulation, in the relevant miniband the electrons are accelerated in the direction of the current flow, and they experience a gain in their energy. However, because of the very narrow energy width of the miniband, there is the possibility that the electrons will reach the upper edge of the miniband without ﬁrst losing some energy in a collision process (Fig. 11.2). At the upper edge of the miniband the electrons are reflected, since they cannot traverse the adjoining energy gap in order to reach the next higher miniband. This is exactly the process of Bragg reflection experienced by the electrons representing quantum mechanical matter waves. We illustrate this with the example of a one-dimensional periodic chain of atoms with the lattice constant a. The energy spectrum between the boundaries of the ﬁrst Brillouin zone, p/a und −p/a, is shown in Fig. 11.3. We start from (5.1) for the force acting on the electrons and obtain Dk = e E/h: ð11:1Þ Dt In the absence of any scattering processes, in an electric ﬁeld, an electron (or hole) gains momentum and energy until the value k = p/a is reached. By means of a Bragg reflection, the electron is reflected from k = p/a to k = −p/a, and subsequently its wave number increases again due to (11.1). This process repeats itself and results in a periodic oscillation of the electrons, the “Bloch oscillation”. The time needed for increasing the wave number by the amount Dk = 2p/a, we denote by sB. From (11.1) we obtain 2p=a ¼ e E sB =h and

ð11:2Þ

11.1

Superlattices, Bloch Oscillations

193

Conduction Band

Fig. 11.2 In an electric ﬁeld, the energy bands are inclined in the ﬁeld direction because of the potential gradient, and during their motion the electrons are brought closer to the upper edge of the conduction band. However, in a standard semiconductor (left side) the electrons already experience a collision process, during which their energy is lowered because of the emission of a phonon, long before they reach the upper edge of the band. On the other hand, in the narrow miniband of a semiconductor superlattice (middle) the electrons reach the upper band edge long before a collision process takes place. At the upper band edge they undergo a Bragg reflection, and this process repeats itself as a “Bloch oscillation”, until it is interrupted by a collision process. The enlarged section of a miniband (right side) shows how the electrons move by a distance Dz in the ﬁeld direction with each collision process, at which their energy is lowered by the emission of a phonon Fig. 11.3 Energy spectrum e(k) in the ﬁrst Brillouin zone between k = p/a and k = −p/a

xB 2p=sB ¼ e E a= h:

ð11:3Þ

The angular frequency xB is the Bloch frequency. For the Bloch oscillation to occur, the average scattering time s of the electrons must be sufﬁciently long and must satisfy the condition xB s 1.

ð11:4Þ

Furthermore, for the appearance of the oscillations very pure materials and low temperatures are required. An additional important requirement is a large value of the lattice constant a, resulting in a small energy width of the miniband and in a correspondingly large value of xB according to (11.3).

194

11

Nanostructures: Superlattices, Quantum Wires, and Quantum Dots

Above all, it is the relatively small energy width of the minibands, which plays a crucial role in this behavior. Compared with a semiconductor superlattice, in a usual semiconductor crystal, the width of the energy bands is much larger. Therefore, in this case, during their energy gain in the electric ﬁeld, the electrons already undergo a collision process due to the lattice vibrations long before they have reached the upper edge of the band. During such a collision process energy is always transferred from the electrons to the crystal lattice, and, hence, the upper edge of the energy band remains far away, and the Bloch oscillations cannot occur. However, for the minibands of the superlattice this is totally different (Fig. 11.2). If the electric voltage applied perpendicular to the layers of the superlattice is increased more and more, eventually the electric potential difference between two neighboring unit cells of the superlattice becomes sufﬁciently strong that the cells are decoupled from each other. Whereas at relatively small electric ﬁelds the quantum mechanical wave function of the electrons extends spatially coherently over many cells of the superlattice, and the electronic structure of the minibands still remains intact, at high electric ﬁelds the wave function becomes more and more spatially localized at each individual cell, and decoupling between the cells occurs. Instead of a miniband extending over the whole superlattice, now in each cell individual discrete energy levels exist, which are adjusted to the electrical potential gradient across the superlattice. This splitting of the continuous energy of the miniband into the discrete energy levels is known as the “Wannier-Stark ladder”. The name Wannier-Stark ladder originates from two distinguished physicists: in the beginning of the last century the German Johannes Stark had discovered the splitting of spectral lines due to an electric ﬁeld, referred to since as the Stark effect, while the American Gregory Hugh Wannier had contributed signiﬁcantly to the theoretical foundations of solid state physics. During Bloch oscillation as well as during the splitting of a miniband into the individual energy levels of the Wannier-Stark ladder, the mobile electrons become localized within only a few, and eventually only within a single cell, of the superlattice, because of the electric ﬁeld. This effect increases with increasing electric ﬁeld, such that above a speciﬁc value of the electric ﬁeld the flow of the electric current decreases with increasing voltage. In this case we have negative differential resistance. Instead of consuming energy, the superlattice can now return energy into an oscillating electrical circuit, in this way acting as an active device generating high-frequency electromagnetic waves. The semiconductor superlattices studied by Esaki represent the case of the “heterostructure superlattices” fabricated layer by layer from two different semiconductors. Esaki also had the idea that it should be possible to produce semiconductor superlattices simply and with a high degree of flexibility, only with a single semiconductor, by means of an alternate spatially periodical n-doping and p-doping of this semiconductor. At the beginning of the 1970s, the German Gottfried H. Döhler, at ﬁrst as a postdoctoral member of Esaki’s group, took up this idea of the doping superlattice. Since the n- and the p-doped layers, respectively, are separated from each other by a thin, electrically insulating semiconductor layer, these superlattices are also referred to as “n-i-p-i crystals”. The ﬁrst n-i-p-i

11.1

Superlattices, Bloch Oscillations

195

structures were fabricated in 1980 by Klaus Ploog at the Max Planck Institute for Solid State Research in Stuttgart. These experiments were performed with the semiconductor galliumarsenide (GaAs). Silicon atoms were used for n-doping and beryllium atoms for p-doping. Subsequent electrical and optical measurements with these doping superlattices have well conﬁrmed their expected physical properties. The possibility of fabricating superlattices from semiconductors has introduced an interesting additional option for the development of new materials in electronics and optoelectronics. In superlattices, the electrical and the optical properties can be varied artiﬁcially. In the meantime many experiments have been performed with semiconductor superlattices. However, at present, the technical applications are only in their very early stages. Highly promising developments concentrate on the “quantum cascade laser” operating in the infrared spectral range. Here transitions between the discrete energy levels are utilized, for which the emitted frequency can be tuned by the variation of the material composition and of the thickness of the layers. Recently, interesting progress has been reported also for the generation of microwaves by means of the Bloch oscillations of the electrons in semicondutor superlattices.

11.2

Mesoscopic Regime, Ballistic Electron Transport, Quantized Conductance Value

Eventually, the use of ultra-pure materials and the ability to fabricate objects with smaller and smaller dimensions made it possible, that within the studied sections of the electrically conducting materials, the electrons experience almost no collision processes, or only very rarely. The probability becomes extremely small that, in these experiments dealing with very small spatial dimensions, the measurements are influenced by many structural defects or chemical impurities in the crystal. Furthermore, at sufﬁciently low temperatures most of the lattice vibrations can be frozen out. Under these conditions, the spatial dimensions belong to the “mesoscopic regime”, located between the single atoms or molecules on the one hand and the macroscopic world of events on the other hand. Within this mesoscopic length scale all aspects of the electrons as matter waves are fully valid, and the observed physical behavior of the electrons can best be understood in terms of a propagating wave (Fig. 11.4). In Sect. 5.2 we discussed the Fermi distribution of the energy of the electrons, resulting from the exact identity of electrons as elementary particles, and we have pointed out that, as a result, most electronic material properties are determined only by the electrons from the immediate proximity of the Fermi energy. Therefore, the unperturbed, “ballistic motion” of the electrons within the mesoscopic dimensions happens at the Fermi velocity. In the following we denote the Fermi velocity by vF. Similarly to the Fermi wave number kF, the Fermi velocity vF is also ﬁxed by the Fermi energy eF.

196

11

Nanostructures: Superlattices, Quantum Wires, and Quantum Dots

Fig. 11.4 Photograph, produced by an electron-transmission microscope, of a ring fabricated from a gold layer of 38-nanometer thickness. The inner diameter of the ring is 784 nm. The width of the conducting lines is 41 nm (R. A. Webb)

The unperturbed, ballistic propagation of particles or energy quanta is in contrast to the other limit, in which the propagation is always interrupted by collisions and deflections (Fig. 11.5). A well known example of the latter case is the propagation of light in dense fog, in which all contours disappear, and any orientation becomes impossible. This case is referred to as diffusive propagation, by means of the process of “diffusion”. On the other hand, in the absence of fog we have ballistic and straight arrays of light, propagating with light velocity and clearly marking the spatial environment. The electron transport in the mesoscopic regime in the form of a ballistically propagating wave is characterized by the fact that the internal material properties of the object are no longer decisive, and that, instead, the shape of the external boundary has a much stronger influence. Now the electrons experience collisions and deflections predominantly only at the boundary of the object, for example at the entry or the exit of a constriction. The behavior is much more similar to that in a wave guide. Now the property of the electrons as a quantum mechanical matter wave dominates. Therefore, in the case of such conductors one also speaks of quantum wires. It was the American Rolf Landauer, who considered these questions for the ﬁrst time in the year 1957. Landauer, who originally came from Germany, worked at the American Thomas J. Watson Research Center of IBM. At that time he proposed his famous concept of the transmission channels in mesoscopic electrical conductors, which subsequently turned out to be extremely productive and successful. We will briefly discuss his central idea. The quantum wire is assumed to be placed along the x-direction. At both ends it is connected to electrodes with the energy e þ 1=2 eV and e 1=2 eV, respectively. Here V is the electrical potential

11.2

Mesoscopic Regime, Ballistic Electron Transport …

Fig. 11.5 If the dimensions of an electrical conductor become smaller and smaller (in the ﬁgure from the top to the bottom), the collision processes within the interior of the conductor become less and less important, and the shape of the external boundary will eventually become crucial. In this case the electrons move ballistically as matter waves

197

diffusive

quasi-ballistic

ballistic

difference between both electrodes. If we treat both spins of the electrons separately, we ﬁnd for the current Z I ¼ 2e

dkx 1 1 vx f e þ eV; eF f e eV; eF Ttrm : 2 2 2p

ð11:5Þ

Here, for the Fermi distribution function (5.10), we have used the abbreviation f ðe; eF Þ

1 eðeeF Þ=kB T

þ1

ð11:6Þ

and we have taken into account the current flow in both directions (+x and −x). The quantity Ttrm is a transmission coefﬁcient describing the scattering processes of the electrons, which establish the equilibrium with the local electrochemical potential of the electrodes. We assume that no scattering processes occur within the quantum wire. In the case of small voltage V and low temperatures we have 1 1 @f f e þ eV; eF f e eV; eF eV ¼ 2 2 @ e V¼0 ¼ dðe eF ÞeV:

ð11:7aÞ ð11:7:bÞ

198

11

Nanostructures: Superlattices, Quantum Wires, and Quantum Dots

d(x) denotes the Dirac delta funktion. With vX dkX = (1/ħ)de ﬁnally we obtain the conductance G: G=

I 2e2 ¼ Ttrm ¼ 2GO Ttrm : V h

ð11:8Þ

The quantity GO ¼ e2 =h is the quantized unit of the conductance. Landauer had found, that the electrical conductance of a one-dimensional channel connecting two charge reservoirs has to be measured in quantized units of 2e2/h (The conductance is deﬁned as the inverse of the electrical resistance). In this context we remember the unit h/e2 of the quantized Hall resistance, which we discussed in Chap. 7. The factor 2 of the quantized conductance, according to Landauer, originates from the fact, that here we discuss the case without a magnetic ﬁeld and that, therefore, both spin orientations of the electrons contribute in the same way to the result. On the other hand, the quantized Hall resistance only appears in high magnetic ﬁelds, where both spin orientations clearly must be treated separately. The ﬁrst experiments dealing with ballistic electron transport across a spatial constriction in the mesoscopic regime were carried out in 1965 by the Russian Yurii Vasil‘evich Sharvin. He worked in the famous Institute for Physics Problems in Moscow, which is also named the Kapitza Institute after its founder. In his experiments Sharvin used “point contacts”, prepared by pressing the sharp tip of a metal needle onto the surface of a metallic single crystal. During the electric current flow, at low temperatures, he measured the electrical resistance of this arrangement. However, in these experiments with metals, the role of the electrons as quantum mechanical matter waves is not yet highly pronounced, since, because of the typically relatively large Fermi energy of the electrons in metals, the wave length is only about 0.5 nm and, hence, it is much smaller than the opening of the point contact. Then in 1988 important progress was reported, when almost simultaneously two groups discovered the quantization of the electrical conductance of specially structured semiconductor heterostructures fabricated from galliumarsenide (GaAs) and aluminum-galliumarsenide (AlxGa1−xAs). One group belonged to the University of Delft and to the Philips Research Laboratories in Eindhoven and in Redhill, the other group worked at the Cavendish Laboratory of the University of Cambridge. The semiconductor heterostructure used by both groups was very similar to that in which, a few years earlier, Tsui and Störmer had discovered the fractional quantum Hall effect. In the two-dimensional electron gas of the semiconductor heterostructure the Fermi energy is much smaller than in metals, and correspondingly the Fermi wave length of the electrons is about one hundred times larger than in metals. This provides an excellent opportunity to observe new quantum effects during the passage of electrons through a narrow opening. The two groups used the following technique for the fabrication of the narrow one-dimensional channel between two wide charge reservoirs within the two-dimensional electron gas of the semiconductor heterostructure. They attached two correctly structured metal electrodes, acting as gate electrodes, to the top

11.2

Mesoscopic Regime, Ballistic Electron Transport …

199

conductivity (2e2 / h)

surface of the heterostructure. At the narrowest location the opening between the two gate electrodes was only 250 or 500 nm wide. By applying a suitably selected gate voltage, the sample regions directly below the gate electrodes can be emptied completely of the charge carriers, such that only a conducting channel with an opening width of 250 nm or 500 nm, respectively, remains between both gates. By further increasing the gate voltage, the channel can be constricted even more, until eventually the two wide charge reservoirs are completely separated from each other. During their experiments both groups found that the conductance of their one-dimensional channel shows a regular step structure as a function of the gate voltage, and that the individual plateaus of the steps appeared at integer multiples of the quantized unit 2e2/h of the conductance (Fig. 11.6). These measurements were carried out at low temperatures below 1 K. Apparently, the variation of the gate voltage causes a continuous change in the channel width, such that the number of the discrete and quantized conductance channels increases with increasing channel width. The experimental observation of the quantized conductance of a narrow mesoscopic channel can be looked at as a special case of the concept of transmission channels introduced by Landauer. In the meantime, many papers have appeared dealing with details of this novel quantization phenomenon. However, here we refrain from any further discussion.

gate voltage (V)

Fig. 11.6 Electrical conductance of a narrow one-dimensional channel in a GaAs/AlxGa1−xAs– heterostructure in the quantized unit (2e2/h) plotted as a function of the gate voltage at a temperature of about 1 K. Inset on upper left: Arrangement of the gate electrodes on the surface of the heterostructure. Inset on lower right: cut through the heterostructure (2DEG: two-dimensional electron gas; UG: gate voltage) (B. J. van Wees)

200

11

Nanostructures: Superlattices, Quantum Wires, and Quantum Dots

As the ultimate reduction in the size of an electrical contact between two charge reservoirs, in recent years even single atoms have been studied experimentally and theoretically. These experiments started at the French Commissariat à l’Energie Atomique in Saclay in the group of D. Esteve and Michel H. Devoret with the collaboration of the German guest scientist Elke Scheer. For measurements with individual atoms the technique of piezoelectric actuators, well-known from scanning tunneling microscopy, was employed, in addition to a special technique: the break junction method. The latter method allowed the mechanical control of the contact with an exceptionally high sensitivity. A suspended microbridge of about 2 µm length, 200 nm thickness, and with a 100 nm 100 nm constriction in the middle, was mechanically stretched and eventually broken at the constriction. This was achieved by mounting the microbridge onto an elastic substrate, which could be bent mechanically in a highly controlled way. The authors studied atoms of different metals, such as lead, aluminum, niobium, gold, and sodium. Mostly, the experiments were carried out at temperatures much below 1 K. It was found that, with increasing stretching of the microbridges, the electrical conductance of the samples decreased in steps, until the contact was interrupted. The height of the individual steps was about 2e2/h. The quantized unit of the conductance again appeared. Landauer’s concept of the transmission channels therefore also appears to be conﬁrmed in this case. Furthermore, the experiments performed with the atoms of the different metals suggest that the number of conductance channels is equal to or at least closely related to the number of orbitals of the valence electrons of the central atom. For a quantitative understanding of electrical conductance properties of these contacts, a microscopic model must be developed, which takes into account the orbital structure of the atom as well as the local atomic geometry of the immediate environment. Electrical currents up to about 0.1 mA can pass through a contact consisting only of a single atom. This corresponds to the giant local electric current density of one hundred billion amperes per cm2.

11.3

Bottom up, Fullerenes

For the nanostructures we have just discussed, the sample dimensions are reduced more and more, until eventually one reaches the mesoscopic regime where novel quantum effects in the electron motion can be observed. This method of operation is generally known as the “top-down” procedure. However, for the development of smaller and smaller devices aiming at “nanoelectronics” or eventually also at molecular electronics, the inverse procedure referred to as “bottom-up” gains much more importance. In this case, above all it is the methods of chemistry which are crucial for further advances. From this ﬁeld of the molecular electronics, which presently shows a dramatic development, we wish to select a particular example: the “carbon nanotubes”. However, ﬁrst we must briefly illustrate the preceding history, which has lead to this spectacular development.

11.3

Bottom up, Fullerenes

201

The physics and chemistry of the new forms of carbon started in astrophysics with the exploration of matter within interstellar space. During their experimental attempts to produce interstellar carbon molecules in the laboratory by means of laser evaporation of graphite, in 1985, Richard E. Smalley and Robert Floyd Curl at the American Rice University in Houston, Texas, and also Harold Walter Kroto at the University of Sussex in England, together with their co-workers, discovered the two carbon molecules C60 and C70 by means of mass-spectrometric analyses. At that time they had already presumed, that the C60 molecule possesses the structure of a soccer ball (“bucky ball”), in which the 60 carbon atoms are located at the corners of the ﬁve-cornered and of the six-cornered carbon rings, forming the nearly-spherical surface of the molecule. Altogether, the C60 molecule consists of 12 ﬁve-cornered and of 20 six-cornered carbon rings (Fig. 11.7). The discoverers called the molecule buckminster-fullerene after the American architect Buckminster Fuller, who was famous because of his buildings with a domed structure. Also the C70 molecule is composed of 12 ﬁve-cornered carbon rings, but 25 six-cornered carbon rings. It is stretched slightly and looks similar to an American foot ball. All carbon molecules with an all-round completely closed structure are now denoted as “fullerenes”. Incidentally, more than 200 years ago the Swiss mathematician Leonhard Euler had already proved, that all fullerene structures must have exactly 12 ﬁve-cornered rings, in order to have an all-round completely closed shape. Smalley and Kroto could only produce their fullerene molecules in such tiny amounts, that many supplementary studies and in particular crystallographic structure analyses were impossible. In the year 1990 this changed abruptly, when Walter Krätschmer of the Max Planck Institute for Nuclear Physics in Heidelberg and Donald R. Huffman of the American University of Arizona in Tucson succeeded for the ﬁrst time in producing fullerene molecules in much larger amounts Fig. 11.7 Perspective representation of a soccer-ball-shaped C60 molecule

202

11

Nanostructures: Superlattices, Quantum Wires, and Quantum Dots

than was possible before. Again, both scientists were interested in the preparation of soot particles, because they were dealing with questions about interstellar matter. In their preparation technique they used two rod-shaped graphite electrodes, between which an electric arc is burning with a high current density. During this process the electrode material evaporates. The whole preparation is carried out in an evaporation system, its recipient being ﬁlled with a cooling gas (typically helium). Because of the presence of the cooling gas, the carbon vapor condenses into a smoke of particles, which are then collected. The soot particles and the fullerene molecules are separated from each other by chemical methods. Since May 1990, Krätschmer and also Huffman were able to produce about 100 mg fullerene per day. Now the preparation of single crystals, of microcrystalline powder, and of thin layers followed quickly, and research activities started to grow explosively in many groups. In particular, the initial presumption of the soccer-ball structure of the fullerene molecules was exactly conﬁrmed experimentally. The production method was improved by many groups, and it was scaled up for larger quantities. Now the experiments were extended also to solids consisting of C60 molecules, and electronic properties, as well as the influence of doping with admixtures, were investigated. Following the implantation of strong donors into the C60 solid (n-doping), even superconductivity was found with maximum values of the critical temperature up to Tc = 48 K. Here, the alkali metals potassium, rubidium, and cesium, as well as the alkaline earth metals, were mainly used for electron doping. The C60 and the C70 molecules stand out because of their particularly high stability. Hence, during production their yield is also very high. However, the series of the fullerene molecules still extends much further. For example, there are the “magic” higher fullerenes C76, C78, C82, and C84. In the year 1991 Sumio Iijima from Japan, made a discovery with important consequences for the technical applications, when he observed in the electron microscope for the ﬁrst time a new fullerene type in the shape of thin tubes like a needle. With this discovery of carbon nanotubes, a new phase in the fullerene research had begun. Iijima worked at the Laboratory for fundamental research of the Japanese NEC Corporation in Tsukuba. Since the discovery of carbon nanotubes, the number of publications and also the number of issued patents, dealing with the nanotubes, has grown from year to year. The number of walls of the tubes can vary. In his ﬁrst publication Iijima had already reported tubes with up to seven walls. The tube diameter also varies correspondingly and falls into a range of about 4–30 nm. The typical tube length is about a few µm. Recently, scientists at the American Rensselaer Polytechnic Institute in Troy in the Federal State of New York and at the Chinese Tsinghua University in Beijing have prepared bundles of single-wall nanotubes even up to a length of 20 cm using a special technique (Fig. 11.8). The electronic properties of the multi-wall nanotubes show relatively large variations, which severely hamper their reproducibility. In contrast to this, the single-wall nanotubes are very reproducible. Depending upon their diameter and upon the degree of angular rotation in their structural detail along the axial direction, referred to as the helicity, in terms of their electrical conductivity they behave like a one-dimensional metal or a semiconductor. Apparently, they are well suitable

11.3

Bottom up, Fullerenes

203

Fig. 11.8 Single-wall carbon nanotube placed between two platinum electrodes. The width of the electrodes is 100 nm (C. Dekker)

for use as molecular wires. In addition to the fundamental physical properties of the carbon nanotubes, their potential for application in molecular electronics has been investigated by different groups. Here the manipulation of the nanotubes was accomplished using the methods of atomic force microscopy which we have mentioned in Chap. 1. Apparently, a sharp bend in the single-wall nanotubes acts like a rectifying diode, similarly as a metal-semiconductor contact. Such a bend can be generated by means of a pair of topological defects in the atomic structure of the nanotube, or by a local mechanical deformation. The function of a ﬁeld-effect transistor has been demonstrated already by placing a single-wall nanotube on top of a gate electrode, electrically insulated from the tube. Last but not least, the carbon nanotubes can serve in an excellent way for realizing what are called single-electron effects in electrical transport properties. Here we mean that the physical properties of an object, such as the electrical resistance, for example, are strongly affected by the presence or absence of only a single electron, because of the extremely small dimensions of the object. Because of these developments, large companies within the computer industry presently show a keen interest in the physics and technology of carbon nanotubes. One can hear speculations already that, in the medium-range future, carbon nanotubes may start to compete with the comparatively expensive silicon as the substrate in the semiconductor technology. Carbon nanotubes have an extremely high conductivity for electric currents, and they allow densities of the electric current flow, at which copper wires would have melted long before. Hence, compared to conducting lines made from copper, the carbon nanotubes tolerate much higher electric power levels and operating frequencies. An additional interesting aspect of nanotubes arises due to the possibility that the tubes can be opened at both ends, and that molecules of other substances can be packed into their interior. In this way the tubes can be utilized as carriers of different materials.

204

11.4

11

Nanostructures: Superlattices, Quantum Wires, and Quantum Dots

Graphene

We imagine that the wall of the thinnest carbon nanotube is cut open along the axis, spread out and extended in both directions within the plane. Then we deal with graphene, i.e., with a material with a thickness of only a single carbon atom. The carbon atoms are arranged as a network with a honeycomb structure. In the year 2004, Andre Geim and Konstantin Novoselov succeeded in preparing a graphene sample by using a trick, and subsequently they discovered its fascinating physical properties. By using Scotch tape, they achieved to strip off the top atomic layers of a very pure graphite crystal and to transfer them onto a suitable substrate, such that ﬁnally individual flakes of one-atomic layers became available. Following their initial publications on this subject, an international competing research activity sat in. Within ﬁve years, from 2005 until 2009, more than 5000 papers about graphene were published. Perhaps the most fascinating property of graphene is its electronic band structure. In the undoped state, it shows a linear increase of the energy E of the electrons with their wave number k: E * k. Therefore, the charge carriers act like relativistic particles without mass. Instead of the Schrödinger equation, they satisfy the Dirac equation, and the Fermi velocity vF takes the role of the light velocity. This is in contrast to the usual quadratic increase E * k2 in the case of a three-dimensional crystal (see (4.13) and Fig. 4.5a). In graphene, as the thinnest existing material, the concentration of the charge carriers can be varied strongly, by means of an attached gate electrode and the electric ﬁeld effect. In this way the concentration of the electrons can be changed from that of a regular metal with about 1021 cm−3 to that of a metal with a similar concentration of holes, passing through the (semiconducting) state with only very few charge carriers (Fig. 11.9). In a magnetic ﬁeld, Geim and Novoselov have also clearly observed the half-integer quantum-Hall-effect. The half-integer value arises from the fact that, because of the energy spectrum, at exactly E = 0 there are two energy levels, one with electron character and one with hole character. As an interesting exception, in graphene the quantum-Hall-effect could be observed even at room temperature. In addition to its spectacular electronic properties, graphene has also exceptional mechanical properties. It is harder than diamond, and can become interesting for applications as composite material. Motivated by the characteristic electronic band structure of graphene with its honeycomb-lattice-structure, very recently honeycomb-super-lattices were investigated experimentally and theoretically. Experimentally, these two-dimensional super-lattices consisting of HgTe nano-crystals were fabricated by Daniel Vanmaekelbergh and coworkers at the University of Utrecht using colloid-chemical methods. In this case we deal with the most advanced stage of present research. Experiments on Bloch-oscillations and negative differential resistance due to the electronic mini-bands, as we have discussed in Sect. 11.1, still have to be carried out.

11.5

Quantum Dots

205

Fig. 11.9 In graphene, the concentration of the charge carriers and the electrical conductivity can be varied strongly, by means of an attached gate electrode and the electric ﬁeld effect. The ﬁgure shows the dependence of the conductivity upon the gate voltage and the linear dependence of the Energy E of the electrons upon the wave vector k, E(k), for three values of the Fermi energy EF, in the case of negative, vanishing, and positive gate voltage (A. Geim)

11.5

Quantum Dots

Carbon nanotubes have presented us with a highly promising molecular example as the smallest possible version of a quantum wire. Now we will also drop the last remaining dimension of the spatial extension of these one-dimensional quantum wires. This means that we are dealing with the “quantum dots” as objects with quasi-zero dimension. Again, it is the shape and dimension of the external boundary, which determine the physical behavior of the electrons within the quantum dots. On the other hand, the collision and deflection processes of the electrons in the interior of these objects are moving far into the background. Similar to the situation in an atom, now the quantum mechanical wave function of the electrons is determined to a large extent by the spatial size of the quantum dot. Hence, the quantum dots are also referred to as “artiﬁcial atoms”. Energy bands for the electrons, such as those in an extended crystal, no longer exist. Instead of the energy bands, the electrons can occupy only discrete energy levels, which can be calculated from the geometric dimensions of the quantum dots using the quantum mechanical Schrödinger equation (This is schematically indicated in Fig. 7.3 at the bottom). In some sense, the Periodic Table of the Elements can be imitated by the occupation of individual energy levels of the quantum dots with electrons. Here the Pauli Principle must be obeyed by the electrons as Fermi particles. Hence, each state can be occupied by only two electrons, the spins of which are oriented in opposite directions. However, as an important difference between the quantum dots and the individual atoms we must note that the former are micro-crystals, consisting of about one thousand up to one million atoms, in which lattice vibrations (phonons) and also lattice defects exist. The energy spectrum of the electrons in the quantum dots can be found mainly from their optical properties, for example, from

206

11

Nanostructures: Superlattices, Quantum Wires, and Quantum Dots

the spectroscopy of the energy transitions. It is also not surprising that, for technical applications of quantum dots, the optical properties are particularly interesting, as, for example, in the quantum-dot laser. Quantum dots have been studied experimentally for about the last 20 years. For their fabrication three different general methods are employed. First we mention the relatively traditional “top-down” technique, in which the quantum-dot structures are deﬁned and etched lithographically. However, the necessary processing steps are by no means simple. Furthermore, recently semiconductor nanoparticles, which were fabricated by methods from colloid chemistry, gained special importance. Above all, the II–VI compound semiconductors from the 2nd and the 6th group of the Periodic Table as well as the III–V semiconductors from the 3rd and the 5th group are interesting in the form of nanoparticles. The methods from colloid chemistry yield particles with quasi-spherical shape, the sizes of which can be produced reproducibly from only a few molecules up to highly extended dimensions. Here particles with a diameter between about 1 and 6 nm are particularly interesting, since their fabrication with other techniques is very difﬁcult. This particle size falls into the regime of strong quantization, in which the distance between the discrete energy levels of the electrons in the quantum dots has the same order of magnitude as the energetic band gap in an extended crystal. As a rule, at the end of particle synthesis, a fractionating step for the separation of the particle sizes must be carried out. Based on the colloid chemical methods, quantum dots can be fabricated in amounts of grammes like the standard ﬁne chemicals. Above all, it is the optical properties of these quantum dots, which are interesting for their application, for example, as markers in the fluorescence microscopy of biological samples. The emitted light can be tuned throughout the whole visible spectral range up to the near-infrared range only by the variation of the particle size. Here one utilizes the fact that the distance between the discrete energy levels, relevant for optical transitions, increases with decreasing particle size. The light with the shortest wave length originates from the smallest particles (Incidentally, a similar connection exists between the resonance of the acoustic sound frequency and the spatial size of a musical instrument: the higher the note, the smaller the instrument must be). The third path for the generation of quantum dots becomes possible because of the self-organized, spontaneous growth of well-ordered islands of uniform size in the nanometer range during the deposition of a few atomic monolayers of a semiconductor onto a substrate, under highly special conditions. These self-ordered quantum dots are the ﬁrst nanostructures in the range of 10 nm, which can be produced reproducibly and also in large quantities using the standard methods of semiconductor technology. If the islands with a diameter of only a few nanometers are fabricated from a semiconductor with a small energy gap, and if they are then completely imbedded in a material with a larger energy gap, one obtains electronic quantum dots, which are well decoupled electronically from their environment. For example, quantum dots from indium-galliumarsenide (InxGa1−xAs), imbedded into an environment of gallium-arsenide (GaAs), were intensively investigated. Also three-dimensional lattices of quantum dots can be fabricated by stacking several such layers of quantum dots on top of each other. Again, it is the opticalp properties

11.5

Quantum Dots

207

and in particular the possibility for building a quantum-dot laser, which has stimulated the strong interest in self-ordered quantum dots. Based on these concepts, the ﬁrst quantum-dot laser started to operate in 1994. Since then quantum-dot lasers have been improved considerably in terms of their quantum efﬁciency. Generally, the electronic properties of quantum dots are intermediate between those of bulk semiconductors and of discrete molecules. The quantum-dot technology is particularly attractive because the active region can be modiﬁed to operate at different wavelengths by varying dot size and composition. This leads to the universal use of quantum dots in optoelectronics. In particular, it allows the fabrication of quantum-dot lasers which operate at wavelengths previously not accessible by using semiconductor laser technology. Possible applications of quantum dots include transistors, solar cells, light-emitting diodes, and diode lasers. A spectacular case is the use of quantum dots in flat-panel televisions by Sony in 2013, representing the ﬁrst time they have been used in a mass-produced consumer electronics product. Quantum-dot lasers are expected to play an increasing role in optical data transmission systems.

11.6

Topological Insulators, Metals, and Semimetals

The integer and the fractional quantum-Hall-effect, which we discussed in Chap. 7, can each be understood in terms of new quantum states of the charge carriers in the two-dimensional electron gas. These quantum states appear at the edge of the two-dimensional electron gas (edge states) in the presence of a perpendicularly oriented, high magnetic ﬁeld. They are robust, i.e., insensitive against geometric details and perturbations by impurities. This is the reason for the universality of the numerical values (of the electrical resistivity), which depend only on fundamental constants. In recent years one recognized that similar quantum states with electric current flow through edge channels are possible also in the absence of magnetic ﬁelds. In electrical insulators with a suitable electronic band structure, edge states would be generated, in which charge carriers with opposite spin at a given edge move in opposite directions, different from the quantum-Hall-effect. This phenomenon is referred to as quantum-spin-Hall-effect. Presently, its experimental demonstration represents an important research subject. We will briefly sketch this development. During the search for electrically insulating materials with an electronic band structure which is suitable for this effect, one encountered successfully the compound mercury-telluride (HgTe), a II–VI semiconductor. In this (or a similar) insulator, by means of the spin-orbit coupling, the symmetry of both spin orientations is broken. In the case of the heavy elements, the spin-orbit coupling is particularly strong, and it plays the role of an external magnetic ﬁeld. The quantum-spin-Hall-effect appears at low temperatures (below 10 K) in thin layers (quantum wells), which show a sufﬁciently high mobility of the charge carriers, and which can be fabricated using the technique of molecular-beam epitaxy. In 2012,

208

11

Nanostructures: Superlattices, Quantum Wires, and Quantum Dots

the three pioneers in this ﬁeld, Charles L. Kane, Shoucheng Zhang, and Laurens W. Molenkamp received the highest award in the USA, for their research in the area of the physics of condensed matter, “For the theoretical prediction and experimental observation of the quantum-spin-Hall-effect, opening the ﬁeld of topological insulators”. Today, Kane teaches as a theoretical physicist at the University of Pennsylvania in Philadelphia, Pennsylvania. Zhang worked at Stanford University in California until his early death in 2018. The experimental physicist Molenkamp is heading a group at the University of Würzburg, which concentrates on molecular-beam epitaxy of II–VI semiconductors. A topological insulator is a material, which in its interior behaves like an electrical insulator, and which, at its surface (or at its edge), can transport electric charges. The topological insulators represent an advancement in the ﬁeld of spintronics, which we discussed in Chap. 10 in the context with the technical applications of magnetism. So far we discussed only two-dimensional topological insulators with their current-carrying edge states. In 2007 Charles Kane, mentioned above, together with Liang Fu, predicted that also three-dimensional forms of topological insulators would be possible, in which conducting quantum states appear at the crystal surface (surface states). A ﬁrst example is Bi1−x Sbx, a compound of bismuth (Bi) and antimony (Sb), in which the spin-orbit coupling is particularly large. So far, the experiments have conﬁrmed this prediction. In Bi1−x Sbx the surface states are similar to the two-dimensional states in graphene. As we discussed in Sect. 11.4, in graphene near the Fermi energy, electrons and holes show a linear relation between energy and wave number, which is described by the relativistic Dirac equation of massless fermions. In two-dimensional k-space, the dispersion relation shows the form of two cones stacked on top of each other, the cone ends of which coincide at discrete points (Dirac points) at the Fermi energy (see Fig. 11.9). Whereas graphene shows an even number of Dirac points (namely two), in the case of Bi1−x Sbx there is an odd number. As a result, in graphene the surface states are not topologically robust, and an energy gap easily opens up because of perturbations (impurities). On the other hand, in Bi1−xSbx the surface states are robust (topologically protected) and insensitive against perturbations. Shortly after the discovery of bismuth-antimony as a three-dimensional topological insulator, there were indications of topologically protected surface states also in antimony, bismuth-selenide, bismuth-telluride, and antimony-telluride. Since the 1980s, the ﬁeld of the topological materials has developed rapidly. Here the topological symmetry properties of the electronic band structure in k-space play an important role. In this case the highly fruitful geometric concept of the electronic band structure in k-space promoted by Lars Onsager, which we had pointed out in Sect. 5.3, becomes apparent again. Topology is a subﬁeld of mathematics, which deals with the geometric distortion of objects and the underlying general common aspects. In a famous example it is shown, how a cup with a handle can be distorted continuously into a torus, such that both objects are topologically equivalent. The number of holes in an object remains as the important distinguishing feature. In applying these topological concepts to the electronic crystal properties, the band gap between the valence band and the conduction band

11.6

Topological Insulators, Metals, and Semimetals

209

takes up the role of the holes of the geometric example. In the topological band theory the possible individual cases are classiﬁed in terms of topological indices such as Berry phase and Chern number, which we do not want to discuss here any further. Band crossings between the valence band and the conduction band turned into important subjects of modern developments. In 1996, Martin R. Zirnbauer and co-workers had developed a scheme for classiﬁcation of symmetries of universal properties, which is fundamental also in the case of topological insulators. Today, Zirnbauer is director of the Institute of Theoretical Physics at the University of Cologne. In 2012 he received the Max-Planck-Medal of the German Physical Society for his work. Topological quantum states of matter are very rare. It is noteworthy, that after more than 80 years the electronic band theory of crystals still offers surprises. Already in 1937, the Amerikan Conyers Herring published a paper based on his PhD thesis discussing the accidental energy coincidence of individual states of the electronic band structure of the valence band and the conduction band (“contact points”) in momentum space. He had performed his thesis at Princeton University under the supervision of Eugene Wigner. Herring had studied theoretically in particular the important influence of the symmetry of the crystal lattice on the stability of the contact points in the presence of impurities and other perturbations. Recently (2015), the special cases of the structure of the conduction and valence bands linearly depending on the wave vector k and coinciding at discrete points in k-space, attract increasing attention. (In Fig. 11.9 we show an example in the case of graphene.) The property of fermions having zero mass, resulting from the linear dispersion curves, leads to interesting new physical properties. These developments are based on important advances both in the experimental techniques (angle-resolved photoelectron spectroscopy, ARPES) and in the theoretical band-structure calculations (density functional theory). Already in 1929, the German mathematician Hermann Weyl had predicted the existence of massless Fermi-particles as solutions of the Dirac-equation. Weyl had obtained his PhD in 1908 in Göttingen under the supervision of David Hilbert and subsequently worked in Zurich and in Göttingen. In 1933 he emigrated to the USA, and for many years he worked at the Institute of Advanced Studies in Princeton. There he met again Albert Einstein, whom he had known already from Zurich. The so-called Weyl-semimetals at the Weyl points in momentum space, only possess a single state, which is stable. Furthermore, at the surface of a Weyl-semimetal there appears a novel surface state. In contrast to a Weyl-semimetal, in a Dirac-semimetal the state at the Dirac-points in k-space is twofold degenerate and instable. Presently, an intensive search is carried out for materials having these peculiarities in their electronic properties, and some success has been reported already.

210

11.7

11

Nanostructures: Superlattices, Quantum Wires, and Quantum Dots

Aharonov-Bohm Effect

At the end of this chapter on quantum effects in mesoscopic structures, we wish to return to the geometry of a ring in an external magnetic ﬁeld. This geometry occupied us in Chap. 8 in the context of magnetic flux quantization in superconductors. Nevertheless, in the superconductor we had to deal with the macroscopic wave function of the Cooper pairs with their double elementary charge 2e. However, now we are interested in the quantum effects of the ballistic electron motion within the ring geometry of a normal conductor with sufﬁciently small dimensions, such that the collision processes of the electrons in the interior of the object are negligible and only the external boundary is crucial. The external magnetic ﬁeld will be oriented perpendicular to the plane occupied by the ring. We assume that the diameter of the ring is much larger than the width of the ring-shaped conducting line. For the electron motion along the ring we must take into account the interference during the propagation of the matter wave along the right-half and along the left-half of the ring. It turns out that the propagation difference of the wave between the right and the left path amounts to exactly one wavelength or to an integer multiple thereof, if the magnetic ﬁeld penetrating the ring area corresponds to one magnetic flux quantum (h/e) or to an integer number of magnetic flux quanta. Here it is assumed that both halves of the ring are exactly symmetrical. As a consequence of this interference between the two propagation paths we expect a periodic oscillation of the electrical resistance of the ring conﬁguration during the variation of the external magnetic ﬁeld, with the periodicity (h/e) of the enclosed magnetic flux quanta. We have been confronted with the magnetic flux quantum (h/e) before in our discussion of the fractional quantum-Hall-effect. On the other hand, if we compare the two complete trajectories around the whole ring clockwise and anti-clockwise, respectively, leading back to the same starting point, then the propagation difference between both waves after a complete revolution is exactly one wavelength, if only half a flux quantum (h/2e) occupies the ring area. Correspondingly, this results in a periodic oscillation of the electrical resistance of the ring conﬁguration during the variation of the magnetic ﬁeld with periodicity (h/2e) of the enclosed half magnetic flux quanta. A fundamental difference between the two cases we just have discussed arises due to the fact, that the (h/e) oscillations depend sensitively upon the details of the sample. For example, the exact symmetry between the two halves of the ring becomes extremely important. On the other hand, the (h/2e) oscillations arise only from the comparison between the two complete trajectories around the whole ring along opposite directions, respectively. These two cases are related to each other by the process of time inversion. Hence, they are independent of the microscopic details of the sample. This discussed interference behavior of electron matter waves was predicted theoretically for the ﬁrst time in 1959 by Yakir Aharonov and David Bohm. Hence, this is referred to as the Aharonov-Bohm effect (Fig. 11.10). At the time both scientists worked at the University of Bristol in England. In the early 1960s the effect was demonstrated in interference experiments performed with

11.7

Aharonov-Bohm Effect

211

Fig. 11.10 Aharonov-Bohm effect in ring geometry. The external magnetic ﬁeld is oriented perpendicular to the plane of the ring. a The interference between the trajectories through the right and through the left-half of the ring leads to oscillations in the electrical resistance with periodicity (h/e) of the magnetic flux enclosed by the ring. b For a complete revolution of two trajectories around the ring in opposite directions, respectively, the interference results in oscillations of the resistance with periodicity (h/2e)

electron beams by Gottfried Möllenstedt and co-workers at the University of Tuebingen. For the ﬁrst time the Aharonov-Bohm effect of electrons in a solid has been observed experimentally by Yurii Vasil’evich Sharvin and his son D. Yu. Sharvin in the year 1981 in Moscow. They used a thin metal cylinder made from magnesium with a diameter of 1.5–2 µm and a length of 1 cm. The cylinder was deposited as a thin layer onto a thread of quartz. The magnetic ﬁeld was oriented parallel to the cylinder axis. The temperature was 1 K. The cylinder can be looked at as an object consisting of many rings stacked on top of each other. Therefore, the (sample speciﬁc) (h/e) oscillations average out, and only the (h/2e) oscillations of the electrical resistance could be observed at the time. However, the (h/e) oscillations were also detected experimentally in 1985 for the ﬁrst time by the American Richard A. Webb and his co-workers at the Thomas J. Watson Research Center of IBM in the USA. They used metallic gold rings fabricated from a thin gold layer of only 38 nm thickness (Fig. 11.4). The crucial preparation step in the fabrication of the extremely small structures was the formation of a suitable mask consisting of a protecting contamination layer by means of a computer-controlled high-resolution scanning electron transmission microscope. At a temperature of 0.01 K a gold ring with 784 nm inner diameter and 41 nm width of the conducting line displayed distinct (h/e) oscillations of the electrical resistance during variation of the external magnetic ﬁeld.

Chapter 12

Defects in the Crystal Lattice: Useful or Harmful?

Abstract At thermodynamic equilibrium crystals display some disorder due to the spontaneous generation of lattice defects, as we discuss in the case of lattice vacancies. Other examples of defects are color centers in ionic crystals and radiation damage in nuclear reactors. Understanding the role of dislocations in the mechanical properties of materials represented a great advance. Today, nondestructive materials testing has developed into an important ﬁeld. Magnetic impurities and the Kondo effect are discussed.

During the course of many hundreds, if not thousands. of years, people have gained important and useful experience and have learned rules and recipes for the manufacture, in particular, of things made from metallic materials. At ﬁrst, mechanical properties and strength under mechanical loads, exclusively dominated people’s interest in materials. For example, it had been discovered early on, how long one should hammer a piece of metal in order for it to gain the optimum hardness for its use as a tool, weapon, ornament, or coin. Only in the 19th century was the cold straining and cold-work hardening systematically developed, and at the time it reached an impressively high standard, for example, in the large rolling machines of the steel industry. For a long time, this ﬁeld of metallic materials was dominated by pure empiricism. The microscopic structure of wrought iron was observed for the ﬁrst time only in 1863. At the time, these experimental studies were performed by Henry Clifton Sorby, who was born in a suburb of Shefﬁeld, one of the centers of the English iron and steel industry. As an amateur geologist he was interested in the structure of rocks. After he had polished and subsequently etched his samples of wrought iron, in his light microscope he discovered characteristic structures at the sample surface, which are referred to today as the texture of a metallic sample. About 20 years later, Adolf Martens carried out pioneering research in this ﬁeld, and he gained high recognition as the founder of texture microscopy and of scientiﬁc materials testing in Germany. A prominent milestone in Germany at the time was the establishment of the Kaiser-Wilhelm-Institute for Metals Research in Neubabelsberg near Berlin in the year 1920. During 1934 this Institute was moved to Stuttgart. After the Second World War the latter Institute continued in Stuttgart © Springer Nature Switzerland AG 2019 R. P. Huebener, Conductors, Semiconductors, Superconductors, Undergraduate Lecture Notes in Physics, https://doi.org/10.1007/978-3-030-31420-0_12

213

214

12

Defects in the Crystal Lattice: Useful or Harmful?

as the Max Planck Institute for Metals Research. Similar Institutes were established also in the other industrialized countries. (In 2011 the Institute in Stuttgart was renamed Max Planck Institute for Intelligent Systems). After the many discoveries in the ﬁeld of electricity and magnetism in the 19th century, the electric and the magnetic material properties appeared as important new subjects, which had to be investigated. As we have discussed in Chap. 1 in conjunction with the crash of the two English Comet passenger airplanes, it is always the spectacular events and catastrophes, which impressively demonstrate the need for an almost complete understanding of material properties.

12.1

Disorder at Thermodynamic Equilibrium

Even in the purest crystal, from which all undesired impurities have been removed very carefully, there are unavoidable lattice defects for important fundamental reasons. This arises from the fact that the stable equilibrium state of a substance always requires a distinct amount of disorder. It is the “thermodynamic potential”, which rules the development of the state of equilibrium in a physical system. Only in the presence of some disorder does the thermodynamic potential attain its minimum value, which guarantees equilibrium. The only exception from this exists at absolute zero temperature. The underlying ideas were developed by two physicists in the 19th century: The German Hermann von Helmholtz and the American Josiah Willard Gibbs. In this discussion of disorder, the concept of “entropy” plays a central role. The amount of disorder necessary for establishing the equilibrium can be achieved in crystals by means of the fact that, in the otherwise perfect single crystal, individual lattice sites remain unoccupied by atoms, and a certain number of lattice vacancies are generated in this way.

12.2

Vacancies in the Crystal Lattice

With the example of lattice vacancies in crystals, we will illustrate the thermodynamic treatment. We start with the free enthalpy of a crystal: G ¼ UþpV TS

ð12:1Þ

(U = inner energy; p = pressure; V = volume; T = temperature; S = entropy). From (12.1) we see that an increase in entropy (due to disorder) reduces free enthalpy. Because of the TS-contribution in (12.1), with increasing temperature, this reduction of free enthalpy becomes more and more important. This is exactly the reason, why in thermodynamic equilibrium there appears disorder in a crystal. We consider a crystal consisting of N identical atoms. The presence of n lattice vacancies changes the free enthalpy G by the amount

12.2

Vacancies in the Crystal Lattice

215

DGðn; p; TÞ ¼ n UA þ n p VA n T SA vibr T ðN þ nÞSm :

ð12:2Þ

In (12.2) the proportionality with n is valid only for values of n, which are small compared with N, n N. (In (12.2): UA = activation energy for the formation of a vacancy; VA = activation volume for the formation of a vacancy; SA vibr = entropy change of the lattice vibrations per vacancy; Sm = mixing entropy per particle). The mixing entropy per particle is X Sm ¼ kB xj ln xj ; ð12:3Þ j

where xj denotes the atomic fraction of component j. In the case of vacancies, we have n n N N ln kB ln nþN nþN nþN nþN n n n kB ln þ kB ln 1 þ N N N n n n ln ; kB N N N

Sm ¼ kB

ð12:4aÞ ð12:4bÞ ð12:4cÞ

(again, within the approximation n N). In equilibrium we have

@ DG @n

¼ UA þ p VA T SA vibr þ kB T ln p;T

n ¼0 N

ð12:5Þ

and cðp; TÞ

nðp; TÞ ¼ exp SA vibr =kB exp½ ðUA þ p VA Þ=kB T: N

ð12:6Þ

From (12.6) we see that by plotting log c versus 1/T or versus p, one obtains straight lines (Fig. 12.1). From the slope of the plot versus 1/T one obtains UA + p VA (where, in general, the contribution p VA at p = 1 at is negligible). From the slope of the plot versus p one obtains VA. The equilibrium concentration of vacancies strongly increases with increasing temperature. The spontaneous generation of lattice vacancies contributes also to the volume expansion of the crystal, in addition to the usual thermal expansion. Therefore, the volume expansion turns out to be somewhat larger than expected only from the thermal expansion of the characteristic distance between neighbors in the crystal lattice. The volume of the vacancies must be added also. This effect was detected in a famous experiment by Ralph O. Simmons and Robert W. Ballufﬁ. They compared the measured relative length change DL/L of a crystal with the relative change Da/a of the lattice constant,

216

12

Defects in the Crystal Lattice: Useful or Harmful?

ΔL/L or Δa/a in units 10-3

Fig. 12.1 Plot of log c versus 1/T (left) and versus p (right), schematically after (12.6)

temperature (°C)

Fig. 12.2 Influence of the vacancies, existing in equilibrium within the crystal lattice, upon the temperature dependence of the crystal volume of aluminum. Because of the thermally generated vacancies, the temperature dependence of the relative length change, DL/L, (upper curve) is slightly larger than the temperature dependence of the relative change of the distance between neighbors in the crystal lattice, Da/a (lower curve). The difference between both curves increases with increasing temperature. (R. O. Simmons and R. W. Ballufﬁ)

obtained from X-ray diffraction. In Fig. 12.2 we show their results obtained with an aluminum sample. Incidentally, the volume of a single vacancy is considerably smaller than the volume corresponding to a single atom in the unperturbed crystal (the “atomic volume”), since the neighboring atoms around the vacancy move a bit closer toward each other, and the crystal lattice becomes distorted at this location. The formation of the vacancies is accompanied by a distinct increase of the “inner energy” of the crystal. This also leads to an additional contribution to the speciﬁc heat of the crystal. In the noble metals, copper, silver, and gold, not far below their melting

12.2

Vacancies in the Crystal Lattice

217

temperature, we have about one single vacancy per one thousand lattice atoms. In equilibrium at room temperature the vacancy concentration is smaller by many powers of ten. Furthermore, the vacancies generated in the state of equilibrium can move through the crystal by means of diffusion. During an elementary diffusion jump from one lattice site to the next, vacancies pass through an activated state, in which they are located between two neighboring lattice sites. We denote the number of vacancies in the activated state by n*. For the ratio n*/n one obtains an expression analog to (12.6), in which the following quantities appear: the activation energy of motion, UB, the activation volume of motion, VB, and the change of the entropy of the lattice vibrations, SB vibr : n =n ¼ exp SB vibr =kB exp½ ðUB þ pVB Þ= kB T:

ð12:7Þ

If the concentration of vacancies is sufﬁciently high, they can combine with other vacancies forming double vacancies, similar to a molecule consisting of two atoms. Still larger complexes of vacancies are also possible. In this way an extensive reaction scheme of the vacancies and their larger “molecular compounds” develops. Lattice vacancies and their motion through the crystal also represent an important mechanism for atomic materials transport in crystals and for solid state chemistry. In a crystal the process of hopping from site to site is only possible, if unoccupied lattice sites are available. Therefore, chemical reactions and the diffusion processes in a solid are closely related to the dynamics of vacancies. (This is highly important, for example, for achieving the optimum oxygen concentration in high-temperature superconductors). Before the concept of lattice vacancies had been established, one assumed that there must exist some kind of “pores in the lattice” or “loosened sites”, which allow the transport of matter. In the context of this discussion it is important to note that we have only considered the case of single crystals and that, hence, we have ignored grain boundaries between single-crystalline grains with different crystallographic orientation. Very often such grain boundaries do exist, and then they provide favored diffusion channels for the transport of matter throughout the whole crystal. Whereas in the case of the vacancies an atom is missing at its site in the crystal lattice, there is also the possibility, that one atom too much is present, which must then push itself between the other atoms and accommodate itself at an “interstitial lattice site”. Again, around the interstitial atom the crystal lattice is distorted. In general, the energy gain in the crystal due to the interstitial atom is much larger than that for a vacancy, since the regular atoms in the lattice cannot be pushed away so easily, in order to make room for the newcomer. For the ﬁrst time, the Russian Abram Fedorovich Ioffe proposed the idea of the interstitial lattice sites in the year 1916. During the irradiation of crystals with highly energetic particles, vacancies and interstitial lattice atoms are often generated together, if, for example, due to the particles of the radiation one atom is shot away from its regular lattice site and then must again ﬁnd another place for itself within the crystal lattice. The pair of defects

218

12

Defects in the Crystal Lattice: Useful or Harmful?

consisting of a vacancy and an interstitial lattice atom in the crystal is referred to as a Frenkel defect. This name originates from the Russian theoretical physicist Jakov Iljitsch Frenkel, who as a collaborator of Ioffe belonged to Ioffe’s Institute in Leningrad. In the year 1925 he developed a theory of the defect pair, which was later named after him. In the beginning of the studies of vacancies and interstitial lattice sites in a crystal, both of which are also referred to as point defects, attention was concentrated on the “ionic crystals”. This type of crystal is composed of positively and negatively charged ions. Since the ions have either given up an electron or have taken up one, they possess the favored closed electron shells. Since the number of ions with the opposite electric charge, respectively, is exactly equal, charge neutrality in the crystal is maintained. The binding in the ionic crystals arises from the attractive force between ions with the opposite electric charge, as we discussed in Sect. 2.3. Ionic crystals cannot conduct an electric current and are electrical insulators. A typical example is common salt, NaCl, composed of positive sodium ions and negative chlorine ions. Already in the 1920s, the First Institute of Physics directed by Robert Wichard Pohl at the University of Göttingen in Germany was a prominent location for the investigation of ionic crystals. In addition to his scientiﬁc research, Pohl also became famous because of the highly impressive and intuitive style of his main course in Experimental Physics, which was known as “Pohl’s circus”. This has also become visible in the many editions of his famous textbook on Experimental Physics consisting of three volumes. In Pohl’s Institute many physical properties of the ionic crystals were studied. These crystals are transparent in a large spectral range. However, their electrical and optical properties are extremely sensitive against point defects and other perturbations in the crystal lattice. In particular, the point defects became famous, since they act as “color centers” and display characteristic optical properties. Actually, they were the ﬁrst crystal defects, which were carefully studied experimentally and theoretically. Eventually, different kinds of color centers were discovered in ionic crystals, predominantly due to their optical spectral properties, and theoretical models were subsequently developed for the interpretation of the experimental results. For example, for a speciﬁc center one could show that it must correspond to a vacancy, where a negative chlorine ion ðCl Þ was missing, and where an electron was trapped. At the end of the 1930s it was mainly the Englishman Nevill Francis Mott, who applied quantum mechanics to lattice defects in crystals, similarly to the way in which it had been done before in the physics of atoms. Working in Bristol, Mott directed his attention in particular to the results obtained by Pohl’s group in Göttingen. In the USA at the time it was mainly Frederick Seitz, who took up theoretical studies in this ﬁeld. The point defects in ionic crystals then appeared to represent a relatively simple, but highly promising, ﬁeld of study, from which valuable knowledge also about the electrical properties of semiconductors and the mechanical properties of metals could be gained. In Göttingen, Pohl had established, perhaps worldwide, the ﬁrst signiﬁcant school of solid state physics. He came to Göttingen in the year 1918. Prior to that he had worked in Berlin, among other things on questions dealing with the emission of electrons from metal surfaces under light irradiation (the photo-electric effect), and at the end on problems of the radio technique. When he was asked sometime later, why in Göttingen he shifted his interest mainly to the interior of crystals, he gave the (not so serious) answer, that in the impoverished Göttingen the ﬁnancial means were not sufﬁcient for experiments carried out in high vacuum.

12.3

12.3

Materials Science of Radiation Damage

219

Materials Science of Radiation Damage

During the Second World War, in the USA new developments started because of the operation of the ﬁrst nuclear reactor. On the afternoon of December 2, 1942 at about 3:30 p.m. the ﬁrst nuclear chain reaction was realized in the uranium/graphite pile, which Fermi and his team had constructed below the west stand of the Stagg Field Stadium at the University of Chicago. At the time this achievement was immediately forwarded in the famous encoded announcement: “The Italian navigator has just landed in the New World. …The natives were very friendly.” This event represented the start of the technical use of nuclear reactors for the production of energy. Hence, the ﬁeld of defects and radiation damage in crystals and in metallic materials gained an extreme practicality. At the time, the theoretical physicist (also trained as a chemical engineer) Eugene Paul Wigner feared that the energetic neutrons generated within the reactor would cause a dangerously high concentration of lattice defects in the graphite used for slowing down the neutrons (resulting in an explosive reaction). A similar fear was expressed by Leo Szilard who, like Wigner, also originated from Hungary. The problems were then soon referred to as the “Wigner disease” or the “Szilard complication” by participating co-workers. At the time, the extreme practicality of the subject of radiation damage in crystals and in metallic materials had caused Frederick Seitz to strongly intensify his relevant theoretical calculations. Incidentally, it was Szilard, who only a few years earlier, after the discovery of nuclear ﬁssion by Otto Hahn and Fritz Strassmann in Berlin, had moved Albert Einstein to write his famous letter to the American President Franklin Delano Roosevelt, in which Einstein warned against the possibility of the Atomic Bomb. In the years 1949–1951 Frederick Seitz established a center for basic research in the ﬁeld of defects and radiation damage in solids at the University of Illinois in Urbana. Later on, from the gained knowledge one could estimate, for example, that during an operation time of 10 years of a fast breeder reactor, in its inner components each lattice atom is expelled on the average 340 times from its lattice site into an interstitial position (and back again). An early estimate for the ﬁrst wall of a fusion reactor yielded a similar number, namely 170. In the context of the doping of semiconductors we have become acquainted already with artiﬁcially generated defects or with imperfections caused by chemical admixtures in the crystal lattice. Another example are the pinning centers in superconductors which, as local perturbations of the crystal lattice, hinder the motion of the quantized magnetic flux lines, and hence, strongly reduce the heat losses during electric current flow. In both cases the defects in the crystal exercise highly useful functions. Next we will look more closely at the role of lattice defects in the mechanical strength of materials,

220

12.4

12

Defects in the Crystal Lattice: Useful or Harmful?

Mechanical Strength of Materials

In the year 1660, the Englishman Robert Hooke studied experimentally the elastic strain of metals under mechanical load, and in doing so he discovered the famous Hooke’s law named after him. Later on, for a few years he was Secretary of the Royal Society in London. Hooke’s law says that the elastic strain increases exactly linearly with increasing mechanical load. If the load is removed, the strain returns back to zero. The strain is still reversible. In this context the concept of mechanical stress was introduced. In the simplest case of a rod pulled in a longitudinal direction, it is the pulling force per unit cross-section of the rod. From Hooke’s law the stability of metal structures can be calculated. Hence, in 1779, the ﬁrst bridge worldwide made completely from iron was built near Birmingham in England. Subsequently, it has carried the road trafﬁc for 170 years. In subsequent discussions and in the technical use of their elastic properties, for a long time metals were treated as continuous matter, without paying attention to their inner microscopic structure. However, the still relatively simple, elastic behavior according to Hooke’s law is observed only if the strain of the material does not become too large. Above a critical strain level, plastic deformation sets in, and eventually the material tears apart. Now the changes in the material due to the mechanical load are no longer reversible. At this point the microscopic structure must be taken into account. The same applies also to the changes occurring in metals during bending, rolling, or forging. However, until late into the 19th century, nobody knew what actually happened during these processes. After the crystal structures of the metals were clariﬁed by means of the diffraction of X-rays, the question had to be answered of how the crystal lattice is deformed during mechanical working of the metals. At the time, the largest advance in knowledge was hoped to be gained from samples consisting only of a single crystallite, referred to as single crystals. At the beginning of the 1920s at the Kaiser-Wilhelm-Institute for the Chemistry of Fibrous Materials in Berlin-Dahlem, Hermann Francis Mark, Michael Polanyi, and E. Schmid performed controlled mechanical tension tests with single crystals of zinc. Their experiments showed that the deformation of the metals under tension occurs by shifting parts of the crystal along distinct gliding planes, where the gliding plane and the gliding direction depends upon the crystal structure. During this process the microscopic crystal structure itself remains unchanged (Fig. 12.3). Experiments at the Cavendish Laboratory in Cambridge, England yielded similar results. However, during this research there appeared puzzling surprises. During their deformation, the metals seemed to become mechanically stronger. Therefore, it was presumed that, during the deformation defects are generated within the crystal lattice, which make further deformation more difﬁcult. Furthermore, the calculation of the mechanical tension, at which parts of the crystal start shifting relative to each other, yielded values which were up to thousand times larger than the experimental data. Apparently, the metal crystals were much softer than expected theoretically. Something in the concept was wrong, and a new mechanism had to be invented.

12.4

Mechanical Strength of Materials

221

Fig. 12.3 Deformation of a crystal due to slippage, schematically. Only the front plane of the crystal lattice is shown, and additional lattice planes are further behind. The microscopic crystal structure in the undeformed (top) and in the deformed state (bottom) remains the same. (U. Essmann)

The way out of this dilemma was provided by three scientiﬁc papers, all of which were published independently of each other in 1934. The model required had to present a strategy, in which in the ﬁnal result, a more or less local defect, by its motion through the crystal lattice, achieved a gliding motion of large parts of the crystal relative to each other. In other words: a small cause must achieve a large effect. One of the authors was Michael Polanyi, who had studied the plasticity of metals for some time. The second paper was written by the Englishman, Sir Geoffrey Taylor. During the First World War, he had investigated the susceptibility of crankshafts to cracks for the Royal Air Force, and he had worked on theories about crack formation and crack propagation. Subsequently, as Royal Society Professor at the University of Cambridge, Taylor studied the plasticity of metal single crystals and the processes during their deformation. Egon Orowan, originating from Hungary, was the third author. In the 1920s he had studied electrical engineering at the Technical University in Berlin-Charlottenburg, and also developed an interest in physics. Orowan became acquainted with the problems of plastic deformation through Richard Becker, at the time just recently appointed as Professor of Theoretical Physics. Shortly before, Becker had proposed a theory on this subject. One day, Orowan had to visit Becker in his ofﬁce because of a required signature. How this event abruptly changed the career of the young student, was told by Orowan later as follows: In the next minute my course of life was changed. This happened because of the exceptionally large ofﬁce of the professor. Becker was a shy and hesitating person; however, on my way out, before I had reached the door of his huge ofﬁce, he had arrived at a decision. He called me back and asked if I would not be interested to experimentally check a little theory of plasticity, which he had worked out three years ago. To engage oneself in plasticity looked like a prosaic, if not downgrading proposal during the age of a De Broglie, Heisenberg, and Schrödinger, however, it was still better than having to calculate my sixtieth transformer, and therefore, I accepted.

222

12.5

12

Defects in the Crystal Lattice: Useful or Harmful?

Dislocations

In the quoted three papers the concept of a “dislocation”, which moves through the crystal as a local perturbation of the crystal lattice, was proposed for the ﬁrst time. Here an additional plane of atoms is inserted into part of the crystal, which at its end within the crystal forms the “dislocation line” (Fig. 12.4). In the region around this dislocation line the crystal lattice is distorted. If the dislocation moves along its gliding plane through the crystal, at the end of this motion two parts of the crystal are displaced relative to each other by one atomic distance. During this process only individual atoms on the dislocation line are always displaced by not more than a single atomic distance (Fig. 12.5). In this way, during a deformation it is no longer necessary, to displace all atoms on the gliding plane simultaneously. In agreement with experiment, a relatively small shear stress is now sufﬁcient to induce the motion of the dislocation. At one time, Nevill Francis Mott has vividly illustrated this process: The analogy with a wrinkle in a carpet is very useful… We all know that there are two methods for moving a carpet along the floor. Either we can grab one end and pull, or we can form a wrinkle at one end and drive it carefully to the other end. With a large, heavy carpet the second method needs less effort… Now we want to look at the situation in a crystal. What I have called here a wrinkle, in the technical jargon is denoted as a ‘dislocation’… We see that we arrive at the same result, if a dislocation is generated at one end of the crystal and then moves through the crystal, as if one half is gliding over the other ….

The dislocation line must be understood as the boundary line of a section of the gliding plane, at which the adjoining parts of the crystal on both sides of the gliding Fig. 12.4 Model of an edge dislocation in a simple-cubic lattice. In the lower half one can see an additional (vertical) plane of lattice atoms. (W. Sigle)

12.5

Dislocations

223

Fig. 12.5 Slippage along a gliding plane, caused by the motion of an edge dislocation, schematically. Left hand: the dislocation has been formed at the crystal edge on the left. Middle: the dislocation has reached the middle of the crystal. Right hand: the dislocation has left the crystal at the edge on the right, and has left behind a slippage step. (U. Essmann)

plane have been displaced by one atomic distance against the other. Therefore, a dislocation line cannot terminate somewhere in the middle of the crystal, and, instead, it must extend until it reaches the crystal surface, or at least it must form a closed ring. All of our discussions up to this point refers to the relatively simple case of the “edge dislocations”. However, there also exist other types of dislocations, which need a more complicated description, and which will not be discussed further here. The concept of dislocation provided the key mechanism for clarifying our understanding of the mechanical properties of crystals. At this point we recall our discussion in Sect. 8.6 of the other example where the motion of another type of defect, namely individual magnetic flux quanta, results in the key mechanism for the destruction of superconductivity and the appearance of electrical resistance. The ﬁrst direct experimental evidence for the crystal dislocations by means of their observation in an electron microscope was accomplished in the year 1956 at the Batelle Institute in Geneva and also at the Cavendish Laboratory in Cambridge. At the time, it was a particular highlight, when even the motion of dislocations could be followed in the electron microscope. The distortion of the crystal lattice near the dislocation line results in mechanical stresses in this region of the material. The stress ﬁeld associated with each dislocation extends up to a relatively long distance, and by means of the stress ﬁelds an interaction arises between the dislocations. As the deformation of the crystal progresses, the number of dislocations increases. However, during this process, among the dislocations a mutual blocking effect sets in, such that the force necessary for further deformation increases. The crystal becomes mechanically stronger and harder, until it eventually breaks. The same increase in mechanical strength is achieved during the cold-working of metals, i.e., by forging, rolling, or bending. Hence, it was found essentially, that the same defect in the crystal lattice, which causes the highly useful ductility of metals, also leads to the development of their hardness during cold-working (Fig. 12.6).

224

12

Defects in the Crystal Lattice: Useful or Harmful?

bottom

top (0006)

400nm

Fig. 12.6 Two-beam image showing several parallel edge dislocations in hexagonal BaTiO3 ceramics. The dislocations were imaged by diffraction contrast in a transmission electron microscope. Bragg diffracting planes are bent due to the strain ﬁeld of the dislocations yielding a contrast along the dislocation line. Right: sketch of a dislocation penetrating the TEM foil (about 100 nm thick) from top to bottom. (O. Eibl)

In metals, permanently changing mechanical loads are particularly harmful. There is the possibility of metal fatigue, which eventually leads to “fatigue fracture”. We all know the phenomenon, i.e., that a metal wire can break, if one bends it back and forth often enough. Changing mechanical loads appear very frequently in technical equipment. As long as the load stays precisely within the elastic regime of the material, it is still harmless. However, the situation becomes critical if tiny plastic deformations start to develop, such that dislocations move back and forth within the crystal lattice. Eventually, a collection of many dislocations can lead to the seed of microcracks, representing the ﬁrst stage of fatigue fracture. Here the details are highly complex, and even today they are the subject of further research. It appears that a similar scenario has led to the terrible accident of the Intercity Express Train on June 3, 1998 near Eschede north of Hannover in Germany, with many people killed or severely injured. At the time, the train ICE 884 “Wilhelm Conrad Röntgen”, running between Munich and Hamburg-Altona, was involved. A hidden crack at the inner side of a metal tire eventually resulted in fatigue fracture of the tire. The tire was then caught in a switch, which considerably enhanced the disaster. The involved tire had been in operation since 1994, and it had run 1.8 million kilometers until the day of the accident. However, during these four years it was not exactly and carefully checked one single time.

12.6

12.6

Materials Testing

225

Materials Testing

The accident we have just discussed raises the question of the early detection of defects in materials or of perhaps already developed microcracks or damages due to corrosion. The technical equipment required for this purpose has been available for many years, and it is being continuously improved. In the meantime, “nondestructive materials testing”; has become an important and unavoidable technical subﬁeld. In addition to the inspection of the raw materials of the iron and steel industry, important ﬁelds for the application of testing methods exist, for example, in armored pre-stressed concrete, in certain parts of airplanes such as wheels, fuselage, and wings, or in the under-water steel construction of derricks for oil. In the materials testing of metals a highly prominent role is played by the eddy-current method. In this method an electric high-frequency alternating current is locally induced in the test sample by means of a high-frequency coil, and simultaneously the electrical resistance behavior at this location of the test piece is determined. In this way, even very small microcracks in the interior of the material can be detected. Because of his pioneering research and development in this ﬁeld over many years, which he had started in the 1930s, the German Friedrich Förster gained worldwide fame. During recent years, also the SQUID, based on the Josephson effect and on the magnetic flux quantization in superconductors, has become increasingly important for the nondestructive materials testing and in particular also for the detection of microcracks and foreign inclusions. Having the highest sensitivity of all sensors of magnetic ﬁelds, SQUIDs are used for the detection of local anomalies in the magnetic or the electromagnetic stray ﬁeld. Initially, the SQUIDs were fabricated from classical superconductors, and usually they had to be cooled down to only a few Kelvin using liquid helium. However, for a few years, SQUIDs made from high-temperature superconductors have also been available, which need to be cooled only to about 80 K, for example, with liquid nitrogen. Compared with the traditional electric eddy-current method, discussed above, the SQUID sensors are much more sensitive, in particular for the detection of defects which are located more deeply within the material. Recently, a routine evaluation at the wheel-testing facility of the German Lufthansa Airline at the Airport of Frankfurt, yielded promising results. Using another example we wish to illustrate the importance of materials testing, in particular for constructions made of steel: i.e., the shipwreck of the Titanic during April 1912. Even today this marine catastrophe is a frequently-discussed dramatic subject. In 2012, exactly 100 years after the accident, it received very much attention. The physicist Uwe Essmann, working at the Max Planck Institute for Metals Research in Stuttgart, has impressively summarized this case in an essay entitled “Metals: From Stone Age Ornaments To Jet Turbine Engines”, where he refers to an article in the International Herald Tribune from February 19, 1998. In the following we quote his summary:

226

12

Defects in the Crystal Lattice: Useful or Harmful?

On her maiden voyage, on April 14, 1912 shortly before midnight, the Titanic collided with an iceberg, and on April 15 at 2:20 a.m. she sank. In 1985 the wreck was discovered by the oceanographer Robert Ballard off Newfoundland at a depth of 3650 meters. In 1910, the hull had been assembled from steel sheets of about 2.5 cm thickness at a shipyard in Belfast, using approximately three million forged-iron rivets. By means of special robots, steel sheets from the hull and some rivets could be recovered, and it is expected that, during expeditions to the wreck in the future, additional circumstantial evidence about the course of the collision with the iceberg can be found. A group of ship-building engineers and metallurgists associated with William Garzke, Chairman of the Commision on Damages of the Society of Naval Architects and Marine Engineers, is interested in the metallurgical questions arising in this case. Following a maneuver with the rudder, the Titanic hit the iceberg at its starboard side. Up to now it had been assumed that, because of this collision, a longitudinal rupture appeared across several bulkheads, which eventually resulted in the shipwreck. However, in the year 1996 investigations of the wreck with a special sonar instrument could not conﬁrm this expectation. Instead, six lateral openings were found in the hull, which apparently were caused by blows as the Titanic scratched along the iceberg. With the engineers involved in this case this observation raised the suspicion that, at the openings, the rivet seams between neighboring steel sheets had burst. Then at the (American) National Institute of Standards and Technology in Gaithersburg, Maryland, Tim Foecke started a metallurgical inspection of the salvaged rivets. By means of a diamond saw, one rivet was parted along its length, and its inner texture was studied with a metallurgical microscope. Forged iron does not consist of pure iron, but normally it contains about 2% of slag ﬁbers, which result from slag inclusions during forging, and which are well recognized within the texture. The slag ﬁbers improve the fatigue and the corrosion properties of the material. However, its volume fraction must not exceed 2% by much, since otherwise the mechanical strength of the rivets deteriorates. In the inspected rivet the slag content was 9%, which cannot be tolerated. If initially only a few weak rivets have given in, a seam could rupture further like in textiles, leading to a fatal influx of water. It remains to be seen, if this suspicion will be conﬁrmed. If so, it would not change anything directly relating to the collision with the iceberg. However, if the seams between the hull sheets would have been intact, perhaps only small leaks would have appeared, which could have been handled by the bilge-pumps of the Titanic.

In 2008, together with Jennifer Hooper McCarthy, Tim Foecke published the book What really sank the Titanic—New Forensic Discoveries, in which they reported on the materials research for nearly 10 years, dealing with the objects recovered from the Titanic and particularly with the poor quality of the rivets.

12.7

Magnetic Impurities, Kondo Effect

As we have discussed in Sect. 5.4, in the limit of low temperatures the (nearly temperature independent) residual electric resistance of a metal is due electron scattering by structural lattice defects and chemical impurities. However, already in 1930 Walther Meissner and B. Voigt noted that in certain metals at low temperatures the electric resistivity displayed a minimum and then increased again by a few per cent with decreasing temperature. Subsequently, this resistance minimum was

12.7

Magnetic Impurities, Kondo Effect

227

investigated more closely by G. J. van den Berg and coworkers. The same anomaly was observed in different metals containing a small amount of magnetic impurities (Co in Cu, for example). Although the subject was studied by an increasing number of people, it remained an unexplained mystery. Then in 1964 the Japanese Jun Kondo entered the scene and proposed a theoretical explanation based on the scattering of electrons by magnetic impurities, which is referred to since as the Kondo effect. When Kondo considered the scattering from a magnetic ion that interacts with the spins of the conduction electrons, he made a surprising discovery. He found that one contribution in his calculation can be much larger than expected, and that the resistance of a metal can increase logarithmically at low temperatures with decreasing temperature. Qualitatively, these results can be understood as follows. We start with the simplest model of a magnetic impurity introduced by Philip W. Anderson in 1961: There exists only one electronic level with energy eo below the Fermi energy occupied by an electron with its spin of ½ pointing up (Fig. 12.7a). Quantum-mechanically, the electron can tunnel from the impurity and escape, provided its energy lies above the Fermi energy eF of the surrounding Fermi sea of the conduction electrons. Otherwise the electron remains trapped because all states are occupied.

Fig. 12.7 The Anderson model describes a magnetic impurity in terms of one electronic energy level with energy eo below the Fermi energy occupied by an electron. Coulomb repulsion prohibits the presence of a second electron at this energy. In part a the potential well associated with the impurity and the Fermi sea outside the potential barrier around it is schematically indicated. Part a illustrates the quantum mechanical exchange process during which a spin-up electron escapes from the impurity by tunneling and reaches an unoccupied energy level above the Fermi energy. Simultaneously, an electron with the opposite spin from the Fermi sea tunnels back to the impurity site. Energetically, this exchange process becomes possible because of the Heisenberg uncertainty relation, allowing the passage through a virtual transient state during a very short time. Part b shows the appearance of a sharp peak in the density of states at the Fermi energy due to the presence of many magnetic impurities. Г is the width of the energy level of the impurity, which is broadened by the short lifetime due to the electron tunneling

228

12

Defects in the Crystal Lattice: Useful or Harmful?

However, quantum mechanics allows “exchange processes”, which can flip the spin of the impurity from spin up to spin down, or reverse, while simultaneously creating a spin excitation in the surrounding Fermi sea. In Fig. 12.7a we illustrate the removal of an electron from the localized impurity state and its placement into an unoccupied energy state at the surface of the Fermi sea. Classically, such a process needs an energy input of about 1–10 eV in the case of magnetic impurities. However, quantum mechanics allows such a process in form of the passage through a virtual transient state during a very short time s because of the Heisenberg uncertainty principle. This time s is given by s ¼ h/jeo j

ð12:8Þ

where h is Planck’s constant. Within this time s another electron must tunnel from the Fermi sea back to the impurity. However, the spin of this electron will point in the opposite direction than before, and a spin-flip process had occurred. Theoretically, in this case we deal again with a quantum mechanical exchange interaction. (In Sects. 10.3–10.5 we discussed the prominent role of such interaction in the case of magnetism). If the concentration of the magnetic impurities in the crystal is sufﬁciently small, the individual magnetic defects can be treated independently, and interference effects between them can be neglected. This spin-exchange interaction qualitatively changes the energy spectrum of the system. The presence of many magnetic impurities results in a sharp peak in the density of states (“Kondo resonance”) at the Fermi energy (Fig. 12.7b). This peak provides much additional phase space for the scattering of electrons and, hence, strongly affects the electric resistance at low temperatures. It turns out, that below the “Kondo temperature” the electric resistance increases logarithmically with decreasing temperature. Typically, the Kondo temperature can vary between 1 and 100 K. The strong energy dependence of the density of states near the Fermi energy, seen in Fig. 12.7b, also leads to a large value of the thermoelectric power (“giant thermo-power”) at low temperatures.

Nobel Prizes in Physics Closely Connected with the Physics of Solids

1901 1909 1913

1914 1915 1918 1920

1921 1923 1924 1926 1928 1929

Wilhelm Conrad Röntgen, Munich, for the discovery of the remarkable rays subsequently named after him Guglielmo Marconi, London, and Ferdinand Braun, Strassburg, for their contributions to the development of wireless telegraphy Heike Kamerlingh Onnes, Leiden, for his investigations on the properties of matter at low temperatures which lead, inter alia, to the production of liquid helium Max von Laue, Frankfort/Main, for his discovery of the diffraction of X-rays by crystals William Henry Bragg, London, and William Lawrence Bragg, Manchester, for their analysis of crystal structure by means of X-rays Max Planck, Berlin, in recognition of the services he rendered to the advancement of Physics by his discovery of energy quanta Charles Edouard Guillaume, Sèvres, in recognition of the service he has rendered to precise measurements in Physics by his discovery of anomalies in nickel steel alloys Albert Einstein, Berlin, for services to Theoretical Physics, and especially for his discovery of the law of the photoelectric effect Robert Andrews Millikan, Pasadena, California, for his work on the elementary charge of electricity and on the photo-electric effect Manne Siegbahn, Uppsala, for his discoveries and researches in the ﬁeld of X-ray spectroscopy Jean Baptiste Perrin, Paris, for his work on the discontinuous structure of matter, and especially for his discovery of sedimentation equilibrium Owen Willans Richardson, London, for his work on the thermionic phenomenon and especially for his discovery of the law named after him Louis Victor de Broglie, Paris, for his discovery of the wave nature of electrons

© Springer Nature Switzerland AG 2019 R. P. Huebener, Conductors, Semiconductors, Superconductors, Undergraduate Lecture Notes in Physics, https://doi.org/10.1007/978-3-030-31420-0

229

230

1930 1932

1933 1937

1945 1946

1952

1954 1956

1961

1962 1965

1970

1972

1973

Nobel Prizes in Physics Closely Connected with the Physics of Solids

Venkata Raman, Calcutta, for his work on the scattering of light and for the discovery of the effect named after him Werner Heisenberg, Leipzig, for the creation of quantum mechanics, the application of which has, inter alia, led to the discovery of the allotropic forms of hydrogen Erwin Schrödinger, Berlin, and Paul Adrien Maurice Dirac, Cambridge, for the discovery of new productive forms of atomic theory Clinton Joseph Davisson, New York, N. Y., and George Paget Thomson, London, for their experimental discovery of the diffraction of electrons by crystals Wolfgang Pauli, Zurich, for the discovery of the Exclusion Principle, also called the Pauli Principle Percy Williams Bridgman, Harvard University, Massachusetts, for the invention of an apparatus to produce extremely high pressures and for discoveries he made in the ﬁeld of high pressure physics Felix Bloch, Stanford University, California, and Edward Mills Purcell, Harvard University, Massachusetts, for the development of new methods for nuclear magnetic precision measurements and the discoveries in connection therewith Max Born, Edinburgh, for his fundamental research in quantum mechanics, especially for his statistical interpretation of the wave-function William Shockley, Pasadena, California, John Bardeen, Urbana, Illinois, and Walter Houser Brattain, Murray Hill, New Jersey, for their investigations on semiconductors and their discovery of the transistor effect Rudolf Ludwig Mössbauer, Munich, for his researches concerning the resonance absorption of gamma radiation and his discovery in this connection of the effect which bears his name Lew Dawidowitsch Landau, Moscow, for his pioneering theories for condensed matter, especially liquid helium Sin-itiro Tomonaga, Tokyo, Julian Seymour Schwinger, Cambridge, Massachusetts, and Richard Phillips Feynman, Pasadena, California, for their fundamental work in quantum electrodynamics, with deep-ploughing consequences for the physics of elementary particles Louis Eugène Felix Néel, Grenoble, for fundamental work and discoveries concerning antiferromagnetism and ferromagnetism which have led to important applications in solid state physics John Bardeen, Urbana, Illinois, Leon Neil Cooper, Providence, Rhode Island, and John Robert Schrieffer, Philadelphia, Pennsylvania, for their theory of superconductivity, usually called the BCS-theory Leo Esaki, Yorktown Heights, New York, and Ivar Giaever, Schenectady, New York, one half for their experimental discoveries regarding tunneling phenomena in semiconductors and superconductors, respectively, and with the other half to Brian David Josephson, Cambridge, U.K., for his theoretical predictions of the properties of a supercurrent through a tunnel

Nobel Prizes in Physics Closely Connected with the Physics of Solids

1977

1978 1981 1982 1985 1986

1987

1991

1994

1996

1998

2000

2003

2007

231

barrier, in particular those phenomena which are generally known as the Josephson effects Philip Warren Anderson, Murray Hill, New Jersey, Nevill Francis Mott, Cambridge, U. K., and John Hasbrouck Van Vleck, Cambridge, Massachusetts, for their fundamental theoretical investigations of the electronic structure of magnetic and disordered systems Pyotr Leonidovich Kapitza, Moscow, for his basic inventions and discoveries in the area of low-temperature physics Kai Manne Siegbahn, Uppsala, for his contribution to the development of high-resolution electron spectroscopy Kenneth Geddes Wilson, Cornell University, New York, for his theory of critical phenomena in connection with phase transitions Klaus von Klitzing, Stuttgart, for the discovery of the quantized Hall effect Ernst Ruska, Berlin, for his fundamental work in electron optics and for the design of the ﬁrst electron microscope, and the other half jointly to Gerd Binnig and Heinrich Rohrer, Zurich, for their design of the scanning tunneling microscope Johannes Georg Bednorz and Karl Alexander Müller, Zurich, for their important breakthrough in the discovery of superconductivity in ceramic materials Pierre-Gilles de Gennes, Paris, for discovering that methods developed for studying order phenomena in simple systems can be generalized to more complex forms of matter, in particular to liquid crystals and polymers Bertram Neville Brockhouse, McMaster University, Hamilton, Ontario, for the development of neutron spectroscopy, and to Clifford Glenwood Shull, Massachusetts Institute of Technology, Cambridge, Massachusetts, for the development of the neutron diffraction technique David Morris Lee, Cornell University, New York, Douglas Dean Osheroff, Stanford University, California, and Robert Coleman Richardson, Cornell University, New York, for their discovery of superfluidity in helium-3 Robert Betts Laughlin, Stanford University, California, Horst Ludwig Störmer, Columbia University, New York, and Daniel Chee Tsui, Princeton University, New Jersey, for their discovery of a new form of quantum fluid with fractionally charged excitations Zhores Ivanovich Alferov, St. Petersburg, Herbert Kroemer, Santa Barbara, California, and Jack St. Clair Kilby, Dallas, Texas, for basic work on information and communication technology, in particular for developing semiconductor hetero-structures used in high-speed- and opto-electronics, and for the invention of the integrated circuit Alexei Alexeyevich Abrikosov, Argonne, Illinois, Vitaly Lazarevich Ginzburg, Moscow, and Anthony James Leggett, Urbana, Illinois, for their pioneering contributions to the theory of superconductors and superfluids Albert Louis Francois Fert, Paris, and Peter Grünberg, Jülich, for the discovery of giant magneto-resistance

232

2009

2010

2012

2014

2016

Nobel Prizes in Physics Closely Connected with the Physics of Solids

Willard S. Boyle, Charles Kuen Kao, and George Elwood Smith, Bell Laboratories, Murray Hill, New Jersey, for the invention of an imaging semiconductor circuit—the CCD sensor Andre Geim and Konstantin Novoselov, Manchester, U.K., for discovering and isolating a single free-standing atomic layer of carbon (graphene) and elucidating its remarkable electronic properties Serge Haroche, Collège de France and Ecole Normale Supérieure, Paris, France, and David J. Wineland, National Institute of Standards and Technology and University of Colorado, Boulder, CO, USA, for ground-breaking experimental methods that enable measuring and manipulation of individual quantum systems Isamu Akasaki, Meijo University, Nagoya and Nagoya University, Japan, Hiroshi Amano, Nagoya University, Japan, and Shuji Nakamura, University of California, Santa Barbara, CA, USA, for the invention of efﬁcient blue light-emitting diodes which has enabled bright and energy-saving white light sources David J. Thouless, University of Washington, Seattle, USA, J. Michael Kosterlitz, Brown University, Providence, USA, and F. Duncan M. Haldane, Princeton University, Princeton, USA, for theoretical discoveries of topological phase transitions and topological phases of materials

Nobel Prizes in Chemistry Closely Connected with the Physics of Solids

1920 1936

1949

1954

1966

1968

1977 1985

1988

1991

1996

Walther Nernst, Berlin, in recognition of his work in thermochemistry Peter Debye, Berlin-Dahlem, for his contributions to our knowledge of molecular structure through his investigations on dipole moments and on the diffraction of X-rays and electrons in gases William Francis Giauque, Berkeley, California, for his contributions in the ﬁeld of chemical thermodynamics, particularly concerning the behaviour of substances at extremely low temperatures Linus Carl Pauling, Pasadena, California, for his research into the nature of the chemical bond and its application to the elucidation of the structure of complex substances Robert Sanderson Mulliken, Chicago, Illinois, for his fundamental work concerning chemical bonds and the electronic structure of molecules by the molecular orbital method Lars Onsager, New Haven, Connecticut, for the discovery of the reciprocity relations bearing his name, which are fundamental for the thermodynamics of irreversible processes Ilya Prigogine, Brussels, for his contribution to non-equilibrium thermodynamics, particularly the theory of dissipative structures Herbert Aaron Hauptman, Buffalo, New York, and Jerome Karle, Washington, DC, for their outstanding achievements in the development of direct methods for the determination of crystal structures Johann Deisenhofer, Dallas, Texas, Robert Huber, Martinsried, and Hartmut Michel, Frankfort/Main, for the determination of the three-dimensional structure of a photosynthetic reaction centre Richard Robert Ernst, Zurich, for his contributions to the development of the methodology of high resolution nuclear magnetic resonance (NMR) spectroscopy Robert Floyd Curl, Jr., Rice University, Houston, Texas, Harold Walter Kroto, University of Sussex, and Richard Errett Smalley, Rice University, for their discovery of fullerenes

© Springer Nature Switzerland AG 2019 R. P. Huebener, Conductors, Semiconductors, Superconductors, Undergraduate Lecture Notes in Physics, https://doi.org/10.1007/978-3-030-31420-0

233

234

1998

2000

2007 2011 2014

2016

Nobel Prizes in Chemistry Closely Connected with the Physics of Solids

Walter Kohn, Santa Barbara, California, for his development of the density-functional theory, and John Anthony Pople, Northwestern University, Evanston, Illinois, for his development of computational methods in quantum chemistry Alan Jay Heeger, Santa Barbara, California, Alan Graham MacDiarmid, Philadelphia, Pennsylvania, and Hideki Shirakawa, Tsukuba, for the discovery and development of conductive polymers Gerhard Ertl, Fritz-Haber Institut, Berlin, for his studies of chemical processes at solid surfaces Daniel Shechtman, Technion, Haifa, for the discovery of quasi-crystals Eric Betzig, Howard Hughes Medical Institute, Ashburn, VA, USA, Stefan W. Hell, Max Planck Institute for Biophysical Chemistry, Göttingen, and German Cancer Research Center, Heidelberg, Germany, and William E. Moerner, Stanford University, Stanford, CA, USA, for the development of super-resolved fluorescence Microscopy Jean-Pierre Sauvage, University of Straßburg, J, Fraser Stoddart, Northwestern University, Evanston, USA, and Bernard L. Feringa, University of Groningen, for the development of molecular machines

Bibliography

General Solid State Physics N.W. Ashcroft, N.D. Mermin, Solid State Physics (Holt, Rinehart and Winston, New York, 1976) L. Hoddeson, E. Braun, J. Teichmann, S. Weart (eds.), Out of the Crystal Maze: Chapters from the History of Solid State Physics (Oxford University Press, London, 1992) Ch. Kittel, Introduction to Solid State Physics, 4th edn. (Wiley, New York, 1971)

Solid State Theory A.A. Abrikosov, Fundamentals of the Theory of Metals (North-Holland, Amsterdam, 1988) J. Callaway, Quantum Theory of the Solid State, 2 volumes (Academic Press, New York, 1974) H. Haken, Quantum Field Theory of Solids (North Holland Publ. Co., Amsterdam and New York, 1976) W.A. Harrison, Solid State Theory (McGraw-Hill, New York, 1969) O. Madelung, Introduction to Solid State Theory (Springer, Berlin, 1978) R.M. Martin, Electronic Structure—Basic Theory and Practical Methods (Cambridge University Press, Cambridge, UK, 2004) N.F. Mott, H. Jones, The Theory of the Properties of Metals and Alloys (Dover Publications, New York, 1958) R.E. Peierls, Quantum Theory of Solids (Oxford University Press, London, 1965) F. Seitz, The Modern Theory of Solids (Mc-Graw Hill, New York, 1940) A.H. Wilson, The Theory of Metals (Cambridge University Press, London, 1965) J.M. Ziman, Electrons and Phonons (Oxford University Press, London, 1960) J.M. Ziman, Principles of the Theory of Solids (Cambridge University Press, 1972)

Semiconductors G. Allan, G. Bastard, N. Boccara, M. Lanoo, M. Voos (eds.), Heterojunctions and Semiconductor Superlattices (Springer, Berlin, 1986) V.L. Bonch-Bruyevich, The Electronic Theory of Heavily Doped Semiconductors (American Elsevier Publ, New York, 1966) K. Seeger, Semiconductor Physics, 8th edn. (Springer, Berlin, 2002) B. Shklovskii, A.L. Efros, Electronic Properties of Doped Semiconductors (Springer, Berlin, 1984) E. Spenke, Electronic Semiconductors (McGraw-Hill, New York, 1958) © Springer Nature Switzerland AG 2019 R. P. Huebener, Conductors, Semiconductors, Superconductors, Undergraduate Lecture Notes in Physics, https://doi.org/10.1007/978-3-030-31420-0

235

236

Bibliography

S.M. Sze, Physics of Semiconductor Devices, 2nd edn. (Wiley, New York, 1969) W. Tom Wenckebach, Essentials of Semiconductor Physics (Wiley, Chichester, 1999)

Superconductivity K.H. Bennemann, J.B. Ketterson (eds.), The Physics of Superconductors, 2 volumes (Springer, Berlin, 2003) W. Buckel, R. Kleiner, Superconductivity—Fundamentals and Applications, 2nd edn. (Wiley-VCH Verlag, Weinheim, 2004) P.F. Dahl, Superconductivity—Its Historical Roots and Development from Mercury to the Ceramic Oxides (American Institute of Physics, New York, 1992) P.G. De Gennes, Superconductivity of Metals and Alloys (W. A. Benjamin, New York, 1966) R.P. Huebener, Magnetic Flux Structures in Superconductors, 2nd edn. (Springer, Berlin, 2001) J.B. Ketterson, S.N. Song, Superconductivity (Cambridge University Press, Cambridge, 1999) E.A. Lynton, Superconductivity (Methuen & Co, London, 1962) J. Matricon, G. Waysand, The Cold Wars: A History of Superconductivity (Rutgers University Press, New Brunswick, 2003) R.D. Parks (ed.), Superconductivity, 2 volumes (Marcel Dekker, New York, 1969) ChP Poole Jr., H.A. Farach, R.J. Creswick, Superconductivity (Academic Press, New York, 1995) R. Rickayzen, Theory of Superconductivity (Wiley, New York, 1965) M. Tinkham, Introduction to Superconductivity, 2nd edn. (McGraw-Hill, New York, 1996) J.R. Waldram, Superconductivity of Metals and Cuprates (Institute of Physics Publishing, Bristol, 1996)

Magnetism A.S. Chakravarty, Introduction to the Magnetic Properties of Solids (Wiley, New York, 1980) S. Chikazumi, Physics of Magnetism (Wiley, New York, 1964) S. Chikazumi, Physics of Ferromagnetism, 2nd edn. (Oxford University Press, Oxford, 1997) J. Crangle, The Magnetic Properties of Solids (Arnold, London, 1977) A.H. Morrish, The Physical Principles of Magnetism (Wiley, New York, 1965) R.M. White, Quantum Theory of Magnetism (McGraw-Hill, New York, 1970)

Special Subjects R.D. Barnard, Thermoelectricity in Metals and Alloys (Taylor & Francis, London, 1972) M. Born, K.H. Huang, Dynamical Theory of Crystal Lattices (Oxford University Press, Oxford, 1954) J.H. Davies, The Physics of Low-Dimensional Semiconductors—An Introduction (Cambridge University Press, Cambridge, 1998) J. Hooper McCarty, T. Foecke, What Really Sank the Titanic (Citadel Press Book, 2008) K. von Klitzing, Quantum Hall Effect: discovery and application. Annu. Rev. Condens. Matter Phys. 13 (2017) D.K.C. MacDonald, Thermoelectricity—An Introduction to the Principles (Wiley, New York, 1962) A.A. Maradudin, E.W. Montroll, G.H. Weiss, Theory of Lattice Dynamics in the Harmonic Approximation (Academic Press, New York, 1971) R.E. Prange, S.M. Girvin (eds.), The Quantum Hall Effect, 2nd edn. (Springer, New York, 1990)

Bibliography

237

A.M. Stoneham, Theory of Defects in Solids—Electronic Structure and Defects in Insulators and Semiconductors (Oxford University Press, Oxford, 1975) P.T. Townsend, J.C. Kelly, Color Centers and Imperfections in Insulators and Semiconductors (Crane & Russack, New York, 1973) R. Waser (ed.), Nanoelectronics and Information Technology (Wiley-VCH, Weinheim, 2003)

Author Index

A Abrikosov, Alexei Alexeyevich, 129, 231 Abstreiter, Gerhard, 112 Aharonov, Yakir, 210 Akasaki, Isamu, 232 Akimitsu, Jun, 164 Alferov, Zhores Ivanovich, 231 Amano, Hiroshi, 232 Anderson, Philip Warren, 137, 141, 227, 231 B Ballard, Robert, 226 Ballufﬁ, Robert W., 215 Bardeen, John, 4, 78, 135, 230 Barkhausen, Heinrich, 178 Becker, Richard, 221 Bednorz, Johannes Georg, 151, 231 Bethe, Hans, 72 Betzig, Eric, 234 Binnig, Gerd, 11, 231 Bitter, Francis, 115, 131, 178, 182 Bloch, Felix, 49–51, 64, 137, 139, 178, 179, 181, 230 Bohm, David, 210 Bohr, Niels, 137 Born, Max, 230 Bose, Satyendra Nath, 40 Boyle, Willard S., 232 Bragg, William Henry, 1, 22, 229 Bragg, William Lawrence, 1, 22, 229 Brattain, Walter Houser, 4, 78, 230 Braun, Ferdinand, 73, 74, 82, 229 Bravais, Auguste, 16

Bridgman, Percy Williams, 230 Brillouin, Léon, 72, 137, 171 Brockhouse, Bertram Neville, 43, 231 C Casimir, Hendrik Brugt Gerhard, 122 Chaudhari, Praveen, 161 Chu, Paul Ching-Wu, 152 Clusius, Klaus, 70 Conrad Röntgen, Wilhelm, 18 Cooper, Leon Neil, 135, 230 Cotton, Aimé, 115 Crick, Francis Harry Compton, 27 Curie, Marie, 171 Curie, Pierre, 171 Curl, Robert Floyd, 201, 233 D Davisson, Clinton Joseph, 10, 230 Deaver, Bascom, 131 de Broglie, Louis Victor, 10, 229 Debye, Peter, 5, 26, 39, 43, 233 de Gennes, Pierre-Gilles, 231 de Haas, Wander Johannes, 103 Deisenhofer, Johann, 27, 233 Devoret, Michel H., 200 Dingle, Raymond, 112 Dirac, Paul Adrien Maurice, 49, 62, 169 Doll, Robert, 131 Döhler, Gottfried H., 194 Dorsman, Cornelis, 118 Drude, Paul, 59 Dulong, Pierre Louis, 35

© Springer Nature Switzerland AG 2019 R. P. Huebener, Conductors, Semiconductors, Superconductors, Undergraduate Lecture Notes in Physics, https://doi.org/10.1007/978-3-030-31420-0

239

240 E Einstein, Albert, 36–38, 40, 140, 219, 229 Ernst, Richard Robert, 233 Er-Rakho, L., 153 Ertl, Gerhard, 234 Esaki, Leo, 190, 230 Essmann, Uwe, 131, 225 Esteve, D., 200 Euler, Leonhard, 201 Ewald, Paul Peter, 18 F Fairbank, William, 131 Faraday, Michael, 73, 97 Feringa, Bernard L., 234 Fermi, Enrico, 62, 141 Fert, Albert, 184, 231 Feynman, Richard Phillips, 129, 138, 189, 230 Foecke, Tim, 226 Förster, Friedrich, 225 Franklin, Rosalind, 27, 189 Frenkel, Jakov Iljitsch, 137, 218 Friedrich, Walter, 19 Fu, Liang, 208 Fuller, Buckminster, 201 G Garzke, William, 226 Geballe, Theodore, 141 Geim, Andre, 204, 232 Germer, Lester, 10 Giaever, Ivar, 136, 230 Giauque, William Francis, 5, 233 Gibbs, Josiah Willard, 23, 214 Ginzburg, Vitaly Lazarevich, 127, 130, 231 Gorter, Cornelis Jacobus, 5, 122 Gossard, Arthur C., 112 Grünberg, Peter, 184, 231 Guillaume, Charles Edouard, 229 H Hahn, Otto, 152, 219 Haldane, F. Duncan M., 232 Hall, Edwin Herbert, 98 Haroche, Serge, 232 Hauptman, Herbert Aaron, 233 Heeger, Alan Jay, 234 Heisenberg, Werner, 49, 50, 75, 137, 175, 179, 228, 230 Heitler, Walter Heinrich, 33 Hell, Stefan W., 234 Holborn, Ludwig, 36 Holm, Ragnar, 141 Holst, Gilles, 118

Author Index Hooke, Robert, 220 Hosono, Hideo, 165 Huber, Robert, 27, 233 Huffman, Donald R., 201 Hulm, John, 141 I Iijima, Sumio, 202 Ioffe, Abram Fedorovich, 94, 115, 217 Ittner, W. B., 126 J Jones, H., 72 Jordan, Pascual, 136 Josephson, Brian David, 137, 141, 230 K Kane, Charles L., 208 Kao, Charles Kuen, 232 Kapitza, Pyotr Leonidovich, 115, 231 Karle, Jerome, 233 Kawaji, S., 111 Kelly, Mervin, 3 Kilby, Jack St. Clair, 231 Kim, Young, 141 Kleiner, Reinhold, 163 Knipping, Paul, 19 Knoll, Max, 9, 10 Kohn, Walter, 234 Kondo, Jun, 227 Kosterlitz, J. Michael, 232 Krätschmer, Walter, 201 Kroemer, Herbert, 90, 231 Kronig, Ralph, 137 Kroto, Harold Walter, 201, 233 Kunzler, Gene, 141 Kurti, Nicholas, 5, 6 L Landauer, Rolf, 196 Landau, Lew Dawidowitsch, 101, 116, 127, 129, 137, 170, 230 Landwehr, Gottfried, 108 Langevin, Paul, 170, 171 Laughlin, Robert Betts, 114, 231 Lee, David Morris, 231 Leggett, Anthony James, 130, 231 Lifshitz, Ilya Mikhailovich, 105 Lilienfeld, Julius Edgar, 89 Lindemann, Frederick Alexander, 6 London, Fritz, 6, 7, 33, 124, 125 London, Heinz, 6, 7, 124, 125 Lorentz, Hendrik Antoon, 59, 98 Lummer, Otto, 36

Author Index M Madelung, Erwin Rudolf, 32 Maier-Leibnitz, Heinz, 8, 43 Mannhart, Jochen, 161 Mann, Thomas, 18 Marconi, Guglielmo, 73, 229 Mark, Hermann Francis, 220 Martens, Adolf, 213 Matthias, Bernd, 141 Maurice, Paul Adrien, 230 Maxwell, James Clerk, 97 McCarthy, Jennifer Hooper, 226 McLennan, John C., 121 Meissner, Walther, 120, 121, 141, 226 Mendelssohn, Kurt, 6 Michel, C., 153 Michel, Hartmut, 27, 233 Millikan, Robert Andrews, 229 Moerner, William E., 234 Molenkamp, Laurens W., 208 Möllenstedt, Gottfried, 211 Moore, Gordon E., 92 Mössbauer, Rudolf Ludwig, 43, 226, 230 Mott, Nevill Francis, 72, 218, 222, 231 Müller, Karl Alexander, 151, 231 Müller, Paul, 163 Mulliken, Robert Sanderson, 233 N Näbauer, Martin, 131 Néel, Louis Eugene Felix, 171, 181 Nakamura, Shuji, 90, 232 Nernst, Walther, 40, 233 NingYang, Chen, 139 Novoselov, Konstantin, 204, 232 O Ochsenfeld, Robert, 120 Ohl, Russell Shoemaker, 85, 89 Onnes, Heike Kamerlingh, 4, 117, 118, 229 Onsager, Lars, 66, 72, 103, 233 Orowan, Egon, 221 Osheroff, Douglas Dean, 231 P Pauling, Linus Carl, 33, 233 Pauli, Wolfgang, 62, 64, 137, 169, 174, 175, 230 Peierls, Rudolf E., 45, 50, 55, 64, 80, 103 Peltier, Jean Charles Athanase, 68 Penrose, Roger, 28 Perrin, Jean Baptiste, 229 Perutz, Max, 27 Petit, Alexis Thérèse, 35

241 Pippard, Alfred Brian, 65, 127, 137 Planck, Max, 36–38, 229 Ploog, Klaus, 112, 195 Pohl, Robert Wichard, 218 Polanyi, Michael, 220, 221 Pople, John Anthony, 234 Pound, Robert V., 44 Prigogine, Ilya, 233 Pringsheim, Ernst, 36 Purcell, Edward Mills, 230 Q Quinn, D. J., 126 R Raman, Venkata, 230 Raveau, B., 153 Rebka, Glen A., 44 Richardson, Owen Willans, 229 Richardson, Robert Coleman, 231 Rohrer, Heinrich, 11, 231 Röntgen, Wilhelm Conrad, 1, 18, 19, 26, 94, 152, 229 Roosevelt, Franklin Delano, 219 Rowland, Henry A., 97 Rubens, Heinrich, 36 Ruska, Ernst, 9, 231 Rutherford, Ernest, 115 S Sauvage, Jean-Pierre, 234 Scheer, Elke, 200 Scherrer, Paul, 26 Schmid, E., 220 Schottky, Walter, 80, 82 Schrieffer, Robert, 135, 230 Schrödinger, Erwin, 49, 230 Schwinger, Julian Seymour, 230 Seebeck, Thomas Johann, 69 Seitz, Frederick, 4, 218, 219 Sharvin, D. Yu., 211 Sharvin, Yurii Vasil’evich, 198, 211 Shechtman, Daniel, 28, 234 Shirakawa, Hideki, 234 Shockley, William, 4, 78, 87, 230 Shoenberg, David, 66, 105 Shubnikov, Leo Vasilyevich, 116, 129 Shull, Clifford Glenwood, 231 Siegbahn, Kai Manne, 231 Siegbahn, Manne, 229 Siemens, Werner, 36 Silsbee, Francis Briggs, 120 Simmons, Ralph O., 215 Simon, Franz Eugen, 5, 6

242 Smalley, Richard Errett, 201, 233 Smith, George Elwood, 232 Solvay, Ernest, 40 Sommerfeld, Arnold, 18, 72, 78 Sorby, Henry Clifton, 213 Spenke, Eberhard, 83, 86 Stark, Johannes, 194 Stoddart, J, Fraser, 234 Störmer, Horst Ludwig, 112, 231 Strassmann, Fritz, 152, 219 Szilard, Leo, 219 T Taylor, Sir Geoffrey, 221 Teal, Gordon Kidd, 78 Thomson, George Paget, 230 Thouless, David J., 232 Tomonaga, Sin-itiro, 230 Träuble, Hermann, 131 Tsuei, Chang C., 161, 162 Tsui, Daniel Chee, 112, 231 Tsu, Ray, 190 V van Alphen, Pieter M., 103 van den Berg, G. J., 227 Van Vleck, John Hasbrouck, 231

Author Index Voigt, B., 226 von Ardenne, Manfred, 10 von Borries, Bodo, 9 von Helmholtz, Hermann, 36, 97, 214 von Klitzing, Klaus, 108, 110, 231 von Laue, Max, 1, 18, 19, 43, 123, 229 W Waller, Ivar, 43 Wannier, Gregory Hugh, 194 Watson, James D., 27 Webb, Richard A., 211 Weiss, Pierre, 171, 175, 177, 181 Welker, Heinrich, 78, 90 Wien, Wilhelm, 36 Wigner, Eugene Paul, 3, 4, 112, 136, 219 Wilson, Allan H., 56, 72, 80 Wilson, Kenneth Geddes, 231 Wineland, David J., 232 Winkler, Clemens, 77 Wu, Maw- Kuen, 152 Z Zavaritzkii, Nikolay, 129 Zhang, Shoucheng, 208 Zirnbauer, Martin R., 209

Subject Index

A Abrikosov flux-line lattice, 129, 131 Acceptors, 80 Acoustic modes, 42 Adiabatic demagnetization, 5, 174 Aharonov-Bohm effect, 210, 211 Anderson model, 227 Anomalous Hall effect, 75, 99 Antiferromagnetic spin waves, 182 Antiferromagnetism, 181 Artiﬁcial atoms, 205 Atomei, 8 Atomic force microscopy, 12 Atomic volume, 216 B Ballistic motion, 195 Ballistic phonons, 45, 46 Barkhausen jumps, 178 Base, 86 Batelle institute, 223 BCS theory, 135–137 Bell Laboratories, 78, 88, 112, 141 Bicrystal, 161 Bicrystal technique, 161, 162 Bipolar transistor, 86 Bismuth-telluride, 94 Bitter decoration technique, 131, 178 Bloch ansatz, 51 Bloch frequency, 193 Bloch-Grüneisen law, 66, 67 Bloch oscillation, 192, 193 Bloch wall, 179 Bohr’s magneton, 173 Boltzmann distribution, 75, 94, 171

Bose-Einstein distribution, 38, 62, 180 Bose-Einstein statistics, 40 Bosons, 40, 62 Bragg diffraction law, 22 Bragg reflection, 21, 55, 56, 65, 191, 192 Bravais lattices, 16, 17 Breeder reactor, 219 Bremsstrahlung, 26 Brillouin function, 173 Brillouin zones, 23, 25 Buckminster-fullerene, 201 C Cadmium-selenide, 86 Carbon nanotubes, 202, 203 Cathode ray tube, 73 Cavendish laboratory, 223 Clusius separation column, 70 Coercive ﬁeld, 183, 185 Coherence length, 127, 134, 156 Cold-working, 223 Collector, 86 Colloid chemistry, 206 Color centers, 218 Comet jet-aircraft, 2 Common salt, 218 Compound semiconductors, 78 Conduction band, 74 Cooper pairs, 135, 137, 140, 157, 159 Copper-oxide (CuO2) planes, 155 Covalent bond, 32 Critical current, 120 Critical magnetic ﬁeld, 120, 122 Critical state, 141 Critical temperatures, 119, 122, 155

© Springer Nature Switzerland AG 2019 R. P. Huebener, Conductors, Semiconductors, Superconductors, Undergraduate Lecture Notes in Physics, https://doi.org/10.1007/978-3-030-31420-0

243

244 Crystallographic point groups, 16 Cuprate superconductors, 151, 154 Curie-constant, 172 Curie’s law, 171, 172 Curie temperature, 176, 177 Curie-Weiss law, 176 Cyclotron angular frequency, 101 Cyclotron energy, 101 Cyclotron frequency, 103 Cyclotron mass, 101, 103, 104 D Debye energy, 41, 66 Debye frequency, 39, 41 Debye temperature, 41, 66 Debye-Waller factor, 43, 44 De Haas–van Alphen effect, 101, 103, 105 De Haas–van Alphen oscillations, 104 Density of states, 39, 41, 76, 105–108 Diamagnetism, 103, 170 Diamond, 45 Diffraction of neutrons, 8 Diffraction theory, 20 Diffusion, 217 Diffusive propagation, 196 Dirac delta funktion, 198 Dirac points, 208 Dislocation line, 222 Dislocations, 10, 143, 222 Dispersion relation, 180, 182 DNA double helix, 27, 33, 189 Donors, 79 Doped semiconductors, 79, 80 Drift velocity, 67 Drude-Lorentz model, 59 D-wave symmetry, 158, 161 E Edge dislocations, 222–224 Edge states, 207 Einstein frequency, 38 Electrical insulator, 56 Electron-hole droplets, 81 Electron mean free path, 59 Electron microscope, 9, 11 Electron synchrotrons, 26 Elementary cell, 16 Elementary magnets, 169 Emitter, 86 Energy bands, 53, 57 Energy gap, 57, 136

Subject Index Epitaxial layers, 160 Esaki diode, 191 European Synchrotron Radiation Facility (ESRF), 26, 27 Exchange energy, 175, 178 Exchange integral, 181 Exchange interaction, 175, 228 Exchange processes, 228 Excitons, 81 Exclusion principle, 62 Extreme quantum limit, 113 Extrinsic semiconductors, 79 F Fatigue fracture, 224 Fermi-Dirac statistics, 62 Fermi distribution, 62–64, 197 Fermi energy, 63, 64 Fermi surface, 64, 65, 103 Fermi wave vector, 64 Ferromagnetism, 49, 174, 175 Field-effect transistor, 109, 186 Figure of merit, 96 First Solvay-Conference, 40 Flux creep, 142 Flux flow, 142 Flux-flow resistance, 142, 143 Flux-flow voltage, 142 Flux-line motion, 160 Forbidden energy gap, 56 Fractional quantum hall effect, 112–114 Francis Bitter High-Magnetic-Field Laboratory, 113 Free electrons, 55 Free enthalpy, 214 Frenkel defect, 218 Fullerenes, 200–202 G Galliumarsenide, 78, 90, 112 Gate electrodes, 198, 204 Gate voltage, 109, 187 Generation current, 84 German Bureau of Standards, 120 Germanium, 77, 78 Giant magneto-resistance, 184, 185 Giant thermo-power, 228 Gibbs free energy, 122 Ginzburg-Landau theory, 127, 129 Gliding plane, 220 Grain boundaries, 160, 162

Subject Index Grain-boundary junctions, 166 Granular structure, 157, 160 Graphene, 204, 208 H Half-integer magnetic flux quantum, 161, 163 Half-integer quantum-Hall-effect, 204 Half-integer spin, 169 Hall constant, 99 Hall effect, 98, 99 Heat conductivity, 60 High-frequency ﬁlters, 166 High-temperature superconductors, 124, 153, 225 Hole-doping, 155 Holes, 75, 76 Hooke’s law, 220 Hybrid magnets, 115 Hydrogen bond, 33 Hysteresis, 183 I IBM Research Laboratory, 151 Indium-antimonide, 78 Inelastic neutron scattering, 43 Injection laser, 90 Integer quantum Hall effect, 107, 111 Interference, 20 Intermediate state, 128 Interstitial atom, 217 Intrinsic Josephson junction, 163, 164 Intrinsic semiconductors, 75, 77 Inversion at a point, 16 Ionic bond, 31 Ionic crystals, 218 Iron pnictides, 164, 165 Ishikari Project, 167 Isotope effect, 135 J Josephson effect, 137 Josephson equations, 137 Josephson oscillations, 138, 140 Josephson voltage standard, 146 JR-Maglev project, 147 Junction transistor, 87 K Kapitza Institute for Physics, 129, 198 Kondo effect, 226, 227 Kondo temperature, 228

245 L Landau cylinders, 101, 102, 105 Landau theory, 101 Landé-g-factor, 173 Langevin function, 172 Laplace operator, 50 Large Hadron Collider (LHC), 4, 147 Larmor frequency, 170 Laser scanning microscopes, 11 Lattice vectors, 15 Laue diagram, 22, 23 Laue-Langevin Institute, 43 Law of Dulong and Petit, 35, 41 Layered crystal structure, 155, 159 Lennard-Jones potential, 30 Lenz’ rule, 147, 170 Light Emitting Diode (LED), 89, 90 Liquefaction of helium, 122 Lithography methods, 190 London equation, 125 London penetration depth, 125 Longitudinal phonons, 42 Lorentz force, 98–100, 142 Lower critical magnetic ﬁeld, 130 Low-temperature scanning electron microscopy, 157 M Macroscopic quantum state, 135, 137 Madelung constant, 32 Magic higher fullerenes, 202 Magnesium-diboride, 165 Magnetically levitated train, 147 Magnetic bottle, 100 Magnetic coils, 166 Magnetic domains, 178 Magnetic energy-storage, 148 Magnetic flux line, 130, 134 Magnetic flux quantization, 132 Magnetic flux quantum, 104, 129, 130, 131, 133, 210 Magnetic force microscopes, 13 Magnetic hardness, 183 Magnetic penetration depth, 124, 126, 134 Magnetic Random-Access Memories (MRAM), 186 Magnetic susceptibility, 170 Magnetic tunnel junction, 186 Magnetization, 105, 170, 177, 181 Magneto-caloric effect, 174 Magneto-cardiography, 145

246 Magneto-electronics, 184 Magneto-encephalography, 145, 146 Magneto-resistance, 99, 100 Magnons, 179 Manhattan project, 70 Material fatigue, 10 Mathiessen’s law, 68 Max Planck Institute for Metals Research, 214 Mechanical strength, 220 Mechanical tension, 220 Meissner effect, 120–123, 151, 170 Mercury, 117–119 Mercury-telluride, 207 Mesoscopic regime, 195, 196 Metallic bond, 33 Microcracks, 224, 225 Micromanipulation, 190 Micromechanics, 92 Minibands, 192, 193 Mixed state, 130, 131 Mixing cryostat, 6 Mixing entropy, 215 Modulation doping, 112 Momentum space, 23, 25, 64–66, 158 Mond laboratory, 115 Mössbauer effect, 43 Multiﬁlamentary wires, 147 N National High-Magnetic-Field Laboratory, 115 N-doping, 80 Néel temperature, 182 Negative differential resistance, 194 Neutron diffraction, 28 Neutron stars, 144 N-i-p-i crystals, 194 Nondestructive materials testing, 145, 225 Normal modes, The, 35 Northern lights, 100 N-processes, 45 Nuclear demagnetization, 5 Nuclear fusion process, 148 Nuclear magnetism, 182 Nuclear reactor, 219 Nuclear spin tomography, 147 N. V. Philips’ Gloeilampenfabrieken, 118 O Ohm’s law, 60 Optical modes, 42

Subject Index Optoelectronics, 207 Orbital magnetic moment, 169 P Pancakes, 159 Paramagnetic susceptibility, 174 Paramagnetism, 171 Paramagnetism of the electrons, 64 Pauli exclusion principle, 174 P-doping, 80 Peltier cascade, 95 Peltier cooling, 93–95 Peltier effect, 68, 69, 94 Periodic boundary condition, 76 Periodicity condition, 51 Periodic potential, 50, 51, 55, 56 Perovskite structure, 154 Philips research laboratories, 118 Phonon drag, 71 Phonon focusing, 47 Phonons, 38 Phonon spectrum, 38 Photoelectric effect, 36 Photons, 36 Photovoltaics, 89 Physikalisch-Technische Reichsanstalt, 36, 37 Piezoelectric actuators, 200 p-junction, 161 Pinning centers, 144, 156, 160 Planar technology, 91 Planck’s constant, 36 Planck’s radiation law, 40 P-n junction, 82, 83 Pohl’s circus, 218 Point contacts, 198 Point-contact transistor, 87, 88 Population inversion, 90 Powder technique, 26 Protein crystals, 15 Pulsars, 144 Q Quantized conductance, 199 Quantized unit of the conductance, 198, 200 Quantum cascade laser, 195 Quantum dots, 205 Quantum Hall effect, 109 Quantum-spin-Hall-effect, 207 Quantum statistics, 40 Quantum Statistics, Fermi distribution, 62

Subject Index Quantum triangle, 146 Quasi-crystals, 28 R Radar technology, 66 Radiation damage, 219 Rayleigh-Jeans radiation law, 36 Reading head, 184, 186 Reciprocal lattice, 23–25 Recombination current, 84 Rectiﬁcation, 84 Rectiﬁer characteristic, 86 Rectifying effect, 73 Reflection at a mirror plane, 16 Relaxation time, 60 Residual resistance, 68 Rotating-crystal technique, 26 Rotation, 16 Rowland gratings, 97 S Scanning electron microscope, 10 Scanning tunneling microscope, 11–13 Scattering angle, 67 Schottky contact, 82 Schottky diode, 82 Schrödinger equation, 50, 51 Secondary electrons, 10 Second Moore’s Law, 92 Seebeck coefﬁcient, 71 Seebeck effect, 69 Selenium, 86 Selenium rectiﬁers, 86 Self-ﬁeld, 120 Self-ordered quantum dots, 206 Semiconductors, 57, 73 Shapiro steps, 140 Shielding currents, 123 Shubnikov - de Haas oscillations, 105 Siemens & Halske, 9 Siemens company, 86 Silicon, 7, 8, 77, 78 Silicon wafers, 91 Silsbee’s rule, 120 Single crystals, 78, 220 Single-electron effects, 203 Slippage, 221, 223 Solar cell, 89 Sony, 207 Sound velocity, 42 Speciﬁc heat, 38–41 Speciﬁc heat of the electrons, 63 Speciﬁc heat of the magnons, 181 Spin-exchange interaction, 228

247 Spin magnetic moment, 169 Spintronics, 184 Spin valves, 185 Spin waves, 179 SQUID-on-tip, 145 SQUID-scanning microscope, 145, 162 Structure size, 92 Superconducting electric power cables, 148 Superconducting magnetic coils, 148 Superconducting magnets, 115, 147 Superconducting Quantum Interference Device (SQUID), 144, 145, 161, 166, 225 Superconductivity, 117, 119 Superlattices, 190, 191 Surface states, 208 S-wave symmetry, 158 Symmetry of the wave function, 158 Synchrotron radiation, 26 T Table salt, 31 Thermal conductivity, 44 Thermal diffusion, 70, 71 Thermal force, 71 Thermodynamic potential, 214 Thermoelectricity, 68, 93 Thermoelectric voltage, 71 Thermoelements, 71 Thomas J. Watson Research Center, 161, 190, 196, 211 Thomson relation, 72 Titanic, 225, 226 Topological band theory, 209 Topological insulators, metals, and semimetals, 207, 208 Topologically equivalent, 208 Topological materials, 208 Transistor, 4, 86 Translation symmetry, 15, 16 Transmission channels, 196, 200 Transport entropy, 71 Transverse phonons, 42 Tricrystal experiment, 162, 163 Tunneling experiment, 136 Tunnel junction, 136, 137, 140 Two-dimensional electron gas, 108, 112, 113, 186 Two-level-system, 173 Type-II superconductors, 129, 131 U Umklapp-processes, 44, 45 Undulators, 27 Upper critical magnetic ﬁeld, 131, 156

248 V Vacancies, 214–216 Valence band, 74 Van-der-Waals bond, 29 Vibrational energy, 35, 38 Von-Klitzing-constant, 111 W Wafers, 91 Wall energy, 127, 128 Wannier-Stark ladder, 194 Wave vector, 59, 64, 192 Weiss ﬁeld, 175

Subject Index Wiedemann-Franz law, 61 Wien’s radiation law, 36 Wigglers, 27 Wigner crystal, 112 Woodstock of Physics, 152 X X-ray diffraction, 1, 8, 19, 23, 27, 43 Z Zero-point motion, 47 Zone melting process, 8